0 downloads
0 Views
4MB Size

Charge Transport in Molecular Materials: An Assessment of Computational Methods Harald Oberhofer,*,† Karsten Reuter,† and Jochen Blumberger‡,§ †

Chair for Theoretical Chemistry and Catalysis Research Center, Technische Universität München, Lichtenbergstrasse 4, D-85747 Garching, Germany ‡ Department of Physics and Astronomy, University College London, Gower Street, London WC1E 6BT, United Kingdom § Institute for Advanced Study, Technische Universität München, Lichtenbergstrasse 2 a, D-85748 Garching, Germany ABSTRACT: The booming ﬁeld of molecular electronics has fostered a surge of computational research on electronic properties of organic molecular solids. In particular, with respect to a microscopic understanding of transport and loss mechanisms, theoretical studies assume an ever-increasing role. Owing to the tremendous diversity of organic molecular materials, a great number of computational methods have been put forward to suit every possible charge transport regime, material, and need for accuracy. With this review article we aim at providing a compendium of the available methods, their theoretical foundations, and their ranges of validity. We illustrate these through applications found in the literature. The focus is on methods available for organic molecular crystals, but mention is made wherever techniques are suitable for use in other related materials such as disordered or polymeric systems.

CONTENTS 1. Introduction 2. Theoretical Background 2.1. Charge Carrier Density 2.2. Charge Carrier Mobility 2.3. Transport Regimes 3. Hopping Regime 3.1. Polaronic Rate Theory 3.2. Adiabatic and Nonadiabatic Limits 3.3. Driving Force, ΔG0 3.3.1. On-Site Energies 3.4. Reorganization Free Energy, λ 3.5. Nuclear Tunneling Factor, Γn 3.6. Eﬀective Frequency, νeff 3.7. Electronic Coupling, Hab 3.7.1. Generalized Mulliken−Hush Method 3.7.2. Constrained Density Functional Theory 3.7.3. Fragment Orbital Methods 3.7.4. Frozen Density Embedding 3.7.5. Block Diagonalization of the Electronic Hamiltonian 3.7.6. Analytic Overlap Method 3.7.7. Superexchange Eﬀective Couplings 3.8. Kinetic Monte Carlo Simulation of μ 3.9. Applications 4. Band Transport Regime 4.1. Eﬀective Mass 4.1.1. Tight-Binding Model of Electronic Band Structures 4.2. Relaxation Time 4.3. Applications 5. Intermediate Regime © 2017 American Chemical Society

5.1. Ranges of Validity 5.1.1. Polaronic Hopping Model 5.1.2. Band Theory Model 5.2. Polaronic Band Theories 5.3. Propagation of the Charge-Carrier Wave Function 5.3.1. Mean Field Propagation 5.3.2. Surface Hopping Approaches 5.3.3. Other Propagation Methods 5.3.4. Example: Propagation in a Charge Localized Basis 5.4. The Kubo Formula 5.5. Applications 6. Synopsis, Remaining Challenges, and Future Directions Author Information Corresponding Author ORCID Notes Biographies Acknowledgments References

10319 10321 10321 10321 10322 10323 10323 10325 10326 10326 10327 10328 10328 10328 10329 10329 10330 10332 10332 10333 10334 10334 10335 10335 10336

10339 10339 10340 10340 10341 10341 10342 10344 10344 10345 10346 10346 10347 10347 10347 10347 10347 10348 10348

1. INTRODUCTION Organic molecular solids have attracted much interest in the past two decades in diverse disciplines ranging from the medical sciences to the semiconductor industry. Due to the excessive range of possible molecular constituents, molecular solids can

10337 10337 10338 10339

Received: February 8, 2017 Published: June 23, 2017 10319

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

calculation of material properties often necessitates system sizes beyond the reach of modern computational capabilities. While earlier reviews detailed at great length speciﬁc aspects of simulation methodologye.g., for speciﬁc systems7−14in this work we aim to give a comprehensive overview of theoretical methods that are presently established to tackle these problems and thus enable the computation of charge conduction in molecular solid semiconductors. Diﬀerent methods have been established, depending on the prevailing transport mechanism within the material. One generally distinguishes the three regimes of charge hopping, band transport, and intermediate cases. For each of these regimes we outline the methods put forward to compute the respective parameters from ﬁrst principles, as well as from tight-binding and semiempirical methods. We review their theoretical underpinnings and point out similarities and diﬀerences. We illustrate, where possible, each approach with instructive examples and give an overview of applications of the respective methods found in the literature. Hereby, we mainly focus on ordered organic solids, but we will point out below which of the methods discussed are also applicable to disordered systems like organic polymer blends. Finally, one has to appreciate the importance of accurate structural models as a basis for all of the following atomic-scale simulation techniques. There can be no atomistic simulation of charge-carrier transport without a detailed knowledge of the position of all atoms involved. In the context of ordered organic crystals, especially considering material screening studies, this leads to two distinct approaches. On one hand, structural models can be taken from experimental measurements, collated for example in the Cambridge Structural Database (CSD),15 and used in computational screening studies.16 On the other hand, for systems that have either not yet been synthesized or structurally resolved through experiment, one can attempt to gain structural models from purely theoretical considerations. Such structure prediction approaches, based on either specially parametrized force ﬁelds or electronic structure methods, have shown tremendous progress over recent years as evidenced, e.g., by the crystal structure prediction (CSP) blind test series of publications.17−22 While all CSP methods are based on global geometry optimization techniques,23,24 diﬀerent approaches to resolve the material structure have to be utilized for disordered systems, e.g., polymer blends. There, structures are generally taken as snapshots from high-temperature molecular dynamics (MD) simulations, at present predominantly performed on the level of classical force ﬁelds.25−28 In the following we will concentrate on methodological approaches for the simulation of the charge carrier dynamics given speciﬁc geometries as is appropriate for crystalline molecular solids. A generalization to the application to individual geometry snapshots is conceptually straightforward. In compiling a review such as this one, one quickly realizes that the number of ways in which the problem of conductivity in organic molecular crystals has been approached is quite overwhelming. While it is to some extent possible to show that the multiple deﬁnitions of, say, a basic quantity such as the mobility are all equivalent, the computational as well as experimental methods to determine it are diverse, numerous, and partly beyond comparison.10 There is deﬁnitely no single “best” way to approach this problem. Instead there is a rather complete (and partially even redundant) “toolbox” of methods one has to choose from for each given problem at hand. With the present paper we aim to provide a helpful overview of this

show an exceptional variety of properties. In pharmacology, for instance, for a long time molecular solids have been of great importance due to the fact that most medical drugs are delivered in the form of molecular crystal powders. Thus, the structure, isomorphism, and solubility of the molecular drug components are the main points of interest and are under active research both experimentally and theoretically. Much more recently, though, organic solids have been discovered for use as electronic components, ushering in the advent of the ﬁeld of molecular electronics. With organic molecules as their main component, molecular electronics holds great promise with regard to a favorable economic footprint and novel materials properties.1−6 At present, applications of organic solids are mainly divided into three diﬀerent branches of electronics. The ﬁrst is classical electronics in the form of organic ﬁeld eﬀect transistors (OFETs), which for some applications can replace standard inorganic components based on silicon. The second big ﬁeld of interest is the use of molecular electronics in light harvesting and power conversion applications in the form of organic photovoltaics (OPVs). And last, but not least, is the inverse process, i.e., the emission of light under the action of an electric current. This has been successfully deployed to the market in the form of organic light emitting diodes (OLEDs). Supplementing experiments, computational theory can play a major role in studying, understanding, and exploring new organic molecular compounds in all these application ﬁelds. Theoretical approaches can thereby broadly be classiﬁed as follows: 1. Material optimization: The objective is to determine in detail the mechanisms at play in order to identify eﬃciencylimiting loss processes. On the basis of a thorough understanding of a material, one can try to eliminate losses through modiﬁcations of the material at hand. 2. Materials screening: Given the availability of a good descriptor, which correlates well with the desired property of the material, the objective is to screen diﬀerent materials for their suitability in a certain application. Considering that the space of possible molecular compounds is many orders of magnitude larger than the range of organic solids hitherto characterized, this often requires an additional crystal structure prediction stepwhich remains a major challenge to this day. Both kinds of approaches rely to varying degrees on a suﬃciently accurate theoretical description of the underlying atomic-scale processes involved in the desired property. Yet, simultaneously they have to be able to yield experimentally accessible observables to be of practical use. An important ﬁgure of merit in all three electronic applications of organic solidsOFETs, OPVs, and OLEDs is the electric conductivity σ. Simplistically, it is deﬁned in terms of Ohm’s classic law

I = σV

(1)

where I is the current and V is the applied voltage. Any predictive-quality theoretical approach needs to determine σ (or indeed at least any of its constituent parameters as outlined below) as a function of the microscopic structure and dynamics of the molecular solid. In doing so one is generally confronted with severe challenges. Among these, notably the nature of charge carriers and their transport mechanism still remain unclear in many molecular materials. Furthermore, a correct description of the structure and thermal ﬂuctuations of the molecules requires accurate molecular models, while the 10320

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

toolbox, which aids readers with choosing the theoretical approach best suited to their respective needs.

2. THEORETICAL BACKGROUND Regardless of the underlying mechanism of charge transport, the conductivity of any material σ̲which in general is a tensor of rank 2is generally determined by the density ρc of mobile charge carriers and their mobility μ̲ σ̲ = qρc μ̲ (2) where q denotes the charge of the carrier. The detailed transport mechanism enters then through the diﬀerent dependences of ρc and μ̲ on elementary parameters such as temperature or doping. A thorough computational assessment of charge transport properties of a molecular material thus has to include an estimate of both parameters. Concerning notation: throughout this review we use bold letters r to denote vectors and bold underlined letters σ̲ represent second rank (3 × 3) tensors, where columns and lines enumerate the three spatial coordinates. Letters in blackboard bold , ﬁnally, denote second rank tensors of higher dimensionality, i.e., basis set expanded matrices of operators.

Figure 1. Sketch of eﬀect of ﬁnite temperatures on distribution of occupied electronic states. Shown are representative densities of states for both spin-up (blue line) and spin-down electrons (red line) for an artiﬁcial system with a band gap of ≈0.2 eV. At nonzero temperatures thermal excitation described by the Fermi distribution (black line) can lead to the appearance of occupied states above and unoccupied states below the Fermi level.

Extrinsic contributions to the carrier density, on the other hand, are not necessarily as straightforward to include in a computational model. Without explicitly accounting for the dopant or defect electronic levels, a minimalistic description is simply through a change of the Fermi level position. Depending on the sign of the change, this then results in a higher electron or electron−hole carrier density as described by eqs 3a−3c and schematically illustrated in Figure 1.

2.1. Charge Carrier Density

In the absence of optical excitations, the density of mobile charge carriers in a solid can essentially be separated into two contributions: ρc = ρin + ρex. First, the so-called intrinsic carrier density ρin originates from the thermally excited states of the band structure of the ideal material, and second, ρex is the density of mobile carriers due to extrinsic defects in the periodic structure of the material. The latter include all kinds of nonperiodicities, ranging from point defects such as vacant lattice sites (due to a missing molecule) or interstitial molecules (e.g., solvent molecules left over from the crystallization process), to larger higher-dimensional defects such as interfaces with another material.29 Additionally, doping with atoms30,31 or molecules32,33 with diﬀering electronic energy level alignment contributes to the extrinsic density of charge carriers. From a computational point of view the density of intrinsically mobile charge carriers can simply be determined from the ideal system’s Fermi level, εF, and electronic density of states (DOS), ρ(ε). The latter is a measure of the states existing in the system at a given energy ε, while the former is deﬁned as the chemical potential of electrons in the solid. The densities of mobile electrons ρein in the conduction band and electron− holes ρhin in the valence band are given by34 ρine =

∫ε

The charge mobility μ̲ is deﬁned as the velocity response of a charge carrier to an external electric ﬁeld35,36 μij =

d ε ρ (ε) f ( ε ; T )

(3a)

εF

∫−∞ dε ρ(ε) [1 − f (ε; T )]

(3b)

where f (ε ; T ) =

1 e(ε − εF)/ kBT + 1

⟨v⟩i Ej

(4)

where ⟨v⟩i denotes the ith component of the time-averaged velocity ⟨v⟩ of the carrier and Ej is a component of the electric ﬁeld vector E. In condensed systems, both ⟨v⟩ and E generally need to be explicitly described as three-dimensional vectors, which thus yields a (3 × 3) tensorial mobility μ̲. Only in isotropic media, such as liquids or fully disordered solids, the velocity response can be isotropic as well. If additionally the carrier velocity response in any direction i is independent of the applied ﬁeld in all directions but i, the mobility can be reduced ⟨v⟩ to a simple scalar quantity μ = E , involving the magnitudes ⟨v⟩ = ∥⟨v⟩∥ and E = ∥E∥. Note that the average velocity is not generally a linear function of the ﬁeld. This means in turn that the mobility as deﬁned by eq 4 is typically a function of the applied electric ﬁeld. As discussed in more detail in sections 3−5, the mobility can in fact vary strongly with E. Given inaccuracies in both experimental and theoretical studies of the mobility, this can further complicate a direct comparison. For such a comparison it is therefore often useful to linearize ⟨v⟩ with respect to the ﬁeld37

∞

F

ρinh =

2.2. Charge Carrier Mobility

(3c)

is the Fermi−Dirac distribution function for Fermionic (quasi‑) particles such as electrons and holes. Here, T denotes the temperature and kB is Boltzmann’s constant. A sketch outlining the thermal eﬀects on the availability of mobile charge carriers is given in Figure 1.

μij =

⟨v⟩i ∂⟨v⟩i 1 ∂⟨v⟩i ≈ Ej = Ej Ej ∂Ej ∂Ej

(5)

Note that both deﬁnitions of μ̲, eqs 4 and 5, remain ﬁnite even for vanishing ﬁeld, since as Ej → 0 so does the average drift 10321

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

matrix, it is often instructive to transform D̲ into the diagonal principal axis representation. This is always possible because the diﬀusion tensor is by deﬁnition positive deﬁnite and symmetric. In the low-ﬁeld regime these diagonal components of the diﬀusion tensor can be expressed as the product of mean free 37 path l and the thermal velocity of the carrier particle vth i

velocity. Yet, for numerical reasons it can be advantageous to employ eq 5 in low-ﬁeld regimes (vide infra).38 Experimentally, the charge carrier mobility is accessed by obtaining the response of the carrier drift velocity to an external electric ﬁeld. Arguably the most direct method to measure bulk mobility is thereby the time-of-ﬂight (TOF) technique39−43 introduced already in the late 1960s.44 In this method the transit time τtr of a charge carrier through a solid is measured by analyzing the transient behavior of the current as the electric ﬁeld is switched on. For the one-dimensional case, the mobility is then simply given as μ = L/(τtrE), where L is the extension of the solid.45 There are, of course many more experimental approaches available to measure carrier mobilities, each diﬀering in experimental setup as well as accessible charge transport regime.46 Next to TOF measurements other, partly even more prominent, examples are the measurement of the Hall eﬀect mobility,47,48 the analysis of ﬁeld eﬀect transistors,49 the family of space charge limited current techniques,50 time-resolved microwave conductivity measurements,51 and ﬁnally the method of charge extraction with a linearly increasing voltage.52,53 An in-depth review of these techniques is beyond the scope of this review, but exhaustive discussions can be found, e.g., in a review by Tiwari and Greenham,46 a review by Coropceanu et al.,10 or a paper by Shuttle and co-workers.49 Finally, an important connection between the general concept of a charge carrier mobility of eq 4 and classical kinetic theory is given by the Einstein−Smoluchowski (ES) equation

μijES =

Dii = livith

To illustrate the connection between the Einstein mobility and eqs 4 and 5, we depict in Figure 2 the resulting mobilities

Figure 2. Comparison of deﬁnitions of charge carrier mobility for a one-dimensional Marcus hopping model (vth = lk with k ∝ ∥Hab∥2 exp(−(λ − qEd)2/4λkBT), cf. section 3 for a full deﬁnition) for parameters Hab = 50 meV and λ = 150 meV, representative for many organic solids. The Einstein mobility plot is based on eqs 6 and 10, where the latter holds in the case of vanishing ﬁelds. Compared to the full mobility expression (eq 4) and the linearized expression (eq 5), this is clearly not valid for higher ﬁeld strengths.

Dij(E)q kBT

(6)

as a function of the external ﬁeld for a simple one-dimensional hopping model (vth = lk, with k the hopping rate, vide infra). Note that the equality of all three deﬁnitions for E → 0 is here indeed not a coincidence, but rather is an exact property of the employed hopping model. In general, such a perfect coincidence is not guaranteed, though, for all regimes of condensed-phase charge transport. As such the choice of mobility deﬁnition has to be treated with care and possibly be adapted to speciﬁc experimental references. Thereby the full or linearized deﬁnitions are most often used in the context of the TOF technique41,42 and the Einstein expression most strongly associated with, e.g., ﬁeld eﬀect transistor measurements.46,49 Of the two ﬁeld-dependent deﬁnitions, eqs 4 and 5, one can expect the linearized version to perform better in numerical simulations at very low ﬁelds due to the E−1 term appearing in the general mobility deﬁnition.

which relates the mobility of a charged particle to itsgenerally ﬁeld dependent and anisotropicdiﬀusion coeﬃcient D̲ and the thermal energy kBT. In principle, this is an exact classical connection based on a statistical treatment of the carrier particle’s random walk through the medium.54 Possible approximations occur in estimating D̲ , e.g., based on the underlying charge transport mechanism (see below). The deﬁnition of the elements Dij of the diﬀusion tensor in anisotropic media follows from a generalization of Fick’s law55,56 ∞

Dij =

∫t =0 dt ⟨vi(t ) vj(0)⟩

(7)

where vi(t) is the ith component of the particle velocity vector v at time t. Equation 7 is the anisotropic generalization of the well-known Green−Kubo equation for isotropic media54 D=

1 n

2.3. Transport Regimes

∞

∫t =0 dt ⟨v(t )·v(0)⟩

While the deﬁnition of charge carrier mobility given in eq 4 is general, the computational approaches to determine it vary depending on the transport mechanism prevailing in the material under consideration. In terms of this mechanism three regimes are typically discussed, which diﬀer in the degree of the carrier localization. Phrased diﬀerently, there are in fact two opposite limiting regimes (localized hopping vs itinerant band transport) and an intermediate regime featuring intermediate characteristics of both limits. In the limit of polaronic or hopping transport, localized charge carriers move through the material by hopping from one site to the other, where the microscopic meaning of “site” will be further speciﬁed below. This regime applies if such localized charge carriers exist and if there is an activation barrier

(8)

where n is the spatial dimensionality. In the long time limit it reduces to the familiar deﬁnition of the diﬀusion constant as the time derivative of the mean square displacement (MSD) of the charge carrier57 D=

dMSD(t ) 1 lim dt 2n t →∞

(10)

(9)

Note that this isotropic case is given here only for comparison. It rarely applies to molecular crystals due to the diﬀerent relative orientations of the molecules along the crystallographic axes. Yet, instead of the full (3 × 3) diﬀusion 10322

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

between the discrete sites a and b. As detailed below, these rates depend on the speciﬁc relative orbital geometries of initial and ﬁnal sites and are thus in general highly site speciﬁc and directionally dependent. The average drift velocity can be written as a sum over all possible site-to-site hopping rates times the respective distance vectors. For the ith component ⟨v⟩i of an ideal solid composed only of sites of one equivalent type, this yields ⟨v⟩i = ∑ab kabdab,i, where the sum enumerates all possible combinations of initial site a and ﬁnal site b, and dab denotes the center-of-charge distance vector between the sites. In general, the speciﬁc rates also show a dependence on the applied external ﬁeld, which together with eq 4 yields the following expression for the hopping mobility.37,63

separating the localization sites. This is generally the case either in weakly coupled organic crystals or in disordered solids such as polymer melts. Within the hopping regime there are a number of analytical expressions to calculate the mobility, for instance based on rate theories. A variety of computational approaches aim at providing the parameters entering these expressions, and we will survey these approaches in section 3. Band transport is the opposite limiting regime in terms of carrier localization. Here, carriers exist fully delocalized at the (valence or conduction) band edges. They propagate with an eﬀective mass corresponding to the inverse of the band curvature and thus to the coupling between crystal sites. Propagation is limited through impurities and collisions with phonons. This regime generally applies for ultrapure organic crystals with large electronic coupling between sites. In this case the mobility can also be calculated from analytical expressions with parameters accessible for instance through ab initio calculations. The theory and computational approaches geared to conduct band mobility calculations will be outlined in section 4. Experimentally, one can distinguish between these two classic regimes by observing the mobility as a function of temperature. An experimentally determined increase of the mobility with temperature T is usually assigned to activated hopping, whereas a decrease often points to band transport due to increased electron−phonon interactions. Unfortunately, carrier transport in organic molecular crystals does often not adhere exactly to one or the other regime, but instead may follow a mixture of both. For this intermediate regime no simple analytical approach to calculate the mobility exists to date. Rather, one has to explicitly follow the dynamics of the carrier migration through the system to simulate the mobility directly. The state of the art of such approaches is discussed in detail in section 5. To avoid any confusion, the discussion in all subsequent sections will thereby concentrate on the full deﬁnition of μ̲ as given in eq 4.

μij =

∑ dab ,i ab

kab Ej

(11)

Note that expression 11 applies only to perfectly ordered crystals where all sites are equivalent. In the presence of defects or even in the mere case of ideal crystals with multiple inequivalent sites per unit cell, the intricate interplay between diﬀerent hopping rates and sites can no longer be easily described analytically. Instead, the reaction network deﬁned by pairs of localization sites and their hopping rates needs to be solved numerically, for instance through a kinetic Monte Carlo algorithm as described in section 3.8. In either case, the critical microscopic parameters required to determine the mobility are, next to the crystal structure (which provides the site pairs and distance vectors), the charge transfer rates kab. In the following we describe various rate theory approaches that have been put forward for the calculation of these charge transfer rates, as well as for the calculation of the quantities that arise within the corresponding rate theory expressions. 3.1. Polaronic Rate Theory

Polaronic rate theories have been applied to a multitude of condensed matter systems. The main argument underlying these theories is that, in order to obey energy conservation in a closed system, the charge transfer itself (the fast mode of the system) can only occur at a transition state (TS) at which the nuclear conﬁgurations (the slow mode) of initial and ﬁnal polaronic states are energetically degenerate. For a charge transfer to occur, the system must therefore overcome a barrier which physically arises from the polarization of the surrounding medium to a given charge stateat least partially, as will be discussed later. Assuming a harmonic response, one can visualize this process in the form of two parabolas as depicted in Figure 3. Each parabola describes the variation of the free energy upon changes of the nuclear degrees of freedom along a suitable reaction coordinate, while simultaneously constraining the electronic state of the system to the one at the minimum of the parabola. Each parabola thus represents a so-called diabatic state of the system: one for the initial state with the charge at site a and one for the ﬁnal state with the charge at site b. Figure 3 then deﬁnes three important energetic quantities: ﬁrst, the driving force ΔG0 between initial polaronic state a and ﬁnal polaronic state b at their respective minima of the reaction coordinate; second, the diabatic activation energy ΔG‡ necessary to move the system from the initial polaronic state a to the TS; third, the reorganization free energy λ which describes the energy cost to bring the nuclear conﬁguration of the polaronic state b into that of state a while keeping the electronic conﬁguration ﬁxed at state b. All free energies are

3. HOPPING REGIME Hopping transport models assume that the charge carrier is localized on a site in the solid and moves from one site to another by a series of discrete jumps. Depending on the degree of localization, a site in an organic molecular solid can thereby be a single molecular unit, a part of a larger molecule or polymer, or a discrete collection of molecules. The localization can in general be induced by three distinct mechanisms. Small polaron theory predicts a localization of the charge carrier due to its interaction with the medium. The charge induces a local nuclear distortion of a molecular site and the surrounding medium which, in turn, stabilizes the localized charge. The quasi-particle of charge carrier and lattice distortion thus formed is called a small polaron. Recently, another theory for the occurrence of localized carriers has been put forward by Troisi and co-workers,58,59 based on the seminal work by Su, Schrieﬀer, and Heeger,60 as well as work by Hannewald and coworkers.61 In this theory localization is induced by thermal ﬂuctuations of the coupling between sites (so-called nonlocal electron−phonon coupling). Finally, in less ordered systems, charges can also localize simply through the static disorder of the underlying structure,62 which, e.g., breaks conjugation in organic polymer systems. Regardless of the underlying localization mechanism, hopping models describe the charge transfer (CT) through the discrete carrier jumps in terms of charge transfer rates kab 10323

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

overall lower eﬀective free energy barrier and thus an enhanced total transition rate (Γn ≥ 1). Yet, these enhancements generally only play a role at low temperatures due to the large masses of the nuclei involved in the polaronic reorganization (cf. section 3.6).81 In most studies, the nuclear enhancement factor is therefore set to 1 from the outset. With the exception of Γn, all of the quantities entering eq 13 can be expressed in terms of semiclassical Landau−Zener (LZ) theory.83−85 For the electronic transmission coeﬃcient this leads to

Figure 3. Schematic of a two-state polaronic charge transfer model, where the reaction coordinate is a collective variable of all nuclear coordinates R. Initial and ﬁnal electronic states are described by free energy curves Ga(R) and Gb(R), respectively. Both curves meet at the transition state marked “TS”. The curves have minima at the reaction coordinates Ra and Rb which are, in general, energetically separated by ΔG0 = Gb(Rb) − Ga(Ra). For further details see text.

⎧ 2PLZ if ΔG† ≥ −λ ⎪ P + 1 LZ κel = ⎨ ⎪ † ⎩ 2PLZ(1 − PLZ) if ΔG < −λ

where PLZ is the LZ transition probability for a single crossing of the transition region along the reaction coordinate. It is given by

thereby dynamical averages over all nuclear degrees of freedom except the reaction coordinate. The actual choice of reaction coordinate is thereby far from arbitrary. It has long been known64 that a poorly chosen reaction coordinate can lead to an erroneous description of the reaction pathway or, at least, in the case of a dynamical sampling of the process, a bad convergence of sampled quantities.65 In the case of charge carrier hopping, where the reaction coordinate has to be a collective variable describing relaxation of the surrounding medium to changes in a local charge state, Mones and co-workers66,67 recently quantiﬁed the importance of using a good reaction coordinate to avoid hysteresis and slow convergence. Fortunately, this problem had already been addressed in the early 1980s by the pioneering works of Zusman68 and Warshel,69 who proposed to use a coordinate based on the energy gap ΔE between diabatic states. In a given nuclear geometry R it is deﬁned as ΔE(R) = Eb(R) − Ea(R)

PLZ = 1 − e−2πγ

2πγ =

where Ea,b(R) denote the total energies of the initial and ﬁnal diabatic states, respectively. It is therefore a measure for the preference of the charge carrier to localize in either state for any given coordinate and thus depends crucially on the conﬁguration of the dielectric surroundings. Since its inception the energy gap coordinate has shown its feasibility numerous times in both classical 70−74 and quantum mechanical simulations75−78 of charge carrier transport, and yields results that compare well also to experimental results.79,80 In the harmonic approximation, the semiclassical transition state theory (TST) expression for the charge transfer rate reads7,35,81,82 ‡

(15b)

π 3/2⟨|Hab|2 ⟩TS hνeff λkBT

(15c)

Here, h is Planck’s constant and Hab = ⟨Ψa|Ĥ |Ψb⟩TS is the Hamiltonian transition matrix element (or electronic coupling) between initial and ﬁnal diabatic electronic states at the TS. The angular brackets ⟨ ⟩TS thereby denote an equivalent dynamical averaging over all nuclear conﬁgurations of the TS as done for the free energy expressions. This given form of the transition probability, and speciﬁcally eq 15c, is only valid in the harmonic (linear response) regime with identical polarization responses for initial and ﬁnal states, i.e., identical curvatures of both parabolas in Figure 3. Equivalent expressions can be obtained for the general case of diﬀerent (harmonic) polarization responses.81,83,85 Within this LZ theory, Spencer et al.86 showed the two contributions to the activation energy to be

(12)

ΔG‡ =

(λ + ΔG 0)2 4λ 1/2

Δ‡ = ⟨|Hab|2 ⟩TS

−

(16a)

1 ⟨|Hab|2 ⟩a λ

(16b) ‡

where for the adiabatic correction factor (Δ ) they assumed a vanishing driving force ΔG0. The ﬁrst term of eq 16b thereby corresponds to the diﬀerence between adiabatic and diabatic free energy surfaces, averaged at the TS. The second term is the equivalent free energy diﬀerence averaged at the initial adiabatic state a of the charge transfer. Note that earlier work14,37,38,87,88 employed a diﬀerent approximation for this nonadiabatic correction factor, assuming that initial diabatic and adiabatic free energy minima coincide at the same reaction coordinate. Spencer et al. recently pointed out86 that this approximation is not necessarily always justiﬁed and indeed leads to a diﬀerent criterion on Hab and λ for the validity of the TST approach (see section 3.2). As is apparent from eqs 11−16b, the charge mobility within the hopping model is fully determined through the quantities νeff, λ, Γn, Hab, and ΔG0. In the case of suﬃciently weak external ﬁelds which do not signiﬁcantly distort the frontier orbitals of the molecules mediating the charge transfer, to a good approximation only ΔG0 depends on E. This means that all

‡

kab ,TST = νeff κel Γne−β(ΔG −Δ )

(15a)

(13)

with β = 1/kBT. The activation energy is hereby given as (14) ΔG† = ΔG‡ − Δ‡ That is, the diabatic activation energy is reduced by an adiabatic correction factor Δ‡ that accounts for a ﬁnite electronic coupling between the initial state a and ﬁnal state b. The three contributions to the prefactor in eq 13 are the eﬀective vibrational frequency νeff along the reorganization reaction coordinate, the electronic transmission coeﬃcient κel which accounts for a possibly less than perfect transmission of the charge once the TS has been reached, and the nuclear tunneling factor Γn. The last is a correction accounting for quantum eﬀects of the nuclear degrees of freedom which can lead to an 10324

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

other quantities can be estimated in a ﬁeld-free approach. The most common computational techniques to determine all ﬁve parameters will be discussed in sections 3.3−3.7.

the activation energy is much smaller than the activation energy (Δ‡ ≪ ΔG‡) since in most nonadiabatic cases then, according to the deﬁnition of γ, eq 15c, the electronic coupling is much smaller than the reorganization free energy (λ ≫ Hab).86 This ﬁnally means that (λ + ΔG0) ≫ ⟨|Hab|2⟩TS1/2, and thus the full semiclassical LZ rate equation reduces to35 ‡ 2π 1 kab ,nadiab = ⟨|Hab|2 ⟩TS e−β ΔG Γn ℏ 4πλkBT (18)

3.2. Adiabatic and Nonadiabatic Limits

In order to appreciate the actual transport mechanism underlying hopping models in general, it is instructive to consider the adiabatic and nonadiabatic limits of the presented TST rate expression in the semiclassical LZ formulation; cf. eqs 13−16b. Note that adiabatic and nonadiabatic here are taken to describe respective physical processes. To avoid confusion, the label “diabatic” is only applied to charge-separated states which are not eigenfunctions of the Hamiltonian. Physically, in the adiabatic limit the electronic wave function of the charge carrier changes slowly and gradually (“adiabatically”) from the initial to the ﬁnal charge localized states as the system crosses the activation barrier.35,37,38 This is the case for large electronic couplings, small reorganization energy, and small nuclear velocity along the reaction coordinate. In the opposite, nonadiabatic limit, the electronic wave function changes almost instantly at the barrier top. This is the case for small couplings, large reorganization energies, and large velocities along the reaction coordinate.86 In terms of the LZ parameters, the two limits thus correspond to diﬀerent ratios of Hab to λ, and therewith to diﬀerent adiabaticity factors 2πγ; cf. eq 15c. Examining ﬁrst the adiabatic limit, we assume a large coupling between initial and ﬁnal electronic states on the order of the reorganization energy (and compared to the eﬀective frequency). This leads to an adiabaticity factor 2πγ ≫ 1. In this case the LZ probability PLZ approaches unity, cf. eq 15b, which eﬀectively means that every time the system crosses the TS region it will end up in the other charge state. Consequently, in this limit the electronic transmission coeﬃcient κel approaches unity, which reduces the semiclassical TST expression, eq 13, to a standard Arrhenius form35,86 ‡

This is the celebrated Marcus rate equation.89,90 In this limit, the rate does not depend on the eﬀective frequency νeff anymore, but is instead fully determined through λ, Hab, and ΔG0. In this limit the free energy curve of the process is thus indeed best described in terms of the two diabatic parabolas depicted in Figure 3. Also note that in this limit it is common to summarize all λ-dependent terms into the so-called Franck− Condon factor35 ‡ 1 -= e−β ΔG 4πλkBT (19) Even though it is appealing in terms of the physical interpretation of the charge transfer mechanism, it is generally dangerous to directly employ the rate expressions for the adiabatic and nonadiabatic limits, eqs 17 and 18, respectively, in a hopping model study. This uncertainty has recently been pointed out by Gajdos et al.,38 who computed LZ electronic coupling elements and reorganization free energies for the frequently used electron acceptor phenyl-C61-butyric acid methyl ester (PCBM). Depending on the crystal orientation, they obtained Hab values between a few millielectronvolts and >100 meV as illustrated in Figure 5. In contrast, λ was shown to

‡

kab ,adiab = νeff e−β(ΔG −Δ )Γn

(17)

In the adiabatic limit, the prefactor thus only depends on the eﬀective vibrational frequency along the reaction coordinate. Besides this, the only dependence of the rate on the electronic coupling is then via the adiabaticity correction Δ‡, which eﬀectively lowers the free energy barrier of the reaction as indicated in Figure 4. In the opposite, nonadiabatic limit 2πγ ≪ 1, the exponential in the LZ probability, eq 15b, can be expanded in a Taylor series, which, if truncated after the ﬁrst order, yields PLZ ≈ 2πγ. In this case the probability for a charge to cross from one parabola to the otherwhich is proportional to the electronic couplingis very low. In this limit, the adiabatic correction to

Figure 5. (left) Schematic representation of the electron acceptor phenyl-C61-butyric acid methyl ester (PCBM) in the bcc crystal structure. High and low coupling directions along [111] and [100] are indicated by blue and red boxes, respectively. (right) Donor/acceptor molecule pairs, depicting in orange/silver the donor and in red/blue the acceptor orbitals along these directions, respectively. Data taken from ref 38.

be more or less constant at ∼140 meV, which results in room temperature nonadiabaticity factors 10−4 meV/hνeff ≤ 2πγ ≤ 2 meV/hνeff even within this one system. Another important question that appears in this context concerns the validity of the hopping model itself. The initial assumption in this respect was that the excess charge (electron or hole) is localized as a small polaron on a single site. In the semiclassical LZ formulation this is the case if the activation energy for charge transfer, ΔG† = ΔG‡ − Δ‡, is positive, i.e., if a ﬁnite barrier exists at all. Conditions for the existence of a

Figure 4. Schematic of adiabatic potential energy surfaces (solid lines) for a two-state charge transfer compared to the respective diabatic picture (dashed lines). 10325

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

barrier ΔG† > 0 can be estimated by inserting eqs 16a and 16b into the deﬁnition of the activation energy, eq 14. For a vanishing driving force ΔG0 = 0 and under the assumption that the mean square coupling elements averaged in the TS and the initial state agree, ⟨|Hab|2⟩ = ⟨|Hab|2⟩TS = ⟨|Hab|2⟩a, the barrier height is then given by a simple quadratic equation86 in ⟨| Hab|2⟩1/2: ΔG†(ΔG 0 = 0) =

⟨|Hab|2 ⟩ λ − ⟨|Hab|2 ⟩1/2 + λ 4

moving in a homogeneous external ﬁeld E between sites a and b along the vector dab, it generally reads91 ΔG 0 = Ga(R a) − Gb(R b) + q E·dab

(21)

where Ga and Gb are the so-called on-site free energies of the state with the charge at sites a and b, respectively, while Ra and Rb are the corresponding equilibrium nuclear conﬁgurations (cf. Figure 4). Equation 21 thereby rests on the assumption that the external electric ﬁeld is weak enoughdepending on molecular polarizability and orientationnot to perturb the molecular electronic structure. This means that only the third term in eq 21 depends on the external ﬁeld and the contributions Ga,b also called the on-site energiescan be estimated from ﬁeldfree simulations. They do, however, depend on the dielectric response of the entire environment of the two sites a and b involved and therefore an accurate description of both diabatic states in the extended system. In general, Ga,b are therefore estimated directly from simulations of either state using for example a constrained electronic structure approach92 (cf. section 3.7.2) or suﬃciently accurate classical force ﬁelds.93 A more detailed description of the calculation of site energies is given in section 3.3.1. In homomolecular crystalline systems the environmental contribution is canceled by the symmetric equivalence of initial and ﬁnal states, though. This leaves only the contribution due to the external electric ﬁeld. In this case the driving force simpliﬁes to

(20)

Hence, the activation barrier between the initial minimum and the ﬁnal minimum vanishes at ⟨|Hab|2⟩1/2 = λ/2 to yield one single delocalized state. Furthermore, while eq 20 seems to suggest a reemergence of a barrier for values of ⟨|Hab|2⟩1/2 > λ/ 2, the corresponding minima would lie in the complex plane of the reaction coordinate, thus not describing physically relevant states. This has the eﬀect that for such values of ⟨|Hab|2⟩1/2 the shared minimum stays at a value of the reaction coordinate ΔE = 0 and gets deeper the larger the coupling.14,86 This situation is illustrated in Figure 6, where we plot the adiabatic potential energy surface of a PCBM dimer (λ = 140 meV) for a range of diﬀerent coupling values.

ΔG 0 = qE·dab

(22)

which can be calculated analytically for any site-to-site vector dab. 3.3.1. On-Site Energies. As discussed above, the on-site contributions Ga(Ra) and Gb(Rb) cancel each other out in perfect homomolecular crystals. In disordered systems or crystals with inequivalent sites, on the other hand, they have to be determined explicitly. Furthermore, as will be discussed in sections 4.1.1 and 5, other approaches to CT modeling depend on absolute values of the respective on-site contributions instead of just pairwise diﬀerences. On-site free energies are a local property94 in that they depend on the charge being localized on a single site in the crystal, yet they also include the polarization response of the surroundings.91 For a computational study, this means that to determine Ga,b(Ra,b), or neglecting entropic contributions, the on-site energies Ea,b(Ra,b), one needs to be able to construct the diabatic states a and b and to determine their energy in an extended system. Considering the inherent inability of, e.g., density functional theory (DFT) studies to accurately treat charge-localized states, especially in extended systems,95 on-site energies are not amenable to direct treatment by DFT. Instead, a number of approximate methods have been put forward to tackle this problem. For example, Brédas et al.96,97 and Fuchs and co-workers91 ﬁrst determined the charge distributions of single molecules on the level of hybrid level DFT. This charge distribution is then inserted into a polarizable but classical model of the periodic crystal to determine the energy of a given localized state a or b. A similar combined quantum mechanical/ molecular mechanical approach was followed by Norton and Brédas,98 yet based on the ONIOM method where the classical force ﬁeld energy is corrected by quantum mechanical corrections for the central molecule. In an analogous approach, Friederich et al.99 embedded a DFT inner region into a DFT

Figure 6. Adiabatic free energy proﬁles for a PCBM dimer (λ = 140 meV) for diﬀerent square averaged coupling values ⟨|Hab|2⟩1/2, here for simplicity abbreviated as Hab. Curves were calculated with eq 10 of ref 14. Note the disappearance of a dividing barrier between minima a and b for Hab ≥ 70 meV = λ/2.

As mentioned above, earlier studies applied diﬀerent approximations37,38,87,88 to the estimation of the adiabatic correction factor, thus yielding diﬀerent estimatese.g.,14 ⟨| Hab|2⟩1/2 < 3λ/8 for the existence of separate initial and ﬁnal states. This condition disagrees with the transition from doubleto single-well potential, as illustrated in Figure 6. Instead the approximation given in eq 16b should be used. Finally, returning to the example of PCBM, the λ/2 condition yields an upper bound of ⟨|Hab2|⟩1/2 ≤ 70 meV for the existence of an activation barrier and thus the validity of the hopping model. Yet, in all common PCBM crystal structures there exist nearest-neighbor pairs of molecules for which the couplings are of this order of magnitude or even higher.38 For the computational search for high mobility organic electronic materials, this underscores that hopping models, although convenient and relatively cheap to parametrize from ﬁrst principles, have to be applied with caution. 3.3. Driving Force, ΔG0

The driving force is the diﬀerence in free energy between the fully relaxed initial and ﬁnal states, i.e., the minima of the two diabatic surfaces in Figures 3 and 4. For a carrier of charge q 10326

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

tight-binding exterior for the determination of on-site energetic disorder. A quantum chemical approach based on a combination of the valence bond model and Hartree−Fock calculations100 was also shown to not only yield accurate results for on-site energies,101 but also to reproduce their temperature variations due to crystal lattice vibrations.94 In a more approximate approach geared toward on-the-ﬂy determination of charge transfer parameters in a direct charge propagation model (see section 5.3.4), Spencer et al.86,93 determined on-site energies purely from classical force ﬁeld calculations. Finally, Nagata102 pioneered the use of a ﬁtted charge response kernel103 to determine on-site energy disorder in amorphous tris(8-hydroxyquinolinato)aluminum. For the same system Kwiatkowski et al.104 demonstrated a particularly simple approximation to diﬀerences of site energies. They showed that approximating Gb(Rb) − Ga(Ra) as the diﬀerence of the eigenvalues of the involved frontier orbitals yields a distribution consistent with a Gaussian model of site energies. Introduced by Bässler already in 1981,105 the latter simply assumes a Gaussian distribution of site energies, based on the observation that absorption spectra in disordered organic solids are of Gaussian shapes with roughly similar widths.106

acceptor. It is given by110 λin = Gb(Ra) − Ga(Ra), where Ga and Gb are the free energies of the state with the charge at sites a and b, respectively, while Ra and Rb are the corresponding equilibrium nuclear conﬁgurations (cf. Figure 4). Given an electronic structure method that can give an estimate of these diabatic state energies Ga and Gb, e.g., the constrained density functional theory method described in section 3.7.2, λin is straightforward to calculate. Yet, it generally involves an appropriate averaging over all nuclear degrees of freedom, for instance, through MD simulations.92 Otherwise, the standard way to approximate the inner-sphere reorganization free energy contribution is through the so-called four-point scheme, where the system is separated into donor and acceptor fragments (representing sites a and b). Denoting by ECtot and ENtot the total energies of charged and neutral donor and acceptor fragments, respectively, and by RC and RN the equilibrium geometries adopted by the charged and neutral fragments, the scheme reads

3.4. Reorganization Free Energy, λ

Observing again that the reorganization free energy is due to the change in nuclear coordinates Ra → Rb upon transfer of the charge from site a to site b, another way to determine the full reorganization free energy λ presents itself in the fact that each such displacement can be expressedwithin a harmonic approximationin terms of the normal modes (or phonons) of the respective system. By projecting the displacement ΔR = Ra − Rb onto normal coordinates, it is possible to determine the contribution of each normal mode j to the reorganization energy.113 Denoting the 3N vector of mass-weighted Cartesian , we displacement coordinates of a mode v in state {a,b} by L{a,b} v can express this projection in terms of dimensionless displacement parameters:

C N C N λ in = [Etot (R N) + Etot (R C)] − [Etot (R C) + Etot (R N)]

(24)

The reorganization free energy occurring in polaron hopping rate theories is in general a long-range property describing the electrostatic response of the surrounding medium to changes in the charge state of an active region, such as in a charge transfer between two neighboring sites. This long-range nature of λ is generally hard to capture with electronic structure calculations due to the computational cost of simulating appropriately sized systems. A common way around this problem is to separate short-rangeso-called inner-spherecontributions and longrange, outer-sphere contributions to the reorganization free energy λ = λin + λout. In organic solids, a natural separation is, for example, to designate the actual donor and acceptor molecules as inner sphere and everything else as outer sphere. The advantage of such a distinction is then that λout can, for instance, be estimated in a mean-ﬁeld approach via the Marcus continuum formula89 ⎛ 1 1 ⎞⎛ 1 1 1 ⎞ − ⎟⎟⎜ + − λout = (Δq)2 ⎜⎜ ⎟ εs ⎠⎝ 2ra 2rb dab ⎠ ⎝ εop

νv (ΔR)T 1/2 ·Lav h

Bv =

(25)

where is the diagonal matrix of atomic masses associated with the 3N Cartesian degrees of freedom and ν v is the eigenfrequency of mode v. The weight of the contribution of each mode to the reorganization energy is then given by the 1 dimensionless so-called Huang−Rhys factors Sv = 2 Bv 2 :9,114

(23)

Here, Δq is the charge transferred, while ra and rb are the eﬀective radii of the donor molecule at site a and the acceptor molecule at site b, respectively. dab = |dab| is the distance between the two sites as before, and ﬁnally, εop and εs denote the optical (high frequency) and static dielectric permittivities in order to account for the electronic and nuclear responses of the medium outside of the donor and acceptor cavities. The concept of eﬀective radii is based on a simple continuum solvation model,107 and originally ra and rb were introduced by Marcus as simple ionic radii in solution. While there is no unique deﬁnition of the radii,108−110 a common approximation is to assume the reactants are in close contact yielding ra + rb = dab,111,112 which for identical molecular sites leads to ra + rb = 2ra = dab. This implies that the eﬀective radii can be approximated straightforwardly from lattice parameters of the molecular crystal. The inner-sphere contribution is correspondingly given by the intramolecular reorganization energies of the donor and the

λ=

∑ hνvSv v

(26)

where the sum extends over all (3N − 6) modes. While within the harmonic approximation this is in principle exact for both inner- and outer-sphere contributions to λ, so far this approach has been mostly used for the inner-sphere reorganization energy.9,115−117 In this case the displacement projection is restricted to intramolecular modes, with donor and acceptor modes treated separately. Note that the harmonic approximation is thereby expected to work well for rigid molecules with small λ values, but may break down for ﬂoppy molecules with potentially large deviations from their equilibrium geometries.118 Finally, a related approach to determine the reorganization energy is to perform an MD simulation in one of the charge transfer states to calculate the spectral density function J(ω) of the energy gap coordinate (ΔE) as deﬁned by eq 12:110,119 10327

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews J(ω) =

βω 2

∫0

Review

3.6. Eﬀective Frequency, νeff

∞

dt ⟨δ ΔE(0) δ ΔE(t )⟩ cos ωt

(27)

The eﬀective frequency contained in the LZ transition state expression, eq 13, and the tunneling factor, eq 30, describes the number of attempts to cross the barrier per unit of time. Within the LZ approximation, the barrier to charge transfer is largely determined through the nuclear reorganization. As such, νeff is then the (harmonic) vibrational frequency along the nuclear reaction coordinate connecting Ra and Rb.125 A straightforward way to compute νeff is again given in terms of eigenmodes of the system. As outlined above, the contribution of a given eigenmode v to the overall nuclear reorganization is determined by the respective Huang−Rhys factor Sv. This factor can therefore also be used to weigh the contribution of each mode to the eﬀective frequency125,126

The straightforward generalization of eq 26 to a continuum of vibrational states is then given by the integral over J(ω) λ=

2 π

∫0

∞

dω

J(ω) ω

(28)

3.5. Nuclear Tunneling Factor, Γn

The above expressions for the nuclear reorganization energy λ, eqs 23, 24, 26, and 28, all treat the nuclear degrees of freedom classically, which at low temperatures can lead to an overestimation of the reorganization barrier and thus an underestimation of the hopping rate. This shortcoming is addressed through the introduction of a nuclear enhancement tunneling factor Γn into eq 13. Although most room temperature studies set Γn = 1 as long as the diﬀerences between the two polaronic geometries a and b are not extremely large,81,119 it is important to note here that in the case of organic semiconductors the comparatively large vibrational energy stored, e.g., in CC bonds can lead to signiﬁcant nuclear quantum eﬀects.13 While tests, e.g., on biological systems showed an enhancement factor of around 2 even for comparatively large vibrational energies,119 much lower reorganization energies in organic semiconductors compared to biological systems (≈0.1 vs ≈1 eV)119 can lead to a very diﬀerent behavior. Thus, we here give a brief introduction into one of the main approaches available to determine the nuclear tunneling factor. Given a fully quantum mechanical description kab,quantum of the rate, the nuclear tunneling factor is simply deﬁned as the ratio of the rate at the desired temperature T and its high temperature (T → ∞) classical limit:7,81 Γn(T ) =

νeff =

v

As outlined above, Hab is deﬁned as the electronic coupling between two diabatic states |ψa⟩ and |ψb⟩. Hab = ⟨ψa|Ĥ |ψb⟩TS

(33)

where Ĥ is the Hamiltonian of the system and the subscript “TS” again denotes taking the expectation value at the nuclear transition state. Due to the symmetry of the Hamiltonian matrix, the order of initial and ﬁnal states is irrelevant and thus Hab = Hba. A successful computation of such coupling elements rests mostly on the way the diabatic wave functions are determined. These wave functions are not eigenfunctions of the Hamiltonian. Instead, they represent charge localized states that diagonalize the nuclear kinetic energy operator.127,128 Finding a transformation from the adiabatic eigenstates of the electronic Hamiltonian to such diabatic states is unfortunately not a trivial task, especially for extended systems129 where it generally may not even exist.130 The determination of Hab is therefore the most critical step in calculating polaronic hopping rates. A range of approaches approximating a diabatic electronic basis have been put forward in the literature.131 A key aspect to recognize in this respect is that the value of the electronic coupling element depends strongly on the orbital geometries of the respective diabatic wave functions, and as such also on the geometries of the involved donor and acceptor sites. It is of central importance to ﬁnd diabatization methods that are both computationally eﬃcient and accurate, especially in view of amorphous systems where calculations need to be carried out for many conﬁgurations. One commonly made assumption132,133 is an exponential distance dependence of electronic coupling. This is rationalized with an exponential decay of the diabatic wave function tails and allows for extrapolation of the coupling from just a few donor−acceptor distances. As a further observation, we note that there is an exact relationship between diabatic and adiabatic state energies for a two-state donor/acceptor system. In this case, the energies of the two adiabatic stateslabeled E1 and E2 in the following are connected to the diabatic state energies Ea and Eb via the absolute value of the diabatic coupling as

(29)

⎛ sinh(hνin /2kBT ) ⎞1/2 Γn = ⎜ ⎟ ⎝ hνin /2kBT ⎠ (30)

Here, h denotes Planck’s constant, while νin is an eﬀective frequency of the inner-sphere contributions to the charge transfer mode.81 Note that, only at large eﬀective frequencies or low temperatures, Γn will show signiﬁcant deviation from unity and thus contribute noticeably to the charge transfer rate. Finally, a related expression based on individual vibrational modes was recently given by Zhugayevych and Tretiak13 ⎡ ε ⎞⎤ ⎛ε Γn = exp⎢∑ Sv⎜ v − tanh v ⎟⎥ ⎢⎣ v ⎝ 2 2 ⎠⎥⎦

(32)

3.7. Electronic Coupling, Hab

A number of groups have put forward approximations to the full quantum rate expression120,121 based, among others, on Fermi’s golden rule. Appealingly, the model pioneered by Holstein,122−124 instead yields a closed form expression of the tunneling factor.81

× e−((λ / hνin)tanh(hνin /4kBT )) − (hνin /4kBT ))

Sv ∑k Sk

If the projection of the reaction coordinate is dominated by a single normal mode k, i.e., Sv ≈ δvk, the eﬀective attempt frequency can thus be approximated as the frequency of the corresponding mode νeff ≈ νk.

kab ,quantum(T ) kab ,quantum(T → ∞)

∑ νv

(31)

where Sv and ε again denote the Huang−Rhys factors and eigenenergies of the mode v, respectively. The advantage of eq 31 over the eﬀective treatment of eq 30 is that it yields a more detailed insight into the contributions of each mode to the nuclear quantum eﬀects. 10328

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews E1,2 =

1 (Ea + Eb ± 2

Review

(Ea − Eb)2 + 4 |Hab|2 )

value forcharge localizeddiabatic states. At the TS both adiabatic states are degenerate, and thus “rotate into each other” in the terms of quantum chemistry,142 which gives rise to a sharp change in the dipole moment functions of the adiabatic state. At the TS a transformation between adiabatic and diabatic states can thus be found by diagonalizing the adiabatic dipole matrix.142 In addition, only the components of each dipole matrix element in the direction deﬁned by the diﬀerence between adiabatic dipole moments of the ground and excited states are considered. For a two-state problem as considered here, one thus searches for the set of states diagonalizing the dipole moment matrix. The transformation to these states from the adiabatic ground and ﬁrst excited states is then taken as the diabatic transformation matrix. Denoting by Zuv the elements of the dipole moment matrix for adiabatic states u, v = 1, 2, the diabatic coupling element is thus

(34)

The above expression can simply be obtained by determining the characteristic polynomial of a two-state diabatic Hamiltonian matrix. A furtherand highly utilizedsimpliﬁcation can be obtained for a symmetric problem such as a homomolecular dimer, i.e., equivalent sites a and b, where the energies of both diabatic states are exactly identical: Ea = Eb. It is then easy to see that the excited state gap ΔE12 (cf. Δ‡ in Figure 4) is equal to twice the coupling electronic matrix element. ΔE12 = E2 − E1 = 2|Hab|

(35)

This implies that in symmetric cases the coupling can be calculated with any method that yields accurate adiabatic ground and excited state energies, E1 and E2. This fact was among others exploited by Brédas and co-workers for organic crystals to study the geometrical dependency of coupling matrix elements.134,135 Recently, in the context of DFT-based calculations, e.g., fully eigenvalue self-consistent GW136 has been shown to yield excellent results for the ground and excited state properties of organic crystals. Unfortunately, for asymmetric cases no such simple correspondence exists and some form of diabatization is needed for the calculation of electronic couplings. Over the years a large number of methods aimed at calculating electronic coupling elements have been published.131,137 They diﬀer in several aspects, such as the construction of the Hamiltonian (wave function vs DFT vs semiempirical approaches), the deﬁnition of the diabatic states, and whether full determinants or only frontier orbitals are coupled. Especially in the ﬁeld of quantum chemistry, wave function based diabatization methods have long been the focus of active research. Early examples of such approaches include the block diagonalization138 of the adiabatic Hamiltonian discussed in section 3.7.5the line integral approach,139,140 and the calculation of diabatic states from molecular properties,141 e.g., dipole moments.142 These then led to more advanced methods such as the generalized Mulliken−Hush method129 (cf. section 3.7.1), multistep block diagonalization of complete active space self-consistent ﬁeld (CASSCF) wave functions,143 and the construction of approximate, “regularized” diabatic states by removing only the leading nuclear kinetic coupling terms from an adiabatic representation.144 For the sake of brevity, we here describe in detail only some of the available methods, limiting the discussion to the most common approaches found in the literature. Recent, more focused discussions of the merits and shortcomings of coupling element calculation methods can be found, for example, in refs 133 and 145−147. 3.7.1. Generalized Mulliken−Hush Method. In the past 20 years the generalized Mulliken−Hush (GMH) method, as based on early work by Mulliken148 and Hush149,150 and put forward by Cave and Newton,129,151 has become the de facto reference method for the determination of diabatic coupling elements.133,145 It is based on the assumption that diabatic states localized at diﬀerent sites possess zero oﬀ-diagonal elements of the dipole moment matrix for ground and ﬁrst excited states. This is ultimately based142 on the simple observation that the transition dipole moment between ground and excited states tends to vanish in thecharge delocalized adiabatic picture but necessarily takes on a relatively large ﬁnite

GMH |Hab |=

|Z12| (Z11 − Z 22)2 + 4 |Z12|2

ΔE12 (36)

Note that in the case of a symmetric donor/acceptor system (Z11 = Z22), this expression for the coupling reduces trivially to the exact value of half the ground/ﬁrst excited state energy splitting of eq 35. Also, in the literature the dipole moment matrix is generally denoted by the letter “μ”, which we avoid here in order to distinguish it from the carrier mobility. The GMH method is thus applicable to every electronic structure method that yields an accurate excited state splitting and gives access to transition dipole moments of these states. It is thus most often used in conjunction with wave function based approaches or hybrid-level time-dependent density functional theory (TDDFT), both of which tend to be rather computationally demanding for large systems and extended solids as of interest here. 3.7.2. Constrained Density Functional Theory. There are a number of formulations of constrained density functional theory (CDFT). They nevertheless all rest on the same idea of adding an external potential to the density functional theory (DFT) electronic Hamiltonian in order to restrict the selfconsistent ﬁeld (SCF) cycle to a certain predetermined molecular reference charge distribution. In the context of charge transfer between a donor and an acceptor site, this allows for the generation of approximate diabatic states by forcing the transferred charge (electron or hole) to localize at certain atoms or groups of atoms that comprise the donor and acceptor groups, respectively. As pointed out, e.g., by Wu and van Voorhis,152 this basic idea is almost as old as the ﬁeld of computational electronic structure theory itself, with its ﬁrst use for a small model system already in 1963 by Karplus and Mukherji.153 Later it was, among others, picked up by Dederichs,154 Akai,155 Hybertsen,156 Zhang,157 Warshel,158,159 and Behler et al.160,161 for ﬁrst studies of defect states, magnetism, and charge transfer reactions. Today, most modern applications of the CDFT approach for molecular systems are based on work by Wu and van Voorhis,152,162−164 who formulated CDFT in the form of a scleronomic (i.e., not explicitly time-dependent) constraint on the charge (or spin) density which is added to the Kohn−Sham energy functional via a Lagrange multiplier. This new energy functional F[ρ,VL], acting on an electron density ρ, then reads92

∫

F[ρ , V L] = E[ρ] + V L( w(r) ρ(r) dr − Nc) 10329

(37)

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

Figure 7. Hirshfeld weight function for a donor/acceptor pair of molecules in a tetracene crystal. Red shaded areas depict positive (charge accumulating) regions; blue areas depict negative (charge depleting) regions of the weight function. Shown in gray are surrounding molecules not directly included in the weight function.

where the ﬁrst term denotes the unconstrained Kohn−Sham energy functional and the second term denotes the constraint. There, VL is the Lagrange multiplier regulating the strength of the external potential, w(r) is the weight function deﬁning the regions of space that the charge is constrained to, and Nc is the desired charge in the region deﬁned by w. Note that the Lagrange multiplier cannot generally be determined analytically, but has to be optimized separately in a loop on top of the normal density SCF cycle. Also, it is evident from eq 37 that the ﬁnal, self-consistent charge-constrained state will depend somewhat on the choice of the weight function.92 Yet, this at ﬁrst severe drawback is alleviated greatly in the calculation of coupling elements (see below), which in practice show only a limited sensitivity to the weight function.165 Nevertheless, this problem is analogous to attributing electronic charges to atoms in molecules. In the case of DFT, many diﬀerent deﬁnitions of such charges exist, e.g., by Mulliken,166 Hirshfeld,167 or Bader168 to name only a few of the most popular ones. Among these, a real-space deﬁnition of w(r), often based on a form of Hirshfeld charges, has emerged as the standard choice for the study of charge transfer in the diabatic picture,11,132,169 due to their very good accuracy,133,145 robustness, and basis set independence.170 For a constraint on the charge in a region D of a system with M atoms, the Hirshfeld weight function reads w(r) =

CDFT Hab = ⟨ψaCDFT|/ KS[ρb ]|ψbCDFT⟩

= Fb⟨ψaCDFT|ψbCDFT⟩ − VbL⟨ψaCDFT|wb|ψbCDFT⟩ (39a) CDFT Hba = ⟨ψbCDFT|/ KS[ρa ]|ψaCDFT⟩

= Fa⟨ψbCDFT|ψaCDFT⟩ − VaL⟨ψbCDFT|wa|ψaCDFT⟩ (39b)

Note that in this formulation HCDFT (eq 39a) would not be ab guaranteed to equal HCDFT (eq 39b). This complicates the ba comparison of CDFT transition matrix elements to those determined with other methods or with experiment. Furthermore, the CDFT-generated diabatic reference wave functions are not generally orthogonal, as they are not eigenstates of the same Hamiltonian. States ψCDFT and ψCDFT a b CDFT CDFT generally have nonvanishing overlap, ⟨ψb |ψa ⟩ = SCDFT . ab This motivates a transformation as done in the GMH method (see section 3.7.1); i.e., to arrive at the ﬁnal diabatic states they are transformed such that the ﬁnal wave functions ψa,b diagonalize both their overlap matrix = ⟨ψu|ψv⟩ and the weight matrix = ⟨ψu|wv|ψv⟩ with u and v ∈ {a,b}. Matrix elements Hab = Hba in the basis of the orthogonal states are then symmetric and can be compared to other methods. In passing we note that an analogous formulation of CDFT for extended solid-state systems was put forward by Behler and co-workers.161 In their work, the constraint potential is not determined via a Lagrange multiplier but rather via the equalization of the Fermi levels between the constraint regions. This nevertheless leads to equations very similar to those outlined above. On a ﬁnal note we also point out that recently Rapacioli et al. combined the CDFT approach with a selfconsistent charge tight-binding formulation of DFT.171−173 In the latter method, the total energy functional is expanded to second order in a localized basis set, to ultimately yield a Hamiltonian matrix analogous to “full” DFT but with precalculated and tabulated elements for each atomic basis function. An in-depth review of DFTB methods can, for example, be found in refs 174−176. 3.7.3. Fragment Orbital Methods. The fundamental assumption behind the fragment orbital (FO) family of methods is that only the frontier orbitals directly partaking in the charge transfer do change between the initial and ﬁnal diabatic states.177,178 All others remain unperturbed. To illustrate this assumption, we consider the transfer of an excess electron from a donor group to an acceptor group. Excluding the excess electron, the donor group has M occupied orbitals while the acceptor hasin generalN occupied orbitals.

∑u ∈ D ρu (r − R u) M

∑u = 1 ρu (r − R u)

(38)

where ρu(r − Ru) is the noninteracting, sometimes also called promolecular, free atom density of atom u on position Ru. For charge transfer between a donor and an acceptor group, the constraint can actually also be expressed as a constraint on the charge diﬀerence between the groups.92 This avoids the need to deﬁne absolute charges of the respective donor and acceptor groups. An example of a weight function for a charge transfer dimer of tetracene molecules in a tetracene crystal is shown in Figure 7. Within the CDFT framework the diabatic state wave functions ψCDFT and ψCDFT are approximated by those of a b Kohn−Sham eigenstates of suitably constrained DFT calcul a t i o n s w i t h H a m i l t o n i a n s / KS[ρa ] + VaLwa a n d / KS[ρb ] + VbLwb , respectively. The Hamiltonian transition matrix elements between both states can then in principle be determined as 10330

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

Denoting these single electron orbitals as ϕiD,A for donor and acceptor, respectively, diabatic wave functions are given by ψa =

1 (M + N + 1)!

this creates in principle two Hamiltonians that diﬀer by the fragment orbital the electron was removed from, in close analogy to the situation in the CDFT approach. Due to numerical inaccuracies this can in turn lead to diﬀerences between the two matrix elements Hab and Hba and thus a nonHermitian diabatic Hamiltonian. Standard practice in such cases is to average over the two oﬀ-diagonal elements, which amounts to a symmetrization of the two-state Hamiltonian. This approach does, however, neglect (HT) or overestimate (ET) charge reorganization within the respective fragments due to the excess charge.179 A most recent version of FO-DFT179 does also consider these intrafragment eﬀects of the excess charge by constructing the reference state from a charged and an uncharged fragment, e.g., ψM+c and ψNA as illustrated in Figure 8. The Hamiltonian D

det(ϕD1 ··· ϕDM ϕDM + 1ϕA1 ··· ϕAN ) (40a)

ψb =

1 (M + N + 1)!

det(ϕD1 ··· ϕDM ϕA1 ··· ϕAN ϕAN + 1) (40b)

Under the above assumption of otherwise constant orbitals, the calculation of the transition matrix element between wave functions ψa and ψb reduces to determining the Kohn−Sham matrix element between the two single-electron frontier orbitals FO‐DFT Hab ≈ ⟨ϕDN + 1|/ KS|ϕAM + 1⟩

(41)

This implies thatgiven the knowledge of the eﬀective singleparticle Hamiltonian of the systemthe matrix element only depends on orbitals which are localized on either the donor or the acceptor. In the case of intermolecular charge transfer this gives rise to the idea of treating the donor and acceptor as fragments in two separate calculations and then combining their wave functions to determine / KS and the transition matrix element. This approach guarantees the localization of the diabatic wave functions on the respective fragments independent of any errors of the underlying method, such as the electron delocalization error of semilocal DFT.95 On the other hand, in separating donor and acceptor fragments any direct inﬂuences between thempredominantly polarization of one fragment through the charge density on the other oneare neglected. Furthermore, the way how the full Hamiltonian is constructed from the fragment wave functions gives rise to a number of diﬀerent “ﬂavors” of the FO-DFT method.16 Speciﬁcally this concerns the number of electrons used to construct the reference donor and acceptor states, as well as / KS. In the original formulation of the method by Senthilkumar and co-workers,177 regardless of the actual charge transferred, the Hamiltonian is always constructed from the orbitals of the neutral fragments and the reference states are taken as the lowest unoccupied molecular orbitals (LUMOs) in the case of electron transfer (ET) and the highest occupied molecular orbitals (HOMOs) in the case of hole transfer (HT). In this approach the Hamiltonian is therefore constructed from a charge density that deviates from that of the real combined system by exactly the charge that is initially on the donor and that is actually transferred, / KS = / KS[ρ(M + N )]. Computationally, this holds the advantage that only neutral fragments need to be calculated, but can lead to systematic deviations of the matrix elements due to the deviating number of electrons.133,145 Another approach is therefore to treat both fragments in the reduced state (M + N electrons in the case of HT and M + N + 2 for ET) in order to determine the reference states and to construct / KS from these orbitals with the occupation number of one of the frontier orbitals set to 0 (ϕND and ϕM A for HT states M+1 ψa and ψb, respectively, and ϕN+1 for ET states ψa and D and ϕA ψb, respectively).37,132 This approach guarantees the correct number of electrons in the eﬀective Hamiltonian / KS = / KS[ρ(M + N − c)], where c = +1 for electron transfer and c = −1 for hole transfer. In nonsymmetric systems

Figure 8. Sketch of the fragment orbital DFT approach for hole transfer across an ethylene dimer. Both fragments, donor and acceptor, are treated separately when determining their SCF ground state wave functions and densities ρ[{D,A+}]. These are then used to construct a Hamiltonian of the combined system, with the wave functions acting as reference orbitals for the diabatic state.

constructed this way not only has the correct overall number of electrons but also directly includes orbital relaxations due to the excess charge. This, on the other hand, comes at the price of more approximate reference orbitals. All three of these “ﬂavors” of FO-DFT have been compared and critically discussed in a recent study by Schober and co-workers.179 In this work results showed a clear advantage of the latter charged fragment orbital procedure, potentially yielding much greater accuracy than “standard” FO-DFT approaches and at very little additional computational cost due to the need to calculate both charged and neutral fragments. As a side note, Baumeier et al.180 as well as Sutton et al.181 recently demonstrated, in their exhaustive studies of density functionals, the functional dependency of FO-DFT calculated coupling values for organic semiconductors. The latter demonstrated a near-linear correlation of Hab with the amount of exact exchange in the functional, ultimately scaling the coupling by almost a factor of 2 from GGA functionals to pure Hartree−Fock calculations. This further underlines the need to carefully benchmark calculated coupling elements against available test data.133,145 Finally, it is important to note that, although successfully applied by a number of groups,16,104,133,145,177,179,182 fragment orbital approaches are not all restricted to the use with DFT. Indeed any electronic structure method that allows for a combination of fragment wave functions and gives access to a combined Hamiltonian would be suitable. Elstner, Kubař, and co-workers, for instance, presented a series of studies based on a DFT tight-binding (see above) formulation of the fragment orbital approach (FO-DFTB).176 The early research focus there lay on charge transport in DNA183−185 and biomolecular polypeptides.186,187 Most recently, though, the FO-DFTB approach was also applied to CT in organic semiconductors.188,189 There it was also demonstrated that environmental 10331

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

Initially this ansatz was used to eﬃciently determine DFT energies of large supersystems. It was thereby noted early on that the FDE method naturally suppresses the semilocal DFT electron delocalization error and yields fragment-localized charge states similar to the diabatic states of electron transfer.200−202 Pavanello and co-workers have pointed out 146,203,204 that this is mostly due to the missing orthogonality between orbitals of diﬀerent fragments, the localized initial guess, basis sets which eﬀectively rule out delocalization of orbitals over more than one fragment, and eﬀective repulsive regions near the frozen densities of other fragments. Having constructed the diabatic reference states, one could in principle proceed similarly to the FO-DFT or CDFT methods by determining the combined system’s Hamiltonian and extracting the respective matrix elements. The approach chosen by Pavanello195,203,205 instead follows a slightly diﬀerent path, observing that the coupling between (nonorthogonal) diabatic states a and b can be approximated as

eﬀects can straightforwardly be incorporated into FO calculations, e.g., via quantum mechanical/molecular mechanical embedding approaches.176,190 Concerning the accuracy of this approach, recent benchmark studies133,145 indicated relative errors of FO-DFTB matrix elements to be ∼10−20% larger than that of the respective FO-DFT ﬂavors, yet, of course, at much reduced computational cost. Even more economical variants of the FO scheme are based on semiempirical electronic structure methods such as Zerner’s independent neglect of diﬀerential overlap (ZINDO).191 In this method, the Hamiltonian is also constructed in a localized minimal basis, yet with empirically determined parameters. Kirkpatrick and co-workers showed27,192,193 the feasibility of such an approach even for very large systems. Finally, Akimov194 recently employed a fragment orbital scheme based on extended Hückel theory to determine electronic couplings for use in the nonadiabatic propagation of charge carriers (cf. section 5.3). 3.7.4. Frozen Density Embedding. The frozen density embedding (FDE) ansatz, initially presented by Wesolowski and Warshel158 and later adapted to electronic coupling calculations by Pavanello and Neugebauer,195 rests on the partition of a large, but noncovalently bound system into smaller fragments. The total density of the system is thereby expressed as a sum over the number NS of subsystem densities ρw(r)

Hab ≈ SabE[ρ(ab)(r)]

where Sab is the overlap between the two Kohn−Sham determinants of a and b, E[ρ(ab)(r)] denotes an energy functional of a transition density occ

ρ(ab)(r) =

NS

ρ (r ) =

∑ ρw (r) w=1

(43a)

∑ ϕu(a)(r)((ab))uv

−1 (b) ϕv (r)

uv

(43b)

and the sum goes over all occupied states. The overlap matrix between all orbitals contributing to a and b is denoted by (ab). This approximation can be seen as motivated by the solution of a generalized eigenvalue problem for thegenerally unknowndiabatic Hamiltonian.206 In order to yield a coupling element comparable to other methods, the ﬁnal step in this procedure is an orthogonalization step of the resulting diabatic Hamiltonian matrix via

(42)

The main diﬀerence from FO-DFT is that the fragments do interact with each other via their Kohn−Sham eﬀective potentials. In essence, for each fragment a DFT SCF cycle is performed including a constant embedding potential described as the sum of the Kohn−Sham potentials of all other fragments. This in turn yields a new eﬀective potential per fragment. This change in potential has to be accounted for in an outer SCF cycle for each fragment to respond to the presence of the other fragments.196,197 As an illustration of this approach, we depict in Figure 9 the local part of an FDE potential for a cluster of tetracene molecules.

FDE Hab =

⎛ Haa + Hbb ⎞ 1 ⎜H − S ⎟ ab ab ⎠ 2 1 − Sab 2 ⎝

(43c)

(ab)

The energy functional E[ρ (r)] appearing in eq 43a in principle denotes an appropriate energy functional of the full system evaluated for the transition density ρ(ab)(r) given in eq 43b.203 Yet, it can also be calculated from fragments according to the frozen density embedding scheme. 3.7.5. Block Diagonalization of the Electronic Hamiltonian. Based on ideas similar to those for the fragment orbital method, block diagonalization (BD)138,143,151 approximates the coupling between the two diabatic wave functions by the oﬀdiagonal elements of a reference Hamiltonian in a localized basis. Initially conceived for wave function based electronic structure methods, the approach has found use with DFT in the context of extended systems.207 We will therefore illustrate it in terms of a Kohn−Sham DFT Hamiltonian, but keeping in mind that the method can equally be used with Hartree−Fock, single-referene, or multireference wave function based approaches. The basic principle of the BD method is to transform the Hamiltonian matrix from a localized atomic basis into a basis of eigenstates of fragments of the complete system. These fragments are chosen analogously to the FO-DFT ansatz but, as will be seen below, can also be covalently bonded to other fragments. The basis of fragment eigenstates is found by separate diagonalization of the Hamiltonian submatrices

Figure 9. Illustration of the local part of the isosurface of the embedding potential of a cluster of tetracene molecules acting on a central molecule (calculated with DFT-PBE198 and using the FHI-aims code199). In an FDE calculation, the embedding potential is constructed as a superposition of the potentials of each participating fragment {A−D, F−I}, with one of the fragments treated explicitly {E}. Density and potential of the central fragment E would then be determined by treating the embedding potential as ﬁxed, to be used in the determination of the embedding potential of the other fragments in an outer SCF cycle. 10332

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

to represent unoccupied orbitals.215 Careful consideration of the resulting reference orbitals is therefore generally necessary. 3.7.6. Analytic Overlap Method. The methods discussed so far, while reasonably accurate and signiﬁcantly cheaper than quantum chemical reference methods, still require at least one DFT calculation per geometry. In the case of static, rate-based approaches, a single-point DFT calculation per donor/acceptor pair is in general computationally aﬀordable, even in systems with a large number of local donor/acceptor conﬁgurations.37 Yet, there are cases where even such comparatively undemanding approaches become unfeasible. An example would be a direct propagation of the excess charge in a nonadiabatic MD scheme as discussed in section 5.3. There, or in the case of snapshot sampling for disordered systems, a rapid on-the-ﬂy estimation of Hab is essential. In such cases one needs to resort to semiempirical approaches, for instance, FO-DFTB, where relevant integrals are tabulated and are readily available for a given molecular geometry. An even simpler way to rapid estimation of electronic couplings was recently suggested by Gajdos et al.216 Their analytic overlap method (AOM) rests on the idea of establishing a correlation between the electronic coupling and a descriptor that can be very rapidly calculated for a given donor−acceptor geometry. A good linear correlation between the electronic coupling and singly occupied molecular orbital (SOMO) overlap SSOMO was, for instance, identiﬁed. ab This is analogous to resonance integral calculations in extended Hückel theory, which only diﬀer in the type of reference state used in place of the atomic orbitals. Furthermore, Gajdos et al. approximated the overlap integral through an analytical expression, by projecting the frontier orbitals of a reference DFT calculation onto Slater-type p-orbitals. This way, for not too radical departures from the molecular reference geometry, SSOMO can be estimated without any further DFT calculations ab for the diﬀerent geometries. For example, along an MD trajectory the direction of the atomic p-orbital basis functions that form a given fragment π-orbital are updated at each nuclear time step. This is in a ﬁrst approximation performed simply by enforcing the p-orbital axis to lie perpendicular to the πconjugated plane deﬁned by the atom it is centered on and its neighboring atoms. In the AOM approximation the Hamiltonian matrix element reads

belonging to each of the fragments, where the fragments are identiﬁed by their respective localized basis functions. Within these eigenspaces one can then determine the frontier orbitals by counting the states up to the HOMO and LUMO orbitals of the fragments. The unitary transformation matrix of the complete Hamiltonian is thereafter simply given as a combination of the eigenvectors a , b of the fragments a and b. ⎛ a 0 ⎞ = ⎜⎜ ⎟⎟ ⎝ 0 b ⎠

(44)

The electronic coupling Hab is ﬁnally extracted from the thustransformed Hamiltonian as the matrix element between the respective frontier orbitals as illustrated in Figure 10.

Figure 10. Demonstration of the block-diagonalization method for a benzene dimer (calculated with DFT-PBE198 and using the FHI-aims code199). Shown is an orthogonalized and block diagonalized Hamiltonian matrix, for illustrative purposes in a logarithmic scale of the absolute values. Elements belonging to the approximated HOMO orbitals on molecules a and b are highlighted by gray lines.

Unfortunately, this method does suﬀer from some ambiguity when comparing it to other methods, since the localized basis functions of the respective fragments generally show nonvanishing overlap with each other. This means that in order to obtain meaningful Hamiltonian matrix elements208−210 it is advantageous to introduce a basis set orthogonalization step, e.g., employing the symmetric method of Löwdin:211,212 ortho = T

SOMO HabAOM = CSab

(47)

where C is a constant of proportion obtained by a linear ﬁt to Hab values from explicit electronic structure calculations. For a training set of small organic molecules, Gajdos et al. determined C to be 1.819 eV. The same linear correlation was applied remarkably well to a test set of π-conjugated molecules not included in the calibration. With a view of dynamical trajectories, the authors further tested the importance of updating the p-orbital expansion coeﬃcient at each nuclear time step and found that it can be neglected for rigid molecules.93 However, for larger molecules with soft intramolecular modes (e.g., polymers) the fragment orbitals may undergo large electronic reorganizations as the nuclei evolve. In this case one could carry out an ensemble of reference electronic structure calculations for important conformations and use on-the-ﬂy interpolation methods to reconstruct the fragment orbital during the MD simulation. Due to the fact that this method rests solely on analytical terms and just a single reference DFT calculation per molecule is required, its speed easily surpasses any other method on the

(45)

(46) = −1/2 where denotes the overlap matrix. Complications arise here, because any orthogonalization scheme necessarily mixes the basis functions and thus potentially blurs the clear separation between donor and acceptor fragment orbitals. Yet, as pointed out, e.g., by Thoss and co-workers,207 the symmetric approach has two advantages. First, it is least biased compared to other methods, such as the Gram−Schmidt scheme, where all basis functions are orthogonalized with respect to one unchanged reference basis function.212,213 Second, the Löwdin method preserves the character of the basis in a least-squares sense such that its localization is mostly retained and thus the separation between fragments is mostly upheld.214 Yet there are still systems where the donor/acceptor separation fails at this stage, especially in the case of larger basis sets necessary, for instance, 10333

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

current list, while nevertheless reaching comparable accuracies. While Gajdos et al. observed a remarkably good linear correlation for a wide range of π-conjugated compounds, it may be advantageous (and straightforward) to reparametrize the linear relation for a given molecule under consideration for a further reﬁnement of the coupling value estimation. The constant of proportionality is thereby very sensitive to the exponential decay of the frontier orbitals. Hence, application of AOM to ET between nonorganic/non-π-conjugated donor− acceptor systems would require parametrization of the relation. 3.7.7. Superexchange Eﬀective Couplings. While not a diabatization method, we consider here also the case of eﬀective couplings for superexchange (SE) charge transport. All previously mentioned approaches considered direct ET between donor and acceptor with the space between them being empty (vacuum). If the space between donor and acceptor is made up of molecules or a covalent bridge connecting them, most of these methods can still be used to compute couplings. However, the values quickly become very small with increasing bridge length. Here the SE model for ET can be used to estimate eﬀective electronic couplings. In this method it is assumed that the ET is mediated by the lowest unoccupied and/or highest occupied orbitals of the bridge. These bridging orbitals possess considerably diﬀerent site energies (ΔG0 ≠ 0) even without an external electric ﬁeld, or they could simply be considered as other diabatic states. Examples for SE can be found in monocrystals bearing point defects, among diﬀerent molecules in heterocrystals, or in disordered systems.217 In the SE model the eﬀective coupling between donor and acceptor sites can be eﬀectively be expressed using the Green’s function of the bridge35 B (E) = (E B − B )−1

Figure 11. Illustration of a possible hopping network in a naphthalene crystal. Shown is a 2D cut of the crystal with each nearest and nextnearest neighbor sites connected to each other.

sites a and b with a rate kab. Such a problem is ideally suited for a solution with kMC. The advantage of a kMC approach over the analytical solution with eq 11 is that it can also be applied to less-regular systems, including, for example, lattice defects. Among a variety of diﬀerent, numerically eﬃcient kMC algorithms, we will limit our discussion to the common, socalled “rejection-free” procedure.225 In the case of just a single excess charge carrier moving through a system, thus disregarding any interaction between carriers, the corresponding kMC algorithm turns out to be surprisingly simple. 1. At each kMC step with the carrier localized at site a, determine the site b for the next hop from the pool of connected sites with a probability proportional to the rate kab associated with this connection. Technically, this can be achieved by picking a random number p between 0 and ∑b kab, where the sum goes over all sites connected with nonzero rate to the current site a. The site b to hop to is then determined by ﬁnding which interval

(48)

where B and B are overlap and Hamiltonian matrices of the bridge orbitals, and E is the tunneling energy, which is generally taken as equal to the energy at the transition state between the initial and ﬁnal states.14,218 The bridge-mediated eﬀective coupling element is then given as a sum over all bridge states NB:

b

p ∈ [ ∑ ka(b ′− 1) ,

NB (SE) Hab =

∑

b ′= 0

(Hau − ESau)GuvB (Hbv − ESbv)

u,v=1

b+1

∑ ka(b ′− 1)] b ′= 0

(50)

the chosen random variable falls into. 2. Having picked the process a → b to execute, the simulation timer needs to be advanced. The waiting times t for this process to occur are hereby exponentially distributed:

(49)

Here, Hau and Hbv are the coupling elements between the bridge states and the donor and acceptor orbitals, respectively, while Sau and Sbv are the respective overlap matrix elements. While superexchange models have so far been mostly applied in biochemical simulations,14,219,220 ﬁrst applications in organic solids recently started to emerge,217 and more can be expected as research moves toward more complex systems.

pab (t ) = kabekabt

(51)

Thus, the next step is to pick an exponentially distributed random variable to advance the simulation clock. 3. Having picked a process and a waiting time, the ﬁnal step in a kMC cycle is to move the carrier to the new site b and return to step 1. This kMC cycle is repeated either for a number of steps or until a given desired total simulation time τ is reached. The procedure hereby mimics charge diﬀusion trajectories through the molecular solid. In order to determine the mobility according to either eq 4 or eq 6, one needs to determine either the average drift velocity or the root-mean-square displacement, respectively. This can generally be achieved by averaging over many created kMC trajectories. In the standard case of timeindependent ﬁelds and bulk crystals, this is typically replaced by a time average over one suﬃciently long kMC trajectory. For

3.8. Kinetic Monte Carlo Simulation of μ

Initially developed to track radiation damage in solids,221 the kinetic Monte Carlo (kMC) method has evolved in the past 50 years into the main method to study the dynamical evolution of reaction networks connected by rare events.28,222,223 As alluded to earlier, charge carrier hopping through a solid can be viewed as exactly such a process.27,91,193,224 This is illustrated in Figure 11, where we depict the network of all possible nearest and next-nearest neighbor carrier hops in a naphthalene crystal. The basic assumption behind a hopping model is that carriers are localized on individual sites (here individual naphthalene molecules) and percolate as a series of discrete hops between 10334

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

resistive molecular memories. A similar approach was recently followed by Huong, Tai, and Nguyen for modiﬁed thiophene compounds.234 McMahon and Troisi235 evaluated the reorganization free energies of several polyacenes as a measure for their hopping mobility, and Cornil and co-workers employed hopping models to study interfacial dielectric layers of pentacene on polystyrene and polymethacrylate.236 Yet the application of hopping models is not solely conﬁned to ordered molecular crystals. For example, Friederich et al.99 recently published a study of disorder eﬀects of amorphous materials composed of coordination complexes (tris(8hydroxyquinolinato)aluminum) and molecules (N,N′-di(1naphthyl)-N,N′-diphenyl-(1,1′-biphenyl)-4,4′-diamine) and could accurately reproduce experimental mobilities over a range of 4 orders of magnitude. Even more interest was garnered by organic polymer devices, which, due to their disordered nature, can for the most part also be treated with hopping models. Examples for this are the work of Athanasopoulos et al. on polydioctylﬂuorene,237 the works of Nelson,193 Fornari,62 and Pershin238 and their respective coworkers on various modiﬁcations of polythiophenes, and the work of Walker on polyﬂuorenes and polyvinylenes,239 all of which rest on hopping models. In general, the straightforward applicability of the model and the wealth of relatively inexpensive methods to determine its parameters make hopping models still one of the most used models for charge transport in organic solids.

the average drift velocity one thereby considers that each carrier hop a → b in the trajectory covers the distance vector between the centers of mass dab. For the Einstein−Smoluchowski mobility expression, eq 6, these distances can be squareaveraged and tabulated versus the corresponding waiting times t to yield the component-resolved MSD and thus the diﬀusion matrix Dij. For the general mobility equation, eq 4, a ﬁeld E can be applied, which corresponds to adjusting the hopping rates (eqs 13−18, depending on which rate theory is considered). The drift velocity averaged over the whole simulation is then simply determined by the distance vector between the center of mass of the initial site for the excess charge Rinitial and its ﬁnal site Rfinalpossibly taking care of periodic boundary conditionsand the overall simulation time τ: ⟨v⟩ =

R final − R initial τ

(52)

As noted, this simpliﬁed approach applies only to the diﬀusion of a single excess charge carrier, or equivalently to a negligible interaction between excess charge carriers. This approximation holds typically only for very dilute carrier concentrations. For higher carrier densities one generally needs to include interactions with other carriers to achieve a faithful representation of carrier diﬀusion.226 Prominently this concerns the “blocking” of sites by carriers or ﬁnite Coulomb interactions between carriers localized at neighboring sites. The practical treatment of such lateral interactions in kMC simulations is still very much the subject of active research, and we refer the interested reader to refs 227−231 and references therein for a discussion of present state-of-the-art approaches.

4. BAND TRANSPORT REGIME The other regime in which charge transport in condensed matter is mainly discussed is the exact opposite of charge hopping. Whereas in the hopping model charges are assumed to be localized on discrete sites, band theory assumes a delocalization of charge carriers in periodic carrier bands. There is a wealth of literature on the topic of band transport, and (mainly inorganic) semiconductor research has made immense progress in reﬁning band models over the years.240−243 Apart from a more complex crystal structure that is bound by a mixture of covalent andimportantlydispersive forces,136 there is no fundamental diﬀerence between a highly pure organic semiconductor and an inorganic semiconductor that would prohibit the application of these band models also to charge transport in organic solids. The fundamental basis of band theory is Bloch’s theorem. This theorem establishes the general form of an electron orbital in a periodic potential as a superposition of plane waves modiﬁed by a set of periodic functions. By construction, band theoretical approaches are thus restricted to ordered and relatively defect-free crystals, and therefore are not suited for disordered semiconductors such as polymeric solids. Considering the general deﬁnition of charge mobility of eq 4, the deﬁning quantity is again the ﬁeld-dependent time-averaged velocity of the carrier. In this particular case, this velocity corresponds to the average of the group velocity vg of the charge carrier’s wave packet. Given a wave packet composed of Bloch functions with wave vectors near a reciprocal space vector ko and belonging to energy band α, the ﬁeld-free group velocity is given by the reciprocal space gradient of the dispersion relation

3.9. Applications

The use and value, but also the limitations, of hopping models in the context of charge transport in organic crystals are documented in a wide range of literature. C60 and other fullerene derivatives are certainly among the most thoroughly studied molecular solids of the past decade. In 2009 Nelson and co-workers193 employed a Marcus-hopping model, based on semiempirical electronic structure calculations, to study the grain-size dependence of the mobility in disordered C60 ﬁlms. In good agreement with experiment, their simulations showed only a slight dependence of the mobility on the grain size. The same group later studied the eﬀect of C60 functionalization on packing order and thus mobility.26 The actual validity of the hopping model in general and the speciﬁc hopping regimes (section 3.1) in particular was only subsequently scrutinized by some of us, ﬁrst for unmodiﬁed C60 fullerenes37 and later for the popular PCBM modiﬁcation.38 In these DFT-based studies outliers with large coupling elements did cast doubt on the general applicability of the hopping model in these systems. On the other hand, experimental mobilities could still be reproduced to within the correct order of magnitude. In a similar approach, Idé and co-workers232 studied the mobility of crystalline fullerene derivativesPCBM and 1-(3methoxycarbonyl)propyl-1-thienyl-[6,6]-methanofullerene (ThCBM)in a hopping-based kMC model to estimate the inﬂuence of chemical modiﬁcation on the fullerenes’ transport properties. With regard to other molecules, Di Motta et al.233 estimated charge diﬀusion constants for benzoquinone derivatives2,3dichloro-5,6-dicyano-1,4-benzoquinone (DDQ), tetrachlorobenzo-1,4-quinone (TCQ), and tetracyanoquinodimethane (TCN)as well as pentacene to establish their suitability as

vg = 10335

1 ∇k εα(k) ℏ k=ko

(53) DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

⎛ ∂f ⎞ ⎛ ∂f ⎞ ⎛ ∂f ⎞ ∂f =⎜ ⎟ +⎜ ⎟ +⎜ ⎟ ⎝ ∂t ⎠field ⎝ ∂t ⎠diffusion ⎝ ∂t ⎠collision ∂t

Thus, all transport properties of the periodic medium are determined by its band structure represented as a reciprocal space function of electronic eigenenergies, i.e., the dispersion relation εα(k) (see Figure 12 for a representative example). In

It can be solved either by performing a Monte Carlo integration in momentum space245 (a technique that although successfully used for inorganic systems has not yet widely been applied to organic semiconductors) or by introducing the so-called relaxation-time approximation (RTA).246 In the latter method, one linearizes the relaxation of an electron distribution in a given energy band and distorted by an external ﬁeld toward the ﬁeld-free ground state. This leads to a time constant, the relaxation time τs, which is the average time between (elastic) scattering events that reset the carrier distribution in a band. In general, the relaxation time isin exact analogy to the eﬀective massa tensor of rank 2, yet for the sake of simplicity it is often transformed into the principal axes of the crystal.247 In the following we will thus, for improved legibility, also give only the diagonal elements of the involved tensorial quantities, unless stated explicitly otherwise. For a full discussion of band mobilities including anisotropies, we refer the reader to a more specialized discussion in ref 248. In this simpliﬁed formulation and within the RTA, the carrier group velocity is given as249

Figure 12. Semilocal (PBE) DFT valence (orange) and conduction (blue) band structure of a rubrene crystal (cf., e.g., Szulczewski et al.250). Note the relatively large dispersion (curvature) of both conduction and valence bands. In this case the eﬀective mass would be estimated either at the Γ-point or the Z high-symmetry point. Also, given the band gap of ≈1.2 eV and the Fermi level position centrally within the gap, the intrinsic charge carrier concentration would be very low (cf. section 2.1). To still yield nonvanishing conductivity, mobile charge carriers would have to be introduced either via defects or doping.

⎛ 1 ⎞ vg, i = qEiτis⎜ ⎟ ⎝ mα* ⎠ii

fact, it is relatively straightforward to show34 that the change of velocity of a particle with charge q in band α of a periodic semiconductor and due to an applied electric ﬁeld E simply follows a Newtonian equation of motion ⎛ 1 ⎞ −1 dvg, j Fi = qEi = ⎜ ⎟ dt ⎝ mα* ⎠ij

(57)

Inserting this result for the average carrier velocity into the deﬁnition of the mobility, eq 4, yields ⎛ 1 ⎞ ⎟ μii = qτis⎜ ⎝ m* ⎠ii

(58)

without any explicit dependence on the applied electric ﬁeld. Additionally, we here and henceforth drop the index α denoting the respective band of the charge carrier. In the vast majority of cases, it is understood that the charge carrierelectron or holeoccupies its respective lowest energy conﬁguration. As such, the bands in question are those closest to the Fermi level, the CBM for electron transport or the VBM in the case of hole conduction. In summary, in band theory there are two parameters, two second rank tensors to be precise, that need to be evaluated computationally to determine the mobility. Namely, they are the eﬀective mass, which can quite straightforwardly be estimated from the material’s band structure, and the relaxation time. The latter is not as straightforward to calculate. It depends on macroscopic properties such as defect concentration, longrange order, andthrough phononic contributionselastic properties of the material.

(54)

albeit with a generalized eﬀective mass (m̲ *α ), deﬁned as the curvature of the respective band dispersion relation 2 ⎛ 1 ⎞ 1 ⎛ ∂ ε (k) ⎞ ⎟ = 2 ⎜⎜ α ⎟⎟ ⎜ ℏ ⎝ ∂ki ∂kj ⎠ ⎝ mα* ⎠ij

(56)

(55)

Here, vg,i and Ei denote the ith components of the group velocity and the electric ﬁeld, respectively. Note that eq 54 is a harmonic approximation valid only near the valence band maximum (VBM) and the conduction band minimum (CBM) for holes and electrons, respectively. It is therefore limited to small enough electric ﬁelds. Even then, without any dissipative terms this would imply an indeﬁnite acceleration of charge carriers due to the electric ﬁeld. Yet, in a realistic system there are other eﬀects to consider which act in opposition to the particle’s acceleration. These are mainly collisions with defects and impurities, as well as phononic lattice vibrations. The interplay between acceleration through the ﬁeld and scattering at such impurities leads ultimately to a steady-state condition and thus an eﬀective velocity for the charge carrier. Charge transport in such a regime is statistically described by the Boltzmann transport equation, which considers the relative change in the carrier distribution functions f when subjected to an external ﬁeld. Thereby, it accounts for the actions of the ﬁeld: driving the system out of equilibrium, the diﬀusion of the carriers, and collisions of the carriers with phonons and impurities.244

4.1. Eﬀective Mass

As is apparent from eq 55, the eﬀective mass is deﬁned as the reciprocal-space Hessian matrix of the respective energy band. Reference points for the derivatives here are the respective global extrema of the bands in the ﬁrst Brillouin zone,34 i.e., the VBM and CBM. If the extrema do not coincide with the Γpoint (k = (0,0,0)), they can easily be identiﬁed in a conventional band structure plot of the energy bands along a reciprocal space path connecting the high-symmetry points of the Brillouin zone. An example for such a plot is shown in Figure 12. Having identiﬁed the reference point, the next step is to estimate the Hessian matrix. As the band structure is generally not known in a closed analytic form, the derivatives 10336

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

have to be taken numerically along the three reciprocal basis vectors. Unfortunately, in three dimensions this a tedious task due to the mixed derivatives i ≠ j. In an isotropic medium or in the case of only one direction being of interest, there is fortunately a simpler way to estimate the eﬀective mass. Observing that a (nearly) free electron gas model shows a parabolic dependence of the band energy on the reciprocal space vector in the vicinity of the band extremum with energy ε0,34 the following relationship holds

ε(k) = ε0 +

ℏ2 |k|2 2m*

Figure 13. Charge-transfer-relevant directions in a pentacene crystal. Couplings and thus band dispersion in the out-of-plane direction not pictured here are negligible.

(59)

or in the fully anisotropic case ε(k) = ε0 +

1 2

⎛ 1 ⎞ ∑ ∑ ℏ2kikj⎜⎝ ⎟⎠ m* ij i

j

H̃ 22 = 2Hs2 cos k·R s2

̃ = Hn1ei k·R n1 + Hn2ei k·R n2 + Hn3ei k·R n3 + Hn4 ei k·R n4 H12

(60)

(61d)

with the sums running over the three components of the vector k. In this case the eﬀective mass m* can simply be acquired from a parabolic ﬁt to energy eigenvalues calculated for a number of k-points around the extremum. 4.1.1. Tight-Binding Model of Electronic Band Structures. There are a number of electronic structure methods which yield the band structure for a periodic organic solid with varying degrees of accuracy and computational cost. In the semiconductor community, the prevalent method is undoubtedly DFT, but there have also been successful applications of DFTB and semiempirical methods. A straightforward way to determine the eﬀective mass in all these methods proceeds through the explicit calculation of ε(k) at numerous k-points for an extended crystal described in a periodic supercell, and subsequent calculation of numerical derivatives or parabolic ﬁtting. A diﬀerent and computationally much cheaper approach for determining the band structure of organic solids was already suggested in the 1960s by LeBlanc241 and Jortner and co-workers,251 but is still actively developed and used today.252−254 Observing the abundance, eﬃciency, and relative accuracy of methods to determine couplings between charge-localized states of molecular dimers and their respective on-site energies (cf. section 3.7), they devised a tightbinding model on the basis of these states. For a crystal with two molecules sitting at two diﬀerent site types 1 and 2 per unit cell, the band dispersions can then, for instance, be written as252,254 ε(k) =

̃ (k) + H̃ 22(k) H11 2 ̃ (k) − H̃ 22(k))2 (H11 ̃ (k))2 ± + (H12 2

As depicted in Figure 13, Rx are thereby the direction vectors corresponding to the respective couplings listed above. The great advantage of such a model is obviously its closed analytical expression for the band structure. This allows for a direct analytical analysis with respect to extrema andmore importantlyan anaytical calculation of the Hessian matrix and thus the eﬀective mass. The approximations underlying this approach are somewhat similar to those of the hopping model, in that only the ﬁrst neighbor shell of a molecule is included, as opposed to the full periodic structure present in a crystal. 4.2. Relaxation Time

In order to determine the relaxation time within the RTA, one has to consider the exact scattering mechanisms at play. As mentioned earlier, these are mainly elastic collisions of charge carrier wave packets with impurities, as well as with optical and acoustic phonons. If these three mechanisms are statistically independent, the total scattering rate in a direction ithe inverse of the relaxation time tensor element τsiiis simply the sum over the rates of all three events: 1 1 1 1 = imp + opt + ac τiis τii τii τii

(62)

̲ is the relaxation time tensor for impurity scattering, where τimp ̲ and τac̲ are the relaxation time tensors for optical and and τopt acoustic phonon scattering, respectively. All three of these can in general be determined based on Fermi’s golden rule.249 Considering a scattering event that relaxes a charge carrier from state |α,k⟩, where α again enumerates the energy bands and k is the wave vector, to any other state |α′,k′⟩ the rate is249,255 1 2π = τii ℏ

(61a)

where the “+” sign holds for electrons and the “−” sign holds for holes. The coupling functions H̃ nm (n, m = 1, 2) are related to the couplings between the molecular sites in the crystal. If analogously to ref 254we denote the couplings between symmetrically equivalent sites in the crystal as Hs1 and Hs2 for site types 1 and 2, respectively, and we denote the couplings between a central molecule and its four nearest other type neighbors as Hn1, Hn2, Hn3, and Hn4 (n = 1, 2), respectively (cf. Figure 13), the respective periodic couplings H̃ nm in a periodic tight-binding ansatz are given by ̃ = 2Hs1 cos k·R s1 H11

(61c)

∑ |⟨α , k|ΔV̂ |α′, k′⟩|2 δ[εα(k) − εα ′(k′)] α′,k′

⎛ v (α , k) ⎞ × ⎜1 − i ⎟ vi(α′, k′) ⎠ ⎝

(63)

where the last term is a weight function for the scattering angle.256 The operator ΔV̂ appearing in the coupling element between initial and ﬁnal states describes the interaction of the electron with the lattice according to the given scattering mechanism. In the case of lattice impurities, which mainly act as traps for electrons or holes, ΔV̂ would for example be a screened Coulomb operator. To date there are only a few approaches to

(61b) 10337

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

̲ , even less so in the case of molecular accurately determine τimp organic solids. On the other hand, organic crystals displaying high carrier mobilities tend to be relatively pure and defect free. This results in low impurity scattering rates (large elements of ̲ ) as compared to phononic mechanisms. The latter tend to τimp be even more pronounced in organic semiconductors due to their weak binding and thus large thermal ﬂuctuations.257,258 Most theoretical studies therefore focus on electron−phonon scattering as the main mechanism of charge carrier energy dissipation.249,254,259 For such charge-carrier/phonon scattering, ΔV̂ becomes the change of the single electron potential due to a strain on the lattice. In this case, the central matrix element in eq 63 can, for example, be determined via the deformation potential model. ΔV̂ is there taken to depend linearly on strain with a coupling constant D̲ def, the eponymous deformation potential. Most generally, the latter is of course also a tensor of rank 2, but in considering only the diagonal elements of the scattering time tensor, we only need to consider diagonal elements Ddef,ii of the deformation potential. Bardeen and Shockley255 already showed in 1950 that the relaxation rate along a direction i due to acoustic phonons is given by ac τii3D

was derived by Beleznay and co-workers260 and is very similar to the 3D case. Denoting for consistency with the multidimensional cases the direction along which the transport occurs with the index i τi1D =

3(kBT )3/2 Ddef, ii 2(mii*)3/2

Ci1D =

∂ε(k) ∂δli

k=ke

τi

2 1 ∂ Etot V ∂δli 2

2 1 ∂ Etot li ∂δli 2

(65b)

2D

ℏ3ρm vs 2Leff = kBTDi 2mi*

li of the case, the again we by i. It is

(66a)

where ρm denotes the mass density of the 2D system and vs is the velocity of sound in the system. Diﬀerences in this 2D expression from the 1D and 3D cases stem from the fact that here the relaxation expression explicitly includes the degree of localization in the direction perpendicular to the plane of transport. This is owing to the fact that restriction of the wave function to the 2D symmetry leads to quantization in only one direction, but a continuum of Bloch states in the perpendicular direction.261 This is expressed through the localization length Leff

(64a)

(Leff )−1 =

(64b)

∫ dr⊥ |ξ(r⊥)|4

(66b)

where ξ(r⊥) is an envelope function which describes the localization along the perpendicular direction r⊥. In the case of organic molecular crystals, it can often be approximated through the extent of the molecule in this perpendicular direction.254,259 Apart from these small diﬀerences in the underlying equations, the computational approach to determine the relaxation times in 1D and 2D is identical to that in 3D. As ﬁnal remark, note that all of the above relations still rely on a harmonic picture of lattice vibrations, which in weakly bound organic solids might not necessarily be accurate. Improvements over the calculation of purely harmonic phonon modes can be made based on, e.g., the quasi-harmonic approximation by Togo and co-workers,265 where elastic properties and phonon frequencies of a solid also show a direct dependence on the unit cell strain. While not yet applied to organic solids, such an approach should be considered for future studies of band transport in organic solids.

Finally, in contrast to Ddef,ii which is the single electron response to a lattice deformation, C3D i in eq 64a is the crystal’s elastic constant in direction i and therefore a measure for the total energetic response to lattice strain. In a harmonic picture of lattice interactions it is, in a three-dimensional (3D) lattice, given by Ci3D =

(65a)

Here, the prefactor is determined by the length respective unit cell vector. In the two-dimensional relaxation time is generally a (2 × 2) tensor, yet restrict the discussion to the principal axes denoted given by261−264

The deformation potential constant in direction i, Ddef,ii, can in this model straightforwardly be calculated from the response of, e.g., the energy eigenvalue of the band in question (VBM or CBM) at the extremal k-point (ke) to a lattice deformation δli along direction i: Ddef, ii =

2πkBT Ddef, ii 2

with the elastic constant

8π Ci3Dℏ4

=

Ci1Dℏ2 mi*

(64c)

where V is the total volume of the crystal unit cell in the unstrained conﬁguration, and Etot is the total (nuclear and electronic) energy of the unit cell. From a computational viewpoint both C3D and D̲ def are accessible by numerical diﬀerentiation or parabolic and linear ﬁtting procedures, respectively. This also demonstrates the simpliﬁcation brought about by a treatment of band transfer in the principal axes of the crystal. Both parameters necessary to assess the relaxation time can be determined from a number of DFT geometry-optimization calculations in stretched and compressed unit cells.249 With the above equations, it is in total quite straightforward to determine the (RTA) band mobility along the principal axes of a three-dimensional periodic solid. Yet, especially in organic crystals, 254 transport is often constricted to a lower dimensionality, such as one-dimensional (1D) in the case of tightly stacked molecules, or two-dimensional (2D) for molecules that couple only in-plane.254,259 In such cases slightly modiﬁed expressions apply. The one-dimensional expression

4.3. Applications

As discussed above, the coherent bandlike transport regime mostly applies for highly pure and ordered organic solids. While the theoretical foundations have been proposed already in the 1960s, it is only in the past 15 years that band models have increasingly been used to describe the transport in such materials. Cheng and co-workers252 determined the mobility in oligoacene single crystals based on semiempirical estimates of the band structure. Their model ﬁrst explained experimental trends of hole and electron mobilities with regard to conjugation lengths. Similarly, Giuggioli, Andersen, and 10338

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

Kenkre266 rationalized the dependence of the mobility on temperature in pentacene. Northrup259 employed the band model in the deformation potential approximation to address the superior hole transport properties in two thiophene modiﬁcations (DNTT-C10 and BTBT-C12) and thin-ﬁlm pentacene. Later Xi et al.249 employed an analogous approach to predict mobilities of a variety of materials ranging from graphene nanoribbons to oligoacenes, diacene-fused thienothiophenes, and various modiﬁcations thereof. In a comparative study Kobayashi and co-workers254 determined hopping and band mobilities for pentacene, rubrene, and a benzothiophene (C8-BTBT). In line with the theoretical considerations concerning the validity of band and hopping models (see below), as well as with experimental results, they found band transport to be the dominant mechanism at room temperature. Li et al.267 determined the temperature dependence of the eﬀective mass in rubrene from a tight binding approach and successfully reproduced the experimentally observed conductivity behavior. Finally, very recent results revealed bandlike behavior even for weakly coupled directions in highly anisotropic rubrene crystals. In a combined experimental/theoretical study, Blülle and co-workers243 demonstrated a bandlike temperature dependence of the mobility in rubrene for directions perpendicular to the strongly coupled high mobility plane. This was explained as an eﬀect of dynamic disorder, which demonstrates again the need for a careful selection of the correct transport model for a given system.

suﬃcient as zero point vibrations could make polarons unstable as detailed further below.) To put this relation into perspective (see also Figure 14), in molecular crystals the reorganization

Figure 14. Illustration of the interplay of reorganization energy and electronic coupling in a two-state charge transfer model. Adapted from ref 38. Copyright 2013 American Chemical Society.

free energy tends to be rather small, typically around 130 meV in the aforementioned example of fullerene crystals. Equation 67 then implies that a ﬁnite barrier exists only for an electronic coupling of ≲65 meV. Problems arise especially in organic solids with good transport properties, as these are precisely geared toward large coupling and small reorganization energies.38,268 Carrying out computations on a large database of diverse organic crystals, Schober et al.16 have shown that in many compounds electronic coupling values are above the λ/2 threshold. This situation is further complicated when considering lattice vibrations and nuclear quantum eﬀects. Indeed, often already the zero point motion of a large molecule along the charge transfer coordinate may hold suﬃcient energy to “push” it over small activation barriers. For instance, for the prominent case of C60, the corresponding CC stretch of the carbon cage amounts to ≈90 meV of zero point energy. In addition to the existence of a barrier, there is also a dynamic criterion for the validity of a hopping model. Ultimately based on transition state theory, hopping models implicitly assume that, after a hopping event, the nuclear degrees of freedom of the system return to an equilibrium in the new charge state. Yet, for a series of concerted hops, such an equilibration can only occur if the hopping rate is signiﬁcantly lower than the rate of vibrational relaxation. This realization allowed Troisi269 to formulate a criterion on the maximally allowed hopping mobility to still consider a hopping mechanism. To allow a rapid evaluation, the criterion was expressed solely in materials’ properties easily accessible to experiment. For a carrier of charge e in a crystal with a centerof-mass distance between molecules dab, it reads

5. INTERMEDIATE REGIME There are numerous cases of charge transport in organic solids which do not adhere to a mechanism covered by either of the two hitherto discussed, limiting regimes. The charge carrier is neither localized at a given site, nor fully delocalized in a carrier band. With respect to electronic and electron−phonon coupling, this can be seen as an intermediate regime. Before going into more detail on simulation techniques for corresponding intermediate charge transport mechanisms, we brieﬂy summarize the ranges of validity for both limiting cases to point out why neither can yield a fully satisfactory description of charge transport in organic solids. 5.1. Ranges of Validity

5.1.1. Polaronic Hopping Model. In order for a polaronic model to apply, the charge carrier has to exist in a localized form on one or a given (small) number of sites. In organic solids the most natural choice of such sites appears to be individual molecules in the crystal. Leaving the eﬀect of molecular lattice vibrations aside for the moment, a localized state according to the rate theories described by eq 13 exists as long as a barrier ΔG† > 0 separates initial and ﬁnal state. In a perfect periodic crystal without any driving force, the existence of such a barrier rests on the interplay between the electronic coupling and the reorganization energy; cf. Figure 4. The crossing point from positive to vanishing activation energy can for this case be established from eqs 16a and 16b, by determining the root of ΔG‡ with respect to λ and Hab. This yields Hab ≤

1 λ 2

(for ΔG 0 = 0)

μ hop

dab, into the deﬁnition of the mobility, eq 4, leads to the following criterion on μ:

μ band >

dab τsE

(70a)

μ band >

dabq vgm*

(70b)

Figure 16. Illustration of charge carrier localization in a molecular crystal. (top) Carrier probability function |ψ|2 in a fully delocalized band (Bloch) state; (middle) large polaron delocalized over a number of molecular sites; (bottom) small polaron more or less localized on a single site. Normalization of wave functions here is arbitrary for illustration purposes.

such a spread-out state does depend on the temperature and polarizability of the material, and can no longer be described within the conﬁnes of traditional band theory. Eﬀective correction approaches, developed to capture such eﬀects, will be discussed in section 5.2. After that, methods explicitly following the time propagation of the charge carrier wave function, thus yielding an atomistic treatment without any assumptions on the mechanism, will be treated in section 5.3.

Here, E denotes the external applied ﬁeld. As this is not a property of the material, we also provide an equivalent form in eq 70b as a function of the eﬀective mass m* and the group velocity. Compared to the hopping criterion, eq 70b depends on more system speciﬁc parameters, which are not necessarily easily accessible by experiment. To nevertheless provide a rough estimate for the ranges of validity, we used parameters provided by Kobayashi and co-workers254 for three known band conducting materials: highly pure pentacene, rubrene, and 2,7-dioctyl[1]benzothieno[3,2-b][1]benzothiophene, commonly known as C8-BTBT. With group velocities ranging from 5 × 103 to 25 × 103 cm/s and eﬀective masses from 0.6me to 1.3me, we arrive for the aforementioned representative distances of dab = 4−15 Å at a range of minimally allowed

5.2. Polaronic Band Theories

Early approaches to reconcile the eﬀects of nuclear and electronic motions in band theories have been around since the late 1950s in the form of model Hamiltonians; cf. section 4.1.1. In his pioneering work, Holstein122,123 formulated a Hamiltonian that couples electronic states locally to the phononic modes of the system. This basic approach has found many 10340

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

alternative to this ﬁtting procedure, any method outlined in section 3.7 could serve to determine the couplings directly as demonstrated by Troisi for rubrene.282 Parametrization of the Hamiltonian was performed on the level of semiempirical electronic structure calculations based on crystal geometries taken from force ﬁeld MD. This study and earlier work by Girlando and co-workers288 underscored the importance of both Holstein (local) and Peierls (nonlocal) terms for the description of electron−phonon coupling. Finally, it is important to note that the electron−phonon coupling term appearing in the Holstein−Peierls and related models, cf. eq 71, is related to the reorganization free energy contributions of hopping rate theories. Applying the polaron transformation to eq 71 leads to a new Hamiltonian, eq 72, with coupling elements H̃ mn that are modulated by an electron−phonon term. It has been shown13,61 that the leading contribution to this modulating term can be written as a sum over Huang−Rhys factors Sv, which according to eq 26 amounts to the reorganization free energy λ. Together with the electronic coupling Hab, λ thus appears as a deﬁning contribution in hopping, band (via the relaxation time approximation), and intermediate theories. Therefore, they are important, and computationally cheaply accessible, targets for in silico screening approaches.16

applications in the past275−278 and is also undergoing continuous improvement, the most notable being its combination 61,279 with Peierls-type, nonlocal coupling terms.60,280,281 The general form of such a Holstein−Peierls Hamiltonian for tightly bound electrons reads61 HP Ĥ =

∑ Hmnam̂ †an̂ + ∑ ℏωQ ⎛⎝bQ̂ bQ̂ ⎜

mn

+

∑

†

+

Q

† ℏωQ gQmn(bQ̂

1 ⎞⎟ 2⎠

+ b−̂ Q )am̂ †an̂ (71)

mnQ

The three terms in eq 71 are, in order, the electronic term, the phononic term, and the electron−phonon coupling. Thereby, (†) ̂ â(†) m and bQ are the electronic and phononic annihilation (creation) operators, respectively. Sums m and n run over all electronic states which are coupled by Hmn, while Q enumerates phonons of energy ℏωQ and their wave vectors. gQmn, ﬁnally, couples electron and phonon states. A coupling g̲ that is diagonal in m and n corresponds thereby to a local (Holstein) coupling, while a purely nondiagonal g leads to a fully nonlocal (Peierls) model. Correctly parametrized, such a Hamiltonian leads to eigenstates that fully describe a mixed, electronic/nuclear wave function.282 In the past, the parametrization has been successfully achieved by ﬁtting to experimental or theoretical data.61,274,277 Yet, in the form given above, the Hamiltonian does not lend itself to a straightforward ab initio parametrization or even direct diagonalization.61 It is therefore generally transformed into a more suitable basis via the socalled polaron transformation,61,123,283,284 which is unitary and thus norm-conserving.285 In the new basis comprised of electrons and lattice distortions, the explicit electron−phonon coupling terms disappear and the Hamiltonian reads284 HPpol Ĥ =

⎛

†

∑ H̃ mnam̂ †an̂ + ∑ ℏωQ ⎝bQ̂ bQ̂ ⎜

mn

Q

+

1 ⎟⎞ 2⎠

5.3. Propagation of the Charge-Carrier Wave Function

Considering again that the carrier mobility, eq 4, is deﬁned as a function of the average drift velocity only and that, according to the generalized Ehrenfest theorem, the time evolution of such an average is uniquely determined by the Hamiltonian, a direct calculation of μij from a dynamical simulation of the charge carrier is, in principle, possible. Altogether, such an approach amounts to solving the time-dependent Schrödinger equation for the combined nuclear−electronic system. The two most common propagation techniques used in this context are Ehrenfest based mean ﬁeld (MF) dynamics289 and Tully’s surface hopping (SH) method.290−292 It is important to note that both techniques, though semiclassical in that nuclear degrees of freedom are treated classically, are not tied to propagation with model Hamiltonians. Especially SH has been applied in combination with a wide variety of electronic structure methods, ranging from fully ab initio approaches based on multireference conﬁguration interaction,293 conﬁguration interaction,294 and complete active space self-consistent ﬁeld,293,295,296 via DFT (in the form of TDDFT297−299 and open-shell Kohn−Sham300,301), to semiempirical302−306 and tight-binding DFT307−310 approaches. In practice, though, the high computational cost restricts the application of full ab initio methods presently to small (reference) systems.133,145 Note that both charge propagation methods (MF and SH) discussed below are of a semiclassical nature in that nuclear degrees of freedom are treated classically with typically only the charge carrier itself evaluated in a fully quantum mechanical fashion. Such mixed quantum−classical approaches have shown to be an optimal combination of good accuracy and reasonable computational cost for the study of complex interactions between charge carriers and phonons.311 5.3.1. Mean Field Propagation. In the MF or Ehrenfest approach the evolution of the classical nuclear degrees of freedom is governed by the gradient of the expectation value of the system’s total energy. This includes the time-dependent quantum degrees of freedom, described, e.g., by a Hamiltonian such as eq 72. In eﬀect this means that the classical degrees of

(72)

where H̃ mn now represents the coupling of states in the interacting electron−phonon system and as such depends on both the electronic and the electron−phonon coupling constants. In fact, H̃ mn is not simply a number, but instead still contains phonon operators, thus fully including the eﬀect of polaron/phonon scattering.284 Eigenvalues of this Hamiltonian consequently represent the energy levels of the now interacting polaronic electron bands. Given the knowledge of these bands, all the methods outlined in section 4 for determining the charge carrier mobility can be applied as well. In fact, Hannewald and co-workers61 could demonstrate a distinct narrowing of the bandwidth with temperature due to polaronic eﬀects that is not accounted for in standard, T = 0 band theories. This narrowing is due to a decrease of the eﬀective coupling H̃ mnand with it an increase of eﬀective masswith increasing temperature due to a less perfect overlap of molecular orbitals in thermally excited systems.286 Compared to purely electronic band theories, charge carriers in phononic bands are thus eﬀectively heavier, which ultimately leads to a decrease in mobility. In refs 61 and 285 the authors also outline a way to parametrize eq 72 from ground state, ab initio calculations. They ﬁt apurely electronictight binding model of the band structure, cf. eqs 61a−61d, to DFT results in order to obtain the electronic couplings. The electron−phonon coupling is then determined numerically by displacing molecules in the crystal lattice and calculating the change of coupling.287 As an 10341

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

does not change in time. Equation 76, on the other hand, gives zero if the quantum particle delocalizes symmetrically around the origin and the center of charge therefore does not move. The right deﬁnition of the MSD thus has to be chosen based on the problem at hand. As already outlined in section 2.2, the linear section of the MSD function along axis i is directly proportional to the diagonal element Dii of the diﬀusion tensor D̲ of the charge carrier; cf. eq 9. This, in turn can directly be inserted into the Einstein−Smoluchowski equation, eq 6, to yield the mobility. Advantages of the MF approach over other methods, such as the SH scheme described in section 5.3.2, are its simplicity and that it can be derived from ﬁrst principles. Its validity for charge transport simulations, on the other hand, is very much in question. In a general context this has been shown by Tully already in 1998,291 and in the case of charge transfer in organic molecular systems it was reinforced in 2013 by Wang and Beljonne.311 They showed that, while MF does indeed yield diﬀusion tensor elements and thus numerical values of the transfer rates within the correct order of magnitude in the hopping regime, it fails to yield a correct temperature dependence of the carrier mobility. The authors were able to ultimately trace back this failure to an assumption implicitly contained in the MF approach. Use of just a single PES implies an inﬁnite decoherence time of the charge carrier state, which in the localized (hopping) limit of transport mechanisms was shown not to be fulﬁlled at all. Despite these severe shortcomings,315 the MF approach is employed to this day and, if used with care, can lead to physically relevant results.58,59,188,189,282,316−319 5.3.2. Surface Hopping Approaches. The SH algorithm, presented by Tully,290 improves on some aspects over the mean ﬁeld approach. Owing to the method’s great popularity, a number of reviews and various modiﬁcations of the original approach are available in the literature.12,292,320,321 The main diﬀerence with respect to the MF method is that one considers an ensemble of realizations, progressing on a single PES at any time, but with occasional, stochastic transitions (“jumps”) between surfaces instead of one realization of the system evolving on an averaged PES. The motivation for such a treatment is best illustrated with a two-state model as illustrated in Figure 4. There, the dynamics of a carrier wave packet is governed not just by the ground state adiabatic PES, but also by the excited state PES, in case of an incomplete (nonadiabatic) separation of electronic and nuclear degrees of freedom. As outlined above, such a behavior is indeed likely in organic solids and in eﬀect leads to a nonvanishing probability for a wave packet to branch between the PESs. The SH scheme (partially) realizes such a nonzero branching probability through discrete jumps between the PESs. The dynamics of the carrier wave packet is again determined by a time-dependent Schrödinger equation:

freedom move on a single averaged potential energy surface (PES). For a time-dependent QM wave function |ϕ(t)⟩, which in the MF approach is constructed as a coherent superposition of excited states,289 the PES value experienced at time t is thus given by EQM(t) = ⟨ϕ(t)|Ĥ |ϕ(t)⟩. Note that in this notation EQM(t) only contains terms relating to the quantum degrees of freedom and thus leaves out interactions between the classically treated nuclear degrees of freedom. The resulting contribution Eclass(t) can be obtained on the level of a classical force ﬁeld93 (discussed in more detail below) or by coupling the mean ﬁeld approach to an external bath in a Langevin-like approach.311 Given such an averaged, mean ﬁeld PES, the equations of motion for the classical degrees of freedom R are simply Newtonian R̈ i(t ) = − =−

1 ∇i Etot(t ) Mi 1 ∇i [EQM(t ) + Eclass(t )] Mi

(73)

where R̈ i and Mi denote acceleration and mass (in this case that of the charge carrier) along degree of freedom i, and ∇i is the spatial derivative component along i. The time evolution of the QM systemhere the charge carrier wave functionis then given by the time-dependent Schrödinger equation i |ϕ(̇ t )⟩ = − Ĥ |ϕ(t )⟩ (74) ℏ Propagation of the combined system can be carried out with any suitable integration scheme for diﬀerential equations, e.g., the well-known Runge−Kutta integrator,311,312 of at least fourth order.313 For an in-depth analysis of advantages and disadvantages of diﬀerent propagation schemes, we refer the reader to the work of Castro and Marques.314 In order to yield results independent of the chosen initial conditions, the propagation is, in analogy to any other dynamical sampling scheme, generally repeated for a number of diﬀerent initial conditions.311 For the thus resulting ensemble of “trajectories” of the wave function |ϕ(l)(t)⟩, with the superscript l enumerating the trajectories, one then calculates the MSD. Assuming a carrier particle initially fully localized at the origin, Wang and Beljonne showed311 that the MSD can be determined from the width of the charge distribution. In this case the MSD along one of the system’s principal axes i is calculated by evaluating the expectation values of the carrier position operator ri and its square:242 1 MSDi (t ) = L

L

∑ [⟨ϕ(u)(t )|ri 2|ϕ(u)(t )⟩ u=1

− ⟨ϕ(u)(t )|ri|ϕ(u)(t )⟩2 ]

(75)

iℏ|Ψ⟩̇ = ( − iℏad)|Ψ⟩

where L is the total number of trajectories. On the other hand, Spencer and co-workers,93 in simulating the propagation of a charge carrier along a chain of molecules, used the MSD of the center of charge for the calculation of the diﬀusion coeﬃcient MSDi (t ) =

1 L

Here, denotes the adiabatic Hamiltonian matrix (cf. section 3.2) representation in a given basis {|φn⟩}, while ad is the nonadiabatic coupling matrix with elements

L

∑ ⟨ϕ(u)(t )|ri|ϕ(u)(t )⟩2 u=1

(77)

ad dmn =

(76)

Note that both deﬁnitions given here have drawbacks. Equation 75 yields zero for a fully localized quantum particle hopping from one site to the other because there the width

ψm

dψn dt

(78)

Note that basis functions are time dependent due to the general, nonadiabatic nature of the approach, where the motion 10342

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

ﬂuctuations, their interaction is very small, which leads to the occurrence of a cusp on the two PESs pictured as a double cone with the crossing point as common vertex. The nonadiabatic coupling vector between the two states, being inversely proportional to the energy gap, shows a very sharp peak at the crossing and the hopping probability gmn approaches 1. This means that in an exact simulation of the nuclear and electronic dynamics excited states could de-excite simply by going through the vertex. In numerical FSSH runs, however, the cusp can be easily missed due to the ﬁnite nuclear time step. In this case the system does not change state as it should. Consequently, since the state index after and before the crossing remains the same, the new electronic state is now the active state; i.e., a spurious long-range charge transfer has occurred.242,337,338 An insuﬃcient treatment of trivial crossings thus can lead to serious artifacts in the simulated dynamics. To counter this, eﬃcient modiﬁcations to the FSSH scheme have been developed in recent years. The ﬁrst approach is to track trivial crossings along the trajectory, either by detecting unphysical discontinuities of the involved PESs,339 or by following the overlap between the involved adiabatic states at diﬀerent times along the trajectory.337 If indicated, a transition between the PESs is then simply enforced. This approach can be somewhat tedious and becomes ineﬃcient if trivial crossings appear frequently. Second, one can venture to eliminate the interaction between weakly coupled states altogether, by treating only subsystems of the material at hand with FSSH, in the so-called ﬂexible surface hopping scheme.242 Then, all adiabatic states are necessarily physically close, eliminating the possibility of spurious long-range charge transfer. Although the method was applied successfully to simulate CT along a harmonic chain model,242 it is likely to have some limitations. For instance, it may not solve the trivial crossing problem in cases where electronic couplings between physically close diabatic states are very small or when the charge carrier is spatially strongly delocalized. Recently, Prezhdo and co-workers suggested an elegant and eﬀective detection method for trivial crossings based on a rigorous sum rule for hopping probabilities.338 Violation of the sum rule at a given MD step indicates occurrence of a trivial crossing, in which case the hopping probability to the adiabatic state closest in energy to the active adiabatic state is corrected. This method was shown to give excellent results for model systems.338 The only caveat is that it may not provide a correction to the hopping probability where more than two surfaces are involved in a trivial surface crossing. A further drawback of the FSSH approach was shown by recent analyses for small model systems.340,341 These showed that surface hopping does not generally yield the exact equilibrium Boltzmann distribution of electronic states. The deviations from the exact Boltzmann limits, however, were also found to be small especially for systems with small adiabatic energy gaps and/or strong non-adiabatic couplings. Finally, it is evident thatcompared to the single PES considered in the MF approachthe sampling eﬃciency of surface hopping is directly determined by the number of excited state surfaces that need to be included to describe a particular system. In metallic systems, for example,342 FSSH becomes very ineﬃcient due to the large number of PESs contributing to a single band. In this case, hops occur extremely frequently as the energetic separation between the PESs is small at any time, requiring a large number of trajectories for proper sampling.342

of charge carriers represented as the expansion |Ψ⟩ = ∑n cn|ψn⟩ is not time-scale-separated from the nuclear motion. Thus, basis functions localized at the nuclear coordinates cannot be assumed as constant in time during propagation of the carriers. We also point out that eq 77 is in fact identical to eq 74, yet projected onto the adiabatic states of the system. Classical degrees of freedom are again treated simply on the level of Newtonian dynamics; cf. eq 73. The jumps from one adiabatic PES (m) to another (n) then occur with a ﬁnite probability gmn depending on the molecular dynamics time step Δt and the charge carrier’s density matrix amn = cm*cn. gmn = −Δt

ad * dmn 2 Re(amn ) amm

(79)

This particular SH probability is known as the so-called “fewest switches” SH (FSSH) algorithm, as it minimizes the number of transitions between PESs. In this scheme, a single trajectory alone does not carry much physical signiﬁcance due to the stochastic transitions in the dynamics. Averaged over an ensemble of trajectories with appropriately chosen initial conditions, the charge mobility can be estimated similarly to the mean ﬁeld approach.322 Whereas FSSH appears to be a viable approach to the simulation of charge transport in organics, the original method suﬀers from a number of well-known shortcomings compared to a fully quantum mechanical treatment.321,323−326 Standard FSSH, for example, and indeed also the MF approach, do not treat nuclear quantum eﬀects such as tunneling or zero-point motion by construction.290 Recently, though, this limitation has been lifted and nuclear quantum eﬀects have been incorporated into the method by combining it with ring polymer MD.327−329 Additionally, the essential asymmetry between quantum and classical degrees of freedom in this approach can lead to an overly coherent electron dynamics often termed the “decoherence problem”, which can lead to spurious results.323,330,331 The latter can have an especially large impact on charge transfer rates to the point where SH dynamics is not able to recover the Marcus limit if applied to the respective hopping regime.332 This is highly system speciﬁc, though, and studies on simple molecular donor−acceptor complexes, for instance, found the eﬀect of missing decoherence on electron transfer rates to be rather small.86,333 Various methods to correct for the missing decoherence have been suggested. These are, for example, the instant collapse of the electronic wave function to the active state323 or exponential damping of the inactive electronic states as, e.g., used in the coherent switching with decay of mixing approach331 or in the energy-based decoherence correction.320 Landry and Subotnik derived334 an augmentation to the fewest switches SH (a-FSSH) scheme that accounts for the missing electronic decoherence. They demonstrated that by adding a decoherence step, based on a propagation of the ﬁrst moments of the positions and the momenta of the charge carrier, one can indeed recover the correct Marcus behavior.335 This step is indeed just a “collapse” of the wave function that occurs with a probability proportional to the inverse of the so-called coherence time.335 A further problem in practical applications of the original FSSH scheme is its insuﬃcient treatment of so-called trivial and “unavoided” crossings336 between PESs.321 In the context of CT in organic solids they can occur between electronic states that have very small electronic interaction (e.g., when they are far apart). If they come close in energy due to nuclear 10343

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

(MCTDH) method.359,360 This is based on the expansion of the full solution to the time-dependent Schrödinger equation into Hartree products of time-dependent single electron orbitals.361 Inserting this ansatz together with a constraint operator establishing the orthogonality of eigenfunctions at every time step into the Schrödinger equation yields a set of coupled equations for both the single particle orbitals and the expansion coeﬃcients of the full wave function. Given a large enough basis of product functions, MCTDH can thus yield an accurate picture of the time evolution of any prepared initial state. The advantages of MCTDH in the context of this review are thereby twofold. First, the combined electron−nuclear dynamics is fully nonadiabatic and thus in principle not biased toward one speciﬁc CT mechanism.362 The second advantage lies in its systematic improvability, where by adding more product functions one can get an increasingly accurate description. Unfortunately, with the number of product functions the computational cost of MCTDH also grows steeply, which means that early applications were conﬁned to very small systems.360 Yet, recent developments such as multilayer MCTDH,363−365 where the large number of single particle functions is treated in a hierarchical treelike fashion, has reduced the cost of the method such that now thousands of degrees of freedom can be accurately treated for short time scales. First simulations of quantum dynamics of organic systems with MCTDH were reported, e.g., by Burghardt and co-workers,366−368 investigating exciton dynamics and dissociation in oligothiophenes and thiophene−fullerene junctions, or by Zheng et al.369 studying singlet ﬁssion in a pentacene dimer model system. All these studies share their focus on ultrafast processes, owing to the still present resource limitations of the method. A more detailed review of MCTDH and its applications can be found in a focused review by Beck, Jäckle, Worth, and Meyer.361 5.3.4. Example: Propagation in a Charge Localized Basis. To illustrate how explicit time propagation can be realized in practice, we discuss an eﬃcient FSSH scheme recently put forward by Spencer, Gajdos, and Blumberger.93 Inspired by CT rate theory approaches and CDFT, they expand the time-dependent electronic wave function in a basis of charge localized SOMOs. This approach rests on a number of assumptions, ﬁrst and foremost that the excess charge may be described by a one-particle wave function expressed as a linear combination of SOMOs of the molecules. Interactions between carriers were not included in their ﬁrst version, hence limiting its applicability to the low carrier concentration limit. The basis functions |φm⟩ used in the scheme are then analogous to the diabatic states used in rate theoretical approaches (see section 3.1) in that each of them represents a state where the excess charge carrier is entirely localized on a given molecular site. Note that the name “diabatic state” does not strictly apply to such reference states, as they do not diagonalize the nonadiabatic coupling matrix. This is why Spencer and co-workers refer to them as SOMOs. An illustration of this SOMO basis for a fullerene derivative is given in Figure 17. In order to solve the time-dependent Schrödinger equation, eq 77, the wave function |ψ⟩ and thus the Hamiltonian and the nonadiabatic coupling matrix ad are expanded in the SOMO basis for every given snapshot {Rk(t)} of nuclear positions along a trajectory. Comparing to non-adiabatic rate theory, oﬀ-diagonal elements of the Hamiltonian ⟨φm|Ĥ |φn⟩ are in this approach simply given by the electronic coupling elements. These elements can in

Whether or not this will become a problem for the simulation of charge transport in organics remains to be seen. In summary, recent research provided a great number of improvements over the original FSSH scheme, each dealing with diﬀerent shortcomings. For each application the combination of these techniques has to be carefully chosen based on the processes expected to occur. A more in-depth review of FSSH and its state-of-the-art improvements can be found in ref 321. 5.3.3. Other Propagation Methods. Before going on to discuss a speciﬁc example of a combined nuclear−electronic dynamics, we here brieﬂy describe other techniques, which, though not yet as widespread in the ﬁeld of organic solids, can also be employed to model CT processes. 5.3.3.1. Real-Time Time-Dependent DFT. As already mentioned in the introduction to section 5.3, neither MF nor FSSH or its derivatives is limited to speciﬁc descriptions of the electronic degrees of freedom. Although, for the sake of brevity, we have limited the discussion to dynamics based on electronic model Hamiltonians, a more versatile electronic description exists, e.g., in the form of real-time time-dependent DFT (RTTDDFT).343 This is based on the Runge−Gross theorem,344 which is the time-dependent analogue of the ﬁrst Hohenberg− Kohn theorem.345 It states that there is an exact mapping between the time-dependent density ρ(r,t) and the timedependent potential V(r,t) and thus by extension also the timedependent wave function. Yet, analogously to ground state DFT, not every observable can easily be expressed in terms of the density. Thus, based on the work of van Leeuwen,346 one generally employs a reference system of noninteracting, though time-dependent, single electron orbitals with the same density as the full system. This treatment leads to a Hamiltonian comparable to ground state Kohn−Sham DFT347 in that it includes an unknown but time-dependent exchange−correlation (XC) term that needs to be approximated. This is, however, complicated by the fact that the hypothetical “exact” term couples XC contributions at diﬀerent times leading to a memory eﬀect.348,349 A number of studies investigated the eﬀect of memory on RT-TDDFT, for example using an adiabatically exact approximation to the XC potential, which completely neglects XC memory.350−353 Unfortunately, such a simple approach was shown to fail for CT problems,351,353 making it unsuitable for the tasks discussed in this review. Yet there is ongoing research into more accurate approximations to the time-dependent XC functionals, and more in-depth discussion of RT-TDDFT can, for example, be found in ref 343. Finally, while RT-TDDFT provides a way to propagate electronic degrees of freedom, the coupling to nuclear motion is commonly achieved in Ehrenfest-like approaches.289,354,355 Yet, more accurate, though also more expensive, multiconﬁgurational approaches to RT-TDDFT have been reported in the literature.356,357 5.3.3.2. Multiconﬁgurational Time-Dependent SCF Approaches. Propagation of a charge carrier in an extended system with two or more possible states in principle needs to take into account the PESs of all states, as outlined in section 5.3.2. Yet, while the SH and MF approaches treat these in an explicit but stochastic or in an averaged fashion, respectively, the family of multiconﬁgurational time-dependent SCF (MCTDSCF)358 methods represents an approximate but deterministic treatment of time-dependent problems. The most common variant nowadays, which we very brieﬂy discuss here, is the multiconﬁgurational time-dependent Hartree 10344

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

Spencer et al. exploited a number of advantages, such as a possible linear scaling behavior due to the sparsity of the resulting matrices, as well as easy access to the necessary matrix elements for a given nuclear conﬁguration. On top of that, the localized approach somewhat mitigates the well-known chargedelocalization errors of DFT.95,371 Yet, at least in the form presented in ref 93, there are also a number of caveats to such an approach. For example, only intraband CT in the band formed of the SOMOs is considered by construction. Therefore, the dynamics of optical excitations (“excitons”), occurring for example in organic solar cells, could not be addressed with this approach. Moreover and as mentioned previously, no interaction between charge carriers is incorporated yet. In future work, it may be possible to model these eﬀects by suitably expanding the state space of the electronic Hamiltonian.

Figure 17. One-dimensional (1D) illustration of the charge-localized SOMO basis used in the fragment orbital based surface hopping (FOB-SH) approach for a chain of PCBM molecules. Each basis function |φn⟩ is given as a charge carrier (electron or hole) localized on diﬀerent sites in the chain.

5.4. The Kubo Formula

principle be determined with any of the methods discussed in section 3.7. Yet, for practical reasons such as scaling and computational cost, this determination is presently restricted to cheaper methods such as FO-DFT or AOM. The diagonal elements of the Hamiltonian ⟨φm|Ĥ |φm⟩, in turn, represent the site energies of such charge-localized states within the potential of the crystal. As such, they include contributions beyond simple two-site approximations used for the oﬀ-diagonal elements. Again for reasons of computational eﬃciency, Spencer et al. here employ a classical force ﬁeld, which yields the energetics of the charge response to a given localization of the excess electron. Finally, the nonadiabatic coupling elements d′mn(t) between the charge localized states are estimated by ﬁnite diﬀerences from the overlap matrices of the SOMO basis functions taken at diﬀerent times: ′ (t ) = dmn ≈

φm(t )

Finally, we point out that the charge carrier mobility in a material can also be expressed in terms of a time-correlation function of the carrier current I(t) based on the Kubo formula (KF).54,372 Especially considering the relative ambiguity of organic molecular crystals with respect to the carrier transport regime, an unbiased approach based on statistical considerations such as the KF can be of great importance. Indeed, a number of recent studies of organic materials based their approaches on the KF. Ortmann, Bechstedt, and Hannewald,284 for example, applied the KF to a Holstein Hamiltoniancf. eqs 71 and 72to determine carrier mobilities for a realistic model system, showing the temperature-induced transition from hopping-dominated to bandlike transport. Similarly, Fratini and Ciuchi257 employed the KF to determine the carrier mobility in rubrene as a function of temperature, demonstrating the versatility of KF approaches to describe both bandlike and incoherent transport mechanisms. Similarly, Gunnarsson and Han,373 on the other hand, explored the mean free carrier path length in gapless and therefore metallic fullerene crystals. Wang et al.374 employed the related Kubo−Greenwood formalism to study the charge transport properties in diﬀerent phases of polyethylene. In the limit of vanishing momentum transfer from the carrier to the lattice, the KF can be expressed as257

d φ (t ) dt n

1 (⟨φ (t )|φn(t + Δt )⟩ − ⟨φm(t )|φn(t )⟩) Δt m

(80)

These are then transformed into the adiabatic basis to yield the nonadiabatic coupling elements dad mn(t) (cf. eq 78). Here, the analytical time derivative of the basis function |φn(t)⟩ has been replaced by a numerical approximation with a small but ﬁnite time step Δt, which for convenience can be chosen as the time step for the propagation of the nuclei. The thus fully determined Hamiltonian and nonadiabatic coupling matrix cannot yet be used directly for propagation within the SH scheme. For this, they have to be unitary transformed into an orthogonalized basis, for instance through Löwdin’s symmetric approach.211−213 Note that the transformation of the nonadiabatic coupling thereby also necessitates calculation of the time derivative of the transformation matrix, which in the present approach is calculated analogously to ′. With the transformed matrices a prepared initial state is then propagated according to eq 77 using a fourth order Runge−Kutta scheme.370 The necessary nuclear gradients were calculated by Spencer et al. in a mixture of analytical and numerical schemes, as described in detail in ref 93. Given a number of charge trajectories, the carrier mobility was ﬁnally estimated by evaluating the MSD of eq 75 and exploiting the Einstein−Smoluchowski relation, eq 6, in close analogy to the MF approach described in section 5.3.1. By speciﬁcally choosing localized fragment orbitals as basis for the expansion of Hamiltonian and nonadiabatic coupling,

μ=

βπed 2 Zℏ

∫ dω B(ω)e−βω

(81a)

with d the average spacing between crystal sites and B(ω) =

∫ dt eiωt ⟨[I(t ), I(0)]⟩

(81b)

the Fourier transform of the current autocorrelation function. It can be viewed as an energy-resolved, state-speciﬁc mobility function and can be calculated, e.g., from the expectation value of the current operator ∑j ⟨ψ(t)|â†j âj−1 − â†j âj+1|ψ(t)⟩, where â† and â are the creation and annihilation operators and the sum runs over all states. Finally Z=

∫ dω ρ(ω)e−βω

(81c)

with the density of states ρ(ω). Gunnarsson and Han373 demonstrated that the correlation function B(ω)by neglecting so-called vertex correctionscan be factorized into Green’s function terms and matrix elements of the current operator, both averaged over the phonon displacement spectrum. Using 10345

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

this, Fratini and Ciuchi257 further simpliﬁed the calculation of B(ω) to just the calculation of the system’s Green’s function, observing that the latter term can be determined analytically. Moreover, Wang and co-workers374 demonstrated that using a result from Kubo−Greenwood theory372,375,376 one can reduce the computational complexity even further, essentially replacing the current correlation function with a mean square momentum matrix element between pairs of diﬀerent states, averaged over all states.

dynamical approaches to study polaron transport along polymer chains. In another recent approach, Bauer et al.384 used a multiagent quantum Monte Carlo model to model charge transport through disordered multiphase ﬁeld eﬀect transistors consisting of C60 molecules sitting on a layer of alkyl chains.

6. SYNOPSIS, REMAINING CHALLENGES, AND FUTURE DIRECTIONS In the present review, we set out to provide a comprehensive overview of the tools currently available to the computational scientist to tackle the study of charge carrier transport in molecular organic semiconductors. To this end we ﬁrst gave a summary of the theories of conductivity in section 2, highlighting the diﬀerent regimes of transport occurring in organic semiconductors. Then we elaborated them in detail in subsequent sections. In section 3 we ﬁrst detailed the theoretical background of the hopping model, thereby pointing out the diﬀerent limiting cases of hopping rate theories available in the literature. This discussion included all common computational methods available to determine the parameters going into rate theories for an ab initio calculation of charge carrier mobilities within the hopping model. Where the hopping model assumes a localized, polaronic charge carrier, band theory rests on the opposing assumption of a delocalization of carriers in periodic bands. Corresponding approaches were described in section 4. There we again ﬁrst detailed the theoretical foundations of the model before giving an overview of computational methods available in the theorist’s toolbox. Applicability of either model rests on the intricate interplay of charge transfer parameters in each semiconductor. Which model to apply is therefore not necessarily possible to decide beforehand; in some cases even the use of neither model can reasonably be justiﬁed. In such intermediate cases, dynamic simulations as described in section 5 have to be employed. To set this regime into perspective, we ﬁrst discussed in detail the ranges of validity of the limiting carrier transport regimes. Available methods for the intermediate regime comprise the propagation of model Hamiltonians or the explicit propagation of the wave function. Finally, we ended the main part of this review with a discussion of the famous Kubo transport equation in section 5.4, which represents a statistical approach to charge transport in solids, considering time-correlation functions of the charge current. Given such a wealth of methods available to the theoretical researcher, one would be tempted to assume that most challenges in simulating organic semiconductors have been overcome and one can readily employ theoretical methods to predict charge transfer parameters of realistic organic solids. As we have pointed out repeatedly, this is unfortunately not the case. Direct comparison of absolute mobilities to experiment is still only rarely possible for several reasons. On the theoretical side, as pointed out in section 5.1, the exact mechanism underlying charge carrier transport in a system is often unclear or even ill-deﬁned. In such cases only propagation methods discussed in section 5can in principle deliver an unbiased picture. Yet even such methods rest on a number of approximations, given the large sizes of organic molecular systems. On the other hand, experimental studies have their own unique set of challenges to contend with. For instance, mobility measurements of one and the same system can deliver wildly diﬀering values mostly due to minute diﬀerences in preparation, leading to ill-deﬁned or disordered crystal

5.5. Applications

Driven by an increasing awareness that neither hopping nor band models alone are able to fully explain experimentally reported ﬁndings, there has been a strong shift toward the more general approaches in the past decade. As already mentioned in section 5.2. Hannewald and co-workers61,279 conducted seminal studies of polaronic bandwidth narrowing in oligoacene molecular crystals (naphthalene, anthracene, and tetracene) based on a Holstein−Peierls Hamiltonian. Troisi and Orlandi274,316 subsequently showed, for the examples of pentacene and anthracene, that the thermal modulation of the electronic couplings entering such model Hamiltonians cannot be neglected. Next to polaronic band theories, especially nonadiabatic propagation of the charge carrier wave function has been employed to study transport in organic crystals. Troisi282 demonstrated the accuracy of such approaches versus experiments for the absolute charge mobility in rubrene. Using a mixed quantum/classical approach315 based on SH, Wang and Beljonne242,311 studied the crossover from hopping to bandlike transport in organic crystals. Demonstrating the versatility of the method, Ren and co-workers377 also employed nonadiabatic MD to simulate charge transport in two-dimensional pentathiophene butyric acid monolayers to determine the underlying mechanisms of charge transport in such conﬁned systems. Based on a quantized Hamiltonian dynamics, ﬁrst Hannewald and Bobbert,279 and later again Wang et al.378 explained low-temperature experimental results for charge transport in naphthalene crystals. Zhang, Zhong, and Zhao379 employed a time-dependent wave-packet method to explain electron mobilities in pentacene−quinone derivatives, also ﬁnding a crossover from hopping to bandlike behavior. For chains of ethylene-like molecules Spencer et al.86,93 demonstrated that their just-discussed fragment-orbital-based nonadiabatic SH method achieves comparable accuracy to these earlier and computationally more expensive methods. A conceptually similar method, brought forward by Heck and co-workers,188,189 also utilizes a fragment orbital description, based on DFTB, to arrive at an analogous eﬀective QM−MM single-particle description of the charge carrier. In contrast to the FOB-SH, Heck et al. propagated the charge carrier with Ehrenfest dynamics, which has a number of well-known deﬁciencies (cf. section 5.3.1). Nonetheless, the charge mobility computed for chains of organic molecules was in good agreement with experimental data, where available. Finally, dynamical approaches to charge transport are not limited to periodic crystalline materials. For example, Akimov194 utilized a fragment orbital scheme based on semiempirical extended Hückel theory in the nonadiabatic SH propagation of an eﬀective QM−MM Hamiltonian of a molecular donor−acceptor heterojunction of boron subphthalocyanine chloride and C60.380 Johansson and Stafström381,382 as well as An, Wu, and Sun383 employed nonadiabatic 10346

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

In conclusion, then, what is the ideal method to describe CT? Unfortunately, there is no simple answer to this question, as the ideal method will always depend on the system, the regime, the available resources, and ﬁnally the exact question one wants to answer. In general, an ideal theory should yield the transport mechanism as a result and not assume one in the ﬁrst place. This in turn points toward the methods discussed in section 5. At the same time one ideally would like to be able to treat large or even disordered systems which, given even today’s computing resources, can be a challenge for methods relying on direct charge propagation. On the other hand, as outlined in section 5.2, if one is only interested in broad mobility trends in a screening study, in principle only few parameters have to be calculated per system. Then a full nonadiabatic dynamics clearly would go far beyond what is necessary in practice. Thus, the question at hand as well as the system and the available resources inform the choice of method to be used and with this review the authors aimed at providing a guide to the available approaches in the diﬀerent regimes for the reader to choose from.

structures. Many theoretical studies nowadays recognize the problem and introduce models for the inﬂuence of structural disorder on electronic couplings, section 3.7, and on-site energies, section 3.3.1, which indeed show ﬁrst successes. Similarly, dynamical inﬂuences on carrier localization and propagation, through electron−phonon coupling, section 4.2, and a certain degree of dynamical disorder, are gathering increased attention for more reﬁned modeling studies. Another challenge for the comparison of theory and experiment is interface eﬀects. While this review concentrated mainly on techniques for the study of bulk charge transport phenomena, virtually every real-life application of such systemsand thus also experimental measurementsneeds to interface the semiconducting organic solid with metal electrodes. Disregarding for the moment the problem of structural modeling of the interface, transport across such interfaces is by necessity harder to model, as one needs to combine methods suited for metallic systems with those geared toward molecular transport. In the case of single-molecule/ metal interfaces, a great variety of theoretical studies can be found in the literature due to their potential application in molecular electronics. Yet, with regard to the theory of charge carrier propagation across bulk interfaces between organic solids and metals, there is still much work to be done. Another important aspect is the geometric structure, which necessarily underlies all theoretical studies. While this review focused on ordered organic solids, the class of amorphous or polymeric organic solids is of high interest for applications in display devices, electronics, and even solar cells. The ill-deﬁned microscopic structure of such materials poses a signiﬁcant challenge to any atomically resolved modeling. One way to obtain representative structures used for charge transport calculations is to perform MD simulations, possibly performed at elevated temperatures and based on approximate energetics, to lower the computational burden. Snapshots drawn from the computed trajectories then provide an ensemble of structures which can then be treated using the methods outlined in this review, ultimately yielding a distribution of charge transport parameters. While amorphous semiconductors could in principle also be tackled through such snapshots, sampling the likely nonequilibrium distribution of their structures poses a practical problem. Such a discrepancy in structure distributions can thus potentially lead to large discrepancies between experiment and theory. Finally, one of the great advantages of theory, even given all of the problems outlined in the paragraphs above, is to point out trends and thus provide a link between the structure and function of a material. Given such a link, one could think of employing a number of easily computable parameters for a given system, such as coupling and reorganization energy as discussed in section 5.2, to at least roughly predict its applicability as an organic semiconductor relative to other materials in a computational screening study. Yet, as before, such screening approaches again depend on the knowledge of the microscopic structure of the material, which in principle limits their applicability to already known systems. Luckily, the past couple of years saw great leaps in crystal structure prediction methodology, which brought us to the point where, for any molecule, one can predict to a great degree of accuracy the corresponding crystal structure.22 While these prediction studies tend to be costly, theoretical predictability of charge transport properties for unknown systems is now deﬁnitely within our reach.

AUTHOR INFORMATION Corresponding Author

*E-mail: [email protected]. ORCID

Harald Oberhofer: 0000-0002-5791-6736 Notes

The authors declare no competing ﬁnancial interest. Biographies Harald Oberhofer is a group leader at the Chair for Theoretical Chemistry, Technische Universität München. His research is primarily focused on reactions involving charge transport in both organic and inorganic solids as well as across solid−liquid interfaces. He received his Ph.D. in physics in 2008 from the University of Vienna, working on nonequilibrium statistical mechanics under the supervision of Prof. Christoph Dellago. He then joined the group of Prof. Jochen Blumberger at Cambridge University for a three-year postdoctoral stay. There he ﬁrst became interested in the simulation of charge carrier transport, which he is working on to this day. In 2011 he joined the group of Prof. Karsten Reuter at Technische Universität München ﬁrst as an Alexander von Humboldt postdoctoral research fellow and then as a group leader. Karsten Reuter holds the Chair for Theoretical Chemistry at Technische Universität München (TUM), is an adjunct professor in the TUM Physics Department, and is aﬃliated with the TUM Catalysis Research Center. His research interests center on a quantitative multiscale modeling of properties and functions in materials, catalysis, and energy. He received his Ph.D. in physics from the Universität Erlangen−Nürnberg in 1998. After postdoctoral stays at the Fritz-Haber-Institut der Max-Planck-Gesellschaft in Berlin and the FOM-Institut for Atomic and Molecular Physics in Amsterdam, he headed an independent junior research group at the Fritz-Haber-Institut until moving to TUM in 2009. In 2014−2015 he was a visiting professor at the Chemical Engineering Department of Stanford University. Jochen Blumberger’s research interests focus on the development and application of quantum and classical molecular simulation methods to study redox and charge transfer reactions in biological systems, organic semiconductors, and most recently also at solid/liquid interfaces. He obtained his Ph.D. in 2005 from Cambridge University, U.K., where he 10347

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

(16) Schober, C.; Reuter, K.; Oberhofer, H. Virtual Screening for High Carrier Mobility in Organic Semiconductors. J. Phys. Chem. Lett. 2016, 7, 3973−3977. (17) Lommerse, J. P. M.; Motherwell, W. D. S.; Ammon, H. L.; Dunitz, J. D.; Gavezzotti, A.; Hofmann, D. W. M.; Leusen, F. J. J.; Mooij, W. T. M.; Price, S. L.; Schweizer, B.; et al. A Test of Crystal Structure Prediction of Small Organic Molecules. Acta Crystallogr., Sect. B: Struct. Sci. 2000, 56, 697−714. (18) Motherwell, W. D. S.; Ammon, H. L.; Dunitz, J. D.; Dzyabchenko, A.; Erk, P.; Gavezzotti, A.; Hofmann, D. W. M.; Leusen, F. J. J.; Lommerse, J. P. M.; Mooij, W. T. M.; et al. Crystal Structure Prediction of Small Organic Molecules: A Second Blind Test. Acta Crystallogr., Sect. B: Struct. Sci. 2002, 58, 647−661. (19) Day, G. M.; Motherwell, W. D. S.; Ammon, H. L.; Boerrigter, S. X. M.; Della Valle, R. G.; Venuti, E.; Dzyabchenko, A.; Dunitz, J. D.; Schweizer, B.; van Eijck, B. P.; et al. A Third Blind Test of Crystal Structure Prediction. Acta Crystallogr., Sect. B: Struct. Sci. 2005, 61, 511−527. (20) Day, G. M.; Cooper, T. G.; Cruz-Cabeza, A. J.; Hejczyk, K. E.; Ammon, H. L.; Boerrigter, S. X. M.; Tan, J. S.; Della Valle, R. G.; Venuti, E.; Jose, J.; et al. Significant Progress in Predicting the Crystal Structures of Small Organic Molecules − A Report on the Fourth Blind Test. Acta Crystallogr., Sect. B: Struct. Sci. 2009, 65, 107−125. (21) Bardwell, D. A.; Adjiman, C. S.; Arnautova, Y. A.; Bartashevich, E.; Boerrigter, S. X. M.; Braun, D. E.; Cruz-Cabeza, A. J.; Day, G. M.; Della Valle, R. G.; Desiraju, G. R.; et al. Towards Crystal Structure Prediction of Complex Organic Compounds - A Report on the Fifth Blind Test. Acta Crystallogr., Sect. B: Struct. Sci. 2011, 67, 535−551. (22) Reilly, A. M.; Cooper, R. I.; Adjiman, C. S.; Bhattacharya, S.; Boese, A. D.; Brandenburg, J. G.; Bygrave, P. J.; Bylsma, R.; Campbell, J. E.; Car, R.; et al. Report on the Sixth Blind Test of Organic Crystal Structure Prediction Methods. Acta Crystallogr., Sect. B: Struct. Sci., Cryst. Eng. Mater. 2016, 72, 439−459. (23) Wales, D. J.; Scheraga, H. A. Global Optimization of Clusters, Crystals, and Biomolecules. Science 1999, 285, 1368−1372. (24) Wales, D. Energy Landscapes: Applications to Clusters, Biomolecules and Glasses; Cambridge University Press: 2003. (25) Kwiatkowski, J. J.; Frost, J. M.; Nelson, J. The Effect of Morphology on Electron Field-Effect Mobility in Disordered C60 Thin Films. Nano Lett. 2009, 9, 1085−1090. (26) MacKenzie, R. C.; Frost, J. M.; Nelson, J. A Numerical Study of Mobility in Thin Films of Fullerene Derivatives. J. Chem. Phys. 2010, 132, 064904. (27) Rühle, V.; Lukyanov, A.; May, F.; Schrader, M.; Vehoff, T.; Kirkpatrick, J.; Baumeier, B.; Andrienko, D. Microscopic Simulations of Charge Transport in Disordered Organic Semiconductors. J. Chem. Theory Comput. 2011, 7, 3335−3345. (28) Baumeier, B.; May, F.; Lennartz, C.; Andrienko, D. Challenges for In Silico Design of Organic Semiconductors. J. Mater. Chem. 2012, 22, 10971−10976. (29) Silinsh, E. A. Organic Molecular Crystals: Their Electronic States; Springer Science & Business Media: 2012; Vol. 16. (30) Nazin, G.; Qiu, X.; Ho, W. Vibrational Spectroscopy of Individual Doping Centers in a Monolayer Organic Crystal. J. Chem. Phys. 2005, 122, 181105−181105. (31) Giovannetti, G.; Brocks, G.; van den Brink, J. Ab Initio Electronic Structure and Correlations in Pristine and PotassiumDoped Molecular Crystals of Copper Phthalocyanine. Phys. Rev. B: Condens. Matter Mater. Phys. 2008, 77, 035133. (32) Takeya, J.; Yamada, K.; Hara, K.; Shigeto, K.; Tsukagoshi, K.; Ikehata, S.; Aoyagi, Y. High-Density Electrostatic Carrier Doping in Organic Single-Crystal Transistors with Polymer Gel Electrolyte. Appl. Phys. Lett. 2006, 88, 112102. (33) Gregg, B. A.; Cormier, R. A. Doping Molecular Semiconductors: N-Type Doping of a Liquid Crystal Perylene Diimide. J. Am. Chem. Soc. 2001, 123, 7959−7960. (34) Kittel, C. Introduction to Solid State Physics, 7th ed.; John Wiley & Sons, Inc.: 1996.

worked on density functional based molecular dynamics simulation of redox reactions, under the supervision of Prof. Michiel Sprik. After a two-year postdoctoral stay with Prof. Michael L. Klein at the University of Pennsylvania, he returned to Cambridge in 2006 on a Royal Society University Research Fellowship. In 2009 he moved to University College London (UCL), Department of Physics and Astronomy, where he was appointed university lecturer (2009), reader (2013), and professor in chemical physics (2015). He has recently been awarded an ERC Consolidator grant (2016) and currently holds a Hans Fischer Fellowship at the Institute of Advanced Studies at Technische Universität München.

ACKNOWLEDGMENTS H.O. and K.R. gratefully acknowledge support from the Solar Technologies Go Hybrid Initiative of the State of Bavaria. With the support of the Technische Universität MünchenInstitute for Advanced Study (TUM-IAS), funded by the German Excellence Initiative and the European Union Seventh Framework Programme under Grant Agreement No. 291763. J.B. acknowledges the European Union for cofunding of a TUM-IAS Hans-Fischer Fellowship. Finally, the authors thank Christoph Schober, Christoph Scheurer, and Wolfgang Domcke for their valuable input and insightful discussions. REFERENCES (1) Forrest, S. R. The Path to Ubiquitous and Low-Cost Organic Electronic Appliances on Plastic. Nature 2004, 428, 911−918. (2) Gundlach, D. J. Organic Electronics: Low Power, High Impact. Nat. Mater. 2007, 6, 173−174. (3) Minemawari, H.; Yamada, T.; Matsui, H.; Tsutsumi, J.; Haas, S.; Chiba, R.; Kumai, R.; Hasegawa, T. Inkjet Printing of Single-Crystal Films. Nature 2011, 475, 364−367. (4) Sun, Y.; Welch, G. C.; Leong, W. L.; Takacs, C. J.; Bazan, G. C.; Heeger, A. J. Solution-Processed Small-Molecule Solar Cells with 6.7% Efficiency. Nat. Mater. 2012, 11, 44−48. (5) Anikeeva, P.; Koppes, R. A. Restoring the Sense of Touch. Science 2015, 350, 274−275. (6) Stavrinidou, E.; Gabrielsson, R.; Gomez, E.; Crispin, X.; Nilsson, O.; Simon, D. T.; Berggren, M. Electronic Plants. Sci. Adv. 2015, 1, e1501136. (7) Newton, M. D.; Sutin, N. Electron Transfer Reactions in Condensed Phases. Annu. Rev. Phys. Chem. 1984, 35, 437−480. (8) Nitzan, A. Electron Transmission through Molecules and Molecular Interfaces. Annu. Rev. Phys. Chem. 2001, 52, 681−750. (9) Brédas, J.-L.; Beljonne, D.; Coropceanu, V.; Cornil, J. ChargeTransfer and Energy-Transfer Processes in π-conjugated Oligomers and Polymers: a Molecular Picture. Chem. Rev. 2004, 104, 4971−5004. (10) Coropceanu, V.; Cornil, J.; da Silva Filho, D. A.; Olivier, Y.; Silbey, R.; Brédas, J.-L. Charge Transport in Organic Semiconductors. Chem. Rev. 2007, 107, 926−952. (11) Van Voorhis, T.; Kowalczyk, T.; Kaduk, B.; Wang, L.-P.; Cheng, C.-L.; Wu, Q. The Diabatic Picture of Electron Transfer, Reaction Barriers, and Molecular Dynamics. Annu. Rev. Phys. Chem. 2010, 61, 149−170. (12) Akimov, A. V.; Neukirch, A. J.; Prezhdo, O. V. Theoretical Insights into Photoinduced Charge Transfer and Catalysis at Oxide Interfaces. Chem. Rev. 2013, 113, 4496−4565. (13) Zhugayevych, A.; Tretiak, S. Theoretical Description of Structural and Electronic Properties of Organic Photovoltaic Materials. Annu. Rev. Phys. Chem. 2015, 66, 305−330. (14) Blumberger, J. Recent Advances in the Theory and Molecular Simulation of Biological Electron Transfer Reactions. Chem. Rev. 2015, 115, 11191−11238. (15) Groom, C. R.; Bruno, I. J.; Lightfoot, M. P.; Ward, S. C. The Cambridge Structural Database. Acta Crystallogr., Sect. B: Struct. Sci., Cryst. Eng. Mater. 2016, 72, 171−179. 10348

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

(56) Girifalco, L. A. Statistical Mechanics of Solids; Oxford University Press: 2003; Vol. 58. (57) Frenkel, D.; Smit, B. Understanding Molecular Simulation: From Algorithms to Applications; Academic Press: 2001; Vol. 1. (58) Troisi, A.; Cheung, D. L.; Andrienko, D. Charge Transport in Semiconductors with Multiscale Conformational Dynamics. Phys. Rev. Lett. 2009, 102, 116602. (59) Troisi, A.; Cheung, D. L. Transition from Dynamic to Static Disorder in One-Dimensional Organic Semiconductors. J. Chem. Phys. 2009, 131, 014703. (60) Su, W.; Schrieffer, J.; Heeger, A. J. Solitons in Polyacetylene. Phys. Rev. Lett. 1979, 42, 1698. (61) Hannewald, K.; Stojanović, V.; Schellekens, J.; Bobbert, P.; Kresse, G.; Hafner, J. Theory of Polaron Bandwidth Narrowing in Organic Molecular Crystals. Phys. Rev. B: Condens. Matter Mater. Phys. 2004, 69, 075211. (62) Fornari, R. P.; Troisi, A. Theory of Charge Hopping along a Disordered Polymer Chain. Phys. Chem. Chem. Phys. 2014, 16, 9997− 10007. (63) Zhugayevych, A.; Postupna, O.; Bakus, R. C., II; Welch, G. C.; Bazan, G. C.; Tretiak, S. Ab Initio Study of a Molecular Crystal for Photovoltaics: Light Absorption, Exciton and Charge Carrier Transport. J. Phys. Chem. C 2013, 117, 4920−4930. (64) Keck, J. C. Variational Theory of Reaction Rates; Wiley Online Library: 1967. (65) Miller, W. H. Quantum Mechanical Transition State Theory and a New Semiclassical Model for Reaction Rate Constants. J. Chem. Phys. 1974, 61, 1823−1834. (66) Mones, L.; Kulhánek, P.; Simon, I.; Laio, A.; Fuxreiter, M. The Energy Gap as a Universal Reaction Coordinate for the Simulation of Chemical Reactions. J. Phys. Chem. B 2009, 113, 7867−7873. (67) Mones, L.; Csányi, G. Topologically Invariant Reaction Coordinates for Simulating Multistate Chemical Reactions. J. Phys. Chem. B 2012, 116, 14876−14885. (68) Zusman, L. Outer-Sphere Electron Transfer in Polar Solvents. Chem. Phys. 1980, 49, 295−304. (69) Warshel, A. Dynamics of Reactions in Polar Solvents. Semiclassical Trajectory Studies of Electron-Transfer and ProtonTransfer Reactions. J. Phys. Chem. 1982, 86, 2218−2224. (70) Kakitani, T.; Mataga, N. Comprehensive Study on the Role of Coordinated Solvent Mode Played in Electron-Transfer Reactions in Polar Solutions. J. Phys. Chem. 1987, 91, 6277−6285. (71) Kuharski, R. A.; Bader, J. S.; Chandler, D.; Sprik, M.; Klein, M. L.; Impey, R. W. Molecular Model for Aqueous Ferrous-Ferric Electron Transfer. J. Chem. Phys. 1988, 89, 3248−3257. (72) Carter, E. A.; Hynes, J. T. Solute-Dependent Solvent Force Constants for Ion Pairs and Neutral Pairs in a Polar Solvent. J. Phys. Chem. 1989, 93, 2184−2187. (73) Tachiya, M. Relation Between the Electron-Transfer Rate and the Free Energy Change of Reaction. J. Phys. Chem. 1989, 93, 7050− 7052. (74) King, G.; Warshel, A. Investigation of the Free Energy Functions for Electron Transfer Reactions. J. Chem. Phys. 1990, 93, 8682−8692. (75) Tateyama, Y.; Blumberger, J.; Sprik, M.; Tavernelli, I. DensityFunctional Molecular-Dynamics Study of the Redox Reactions of Two Anionic, Aqueous Transition-Metal Complexes. J. Chem. Phys. 2005, 122, 234505. (76) Cheng, J.; Sulpizi, M.; Sprik, M. Redox Potentials and pKa for Benzoquinone from Density Functional Theory Based Molecular Dynamics. J. Chem. Phys. 2009, 131, 154504. (77) Vuilleumier, R.; Tay, K. A.; Jeanmairet, G.; Borgis, D.; Boutin, A. Extension of Marcus Picture for Electron Transfer Reactions with Large Solvation Changes. J. Am. Chem. Soc. 2012, 134, 2067−2074. (78) Stecher, T.; Reuter, K.; Oberhofer, H. First-Principles FreeEnergy Barriers for Photoelectrochemical Surface Reactions: Proton Abstraction at TiO 2 (110). Phys. Rev. Lett. 2016, 117, 276001. (79) Moens, J.; Seidel, R.; Geerlings, P.; Faubel, M.; Winter, B.; Blumberger, J. Energy Levels and Redox Properties of Aqueous Mn2+/3+ from Photoemission Spectroscopy and Density Functional

(35) Nitzan, A. Chemical Dynamics in Condensed Phases: Relaxation, Transfer and Reactions in Condensed Molecular Systems; Oxford University Press: 2006. (36) Atkins, P.; de Paula, J. Physical Chemistry; Oxford University Press: 2006. (37) Oberhofer, H.; Blumberger, J. Revisiting Electronic Couplings and Incoherent Hopping Models for Electron Transport in Crystalline C60 at Ambient Temperatures. Phys. Chem. Chem. Phys. 2012, 14, 13846−13852. (38) Gajdos, F.; Oberhofer, H.; Dupuis, M.; Blumberger, J. On the Inapplicability of Electron-Hopping Models for the Organic Semiconductor Phenyl-C61-Butyric Acid Methyl Ester (PCBM). J. Phys. Chem. Lett. 2013, 4, 1012−1017. (39) Ahrenkiel, R.; Dunlavy, D.; Greenberg, D.; Schlupmann, J.; Hamaker, H.; MacMillan, H. Electron Mobility in p-GaAs by Time of Flight. Appl. Phys. Lett. 1987, 51, 776−778. (40) Campbell, I.; Smith, D.; Neef, C.; Ferraris, J. Consistent Timeof-Flight Mobility Measurements and Polymer Light-Emitting Diode Current {endash} Voltage Characteristics. Appl. Phys. Lett. 1999, 74, 2809−2811. (41) Campbell, A. J.; Bradley, D. D.; Antoniadis, H. Dispersive Electron Transport in an Electroluminescent Polyfluorene Copolymer Measured by the Current Integration Time-of-Flight Method. Appl. Phys. Lett. 2001, 79, 2133−2135. (42) Choulis, S.; Nelson, J.; Kim, Y.; Poplavskyy, D.; Kreouzis, T.; Durrant, J.; Bradley, D. Investigation of Transport Properties in Polymer/Fullerene Blends Using Time-of-Flight Photocurrent Measurements. Appl. Phys. Lett. 2003, 83, 3812−3814. (43) Iino, H.; Hanna, J.; Bushby, R. J.; Movaghar, B.; Whitaker, B. J.; Cook, M. J. Very High Time-of-Flight Mobility in the Columnar Phases of a Discotic Liquid Crystal. Appl. Phys. Lett. 2005, 87, 132102. (44) Spear, W. E. Drift Mobility Techniques for the Study of Electrical Transport Properties in Insulating Solids. J. Non-Cryst. Solids 1969, 1, 197−214. (45) Lebedev, E.; Dittrich, T.; Petrova-Koch, V.; Karg, S.; Brütting, W. Charge Carrier Mobility in Poly (p-phenylenevinylene) Studied by the Time-of-Flight Technique. Appl. Phys. Lett. 1997, 71, 2686−2688. (46) Tiwari, S.; Greenham, N. Charge Mobility Measurement Techniques in Organic Semiconductors. Opt. Quantum Electron. 2009, 41, 69−89. (47) Friedman, L.; Pollak, M. Hall Mobility Due to Hopping-Type Conduction in Disordered Systems. Philos. Mag. B 1978, 38, 173−189. (48) Podzorov, V.; Menard, E.; Rogers, J.; Gershenson, M. Hall Effect in the Accumulation Layers on the Surface of Organic Semiconductors. Phys. Rev. Lett. 2005, 95, 226601. (49) Shuttle, C. G.; Hamilton, R.; Nelson, J.; O’Regan, B. C.; Durrant, J. R. Measurement of Charge-Density Dependence of Carrier Mobility in an Organic Semiconductor Blend. Adv. Funct. Mater. 2010, 20, 698−702. (50) An, Z.; Yu, J.; Jones, S. C.; Barlow, S.; Yoo, S.; Domercq, B.; Prins, P.; Siebbeles, L. D.; Kippelen, B.; Marder, S. High Electron Mobility in Room-Temperature Discotic Liquid-Crystalline Perylene Diimides. Adv. Mater. 2005, 17, 2580−2583. (51) Schouten, P. G.; Warman, J. M.; de Haas, M. P. Effect of Accumulated Radiation Dose on Pulse Radiolysis Conductivity Transients in a Mesomorphic Octa-n-alkoxy-substituted Phthalocyanine. J. Phys. Chem. 1993, 97, 9863−9870. (52) Mozer, A. J.; Dennler, G.; Sariciftci, N.; Westerling, M.; Pivrikas, A.; Ö sterbacka, R.; Juška, G. Time-Dependent Mobility and Recombination of the Photoinduced Charge Carriers in Conjugated Polymer/Fullerene Bulk Heterojunction Solar Cells. Phys. Rev. B: Condens. Matter Mater. Phys. 2005, 72, 035217. (53) Juška, G.; Genevičius, K.; Nekrašas, N.; Sliaužys, G.; Dennler, G. Trimolecular Recombination in Polythiophene: Fullerene Bulk Heterojunction Solar Cells. Appl. Phys. Lett. 2008, 93, 143303. (54) Kubo, R.; Toda, M.; Hashitsume, N. Statistical Physics II. Nonequilibrium Statistical Mechanics; Springer Verlag: Berlin, 1991. (55) Furo, I.; Dvinskikh, S. V. NMR Methods Applied to Anisotropic Diffusion. Magn. Reson. Chem. 2002, 40, S3−S14. 10349

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

Molecular Dynamics Simulation. J. Phys. Chem. B 2010, 114, 9173− 9182. (80) Seidel, R.; Faubel, M.; Winter, B.; Blumberger, J. Single-Ion Reorganization Free Energy of Aqueous Ru (bpy) 32+/3+ and Ru (H2O) 62+/3+ from Photoemission Spectroscopy and Density Functional Molecular Dynamics Simulation. J. Am. Chem. Soc. 2009, 131, 16127−16137. (81) Brunschwig, B. S.; Logan, J.; Newton, M. D.; Sutin, N. A Semiclassical Treatment of Electron-Exchange Reactions. Application to the Hexaaquoiron (II)-Hexaaquoiron (III) System. J. Am. Chem. Soc. 1980, 102, 5798−5809. (82) Newton, M. D. Quantum Chemical Probes of Electron-Transfer Kinetics: The Nature of Donor-Acceptor Interactions. Chem. Rev. 1991, 91, 767−792. (83) Landau, L. D. A Theory of Energy Transfer on Collisions. Phys. Z. Sowjetunion 1932, 1, 88. (84) Landau, L. D. A Theory of Energy Transfer on Collisions II. Phys. Z. Sowjetunion 1932, 2, 46. (85) Zener, C. Non-Adiabatic Crossing of Energy Levels. Proc. R. Soc. London, Ser. A 1932, 137, 696−702. (86) Spencer, J.; Scalfi, L.; Carof, A.; Blumberger, J. Confronting Surface Hopping Molecular Dynamics with Marcus Theory for a molecular donor-acceptor system. Faraday Discuss. 2016, 195, 215− 236. (87) McKenna, K. P.; Wolf, M. J.; Shluger, A. L.; Lany, S.; Zunger, A. Two-Dimensional Polaronic Behavior in the Binary Oxides m- HfO 2 and m- ZrO 2. Phys. Rev. Lett. 2012, 108, 116403. (88) Blumberger, J.; McKenna, K. P. Constrained Density Functional Theory Applied to Electron Tunnelling between Defects in MgO. Phys. Chem. Chem. Phys. 2013, 15, 2184−2196. (89) Marcus, R. A. On the Theory of Oxidation-Reduction Reactions Involving Electron Transfer. I. J. Chem. Phys. 1956, 24, 966−978. (90) Marcus, R. A. Electron Transfer Reactions in Chemistry. Theory and Experiment. Rev. Mod. Phys. 1993, 65, 599−610. (91) Fuchs, A.; Steinbrecher, T.; Mommer, M. S.; Nagata, Y.; Elstner, M.; Lennartz, C. Molecular Origin of Differences in Hole and Electron Mobility in Amorphous Alq3-A Multiscale Simulation Study. Phys. Chem. Chem. Phys. 2012, 14, 4259−4270. (92) Oberhofer, H.; Blumberger, J. Charge Constrained Density Functional Molecular Dynamics for Simulation of Condensed Phase Electron Transfer Reactions. J. Chem. Phys. 2009, 131, 064101. (93) Spencer, J.; Gajdos, F.; Blumberger, J. FOB-SH: Fragment Orbital-Based Surface Hopping for Charge Carrier Transport in Organic and Biological Molecules and Materials. J. Chem. Phys. 2016, 145, 064102. (94) Martinelli, N. G.; Idé, J.; Sánchez-Carrera, R. S.; Coropceanu, V.; Brédas, J.-L.; Ducasse, L.; Castet, F.; Cornil, J.; Beljonne, D. Influence of Structural Dynamics on Polarization Energies in Anthracene Single Crystals. J. Phys. Chem. C 2010, 114, 20678−20685. (95) Cohen, A. J.; Mori-Sánchez, P.; Yang, W. Insights into Current Limitations of Density Functional Theory. Science 2008, 321, 792− 794. (96) Valeev, E. F.; Coropceanu, V.; da Silva Filho, D. A.; Salman, S.; Brédas, J.-L. Effect of Electronic Polarization on Charge-Transport Parameters in Molecular Organic Semiconductors. J. Am. Chem. Soc. 2006, 128, 9882−9886. (97) Ryno, S. M.; Lee, S. R.; Sears, J. S.; Risko, C.; Brédas, J.-L. Electronic Polarization Effects upon Charge Injection in Oligoacene Molecular Crystals: Description via a Polarizable Force Field. J. Phys. Chem. C 2013, 117, 13853−13860. (98) Norton, J. E.; Brédas, J.-L. Polarization Energies in Oligoacene Semiconductor Crystals. J. Am. Chem. Soc. 2008, 130, 12377−12384. (99) Friederich, P.; Symalla, F.; Meded, V.; Neumann, T.; Wenzel, W. Ab Initio Treatment of Disorder Effects in Amorphous Organic Materials: Toward Parameter Free Materials Simulation. J. Chem. Theory Comput. 2014, 10, 3720−3725. (100) Castet, F.; Ducasse, L.; Fritsch, A. From Organic Superconductors to DNA: Fragment Orbital-Based Model. Int. J. Quantum Chem. 2006, 106, 734−746.

(101) Castet, F.; Aurel, P.; Fritsch, A.; Ducasse, L.; Liotard, D.; Linares, M.; Cornil, J.; Beljonne, D. Electronic Polarization Effects on Charge Carriers in Anthracene: A Valence Bond Study. Phys. Rev. B: Condens. Matter Mater. Phys. 2008, 77, 115210. (102) Nagata, Y. Polarizable Atomistic Calculation of Site Energy Disorder in Amorphous Alq3. ChemPhysChem 2010, 11, 474−479. (103) Morita, A.; Kato, S. Ab Initio Molecular Orbital Theory on Intramolecular Charge Polarization: Effect of Hydrogen Abstraction on the Charge Sensitivity of Aromatic and Nonaromatic Species. J. Am. Chem. Soc. 1997, 119, 4021−4032. (104) Kwiatkowski, J.; Nelson, J.; Li, H.; Bredas, J.; Wenzel, W.; Lennartz, C. Simulating Charge Transport in Tris (8-hydroxyquinoline) Aluminium (Alq 3). Phys. Chem. Chem. Phys. 2008, 10, 1852− 1858. (105) Bässler, H. Localized States and Electronic Transport in Single Component Organic Solids with Diagonal Disorder. Phys. Status Solidi B 1981, 107, 9−54. (106) Bässler, H. Charge Transport in Disordered Organic Photoconductors a Monte Carlo Simulation Study. Phys. Status Solidi B 1993, 175, 15−56. (107) Eley, D.; Evans, M. Heats and Entropy Changes Accompanying the Solution of Ions in Water. Trans. Faraday Soc. 1938, 34, 1093− 1112. (108) Bader, J. S.; Cortis, C. M.; Berne, B. Solvation and Reorganization Energies in Polarizable Molecular and Continuum Solvents. J. Chem. Phys. 1997, 106, 2372−2387. (109) Ayala, R.; Sprik, M. A Classical Point Charge Model Study of System Size Dependence of Oxidation and Reorganization Free Energies in Aqueous Solution. J. Phys. Chem. B 2008, 112, 257−269. (110) Blumberger, J.; Lamoureux, G. Reorganization Free Energies and Quantum Corrections for a Model Electron Self-Exchange Reaction: Comparison of Polarizable and Non-Polarizable Solvent Models. Mol. Phys. 2008, 106, 1597−1611. (111) Weaver, M. J.; Gennett, T. Influence of Solvent Reorientation Dynamics upon the Kinetics of Some Electron-Exchange Reactions. Chem. Phys. Lett. 1985, 113, 213−218. (112) Nielson, R. M.; McManis, G. E.; Golovin, M. N.; Weaver, M. J. Solvent Dynamical Effects in Electron Transfer: Comparisons of SelfExchange Kinetics for Cobaltocenium-Cobaltocene and Related Redox Couples with Theoretical Predictions. J. Phys. Chem. 1988, 92, 3441− 3450. (113) Reimers, J. R. A Practical Method for the use of Curvilinear Coordinates in Calculations of Normal-Mode-Projected Displacements and Duschinsky Rotation Matrices for Large Molecules. J. Chem. Phys. 2001, 115, 9103−9109. (114) Closs, G. L.; Miller, J. R. Intramolecular Long-Distance Electron Transfer in Organic Molecules. Science 1988, 240, 440−448. (115) Gruhn, N. E.; da Silva Filho, D. A.; Bill, T. G.; Malagoli, M.; Coropceanu, V.; Kahn, A.; Brédas, J.-L. The Vibrational Reorganization Energy in Pentacene: Molecular Influences on Charge Transport. J. Am. Chem. Soc. 2002, 124, 7918−7919. (116) Amashukeli, X.; Winkler, J. R.; Gray, H. B.; Gruhn, N. E.; Lichtenberger, D. L. Electron-Transfer Reorganization Energies of Isolated Organic Molecules. J. Phys. Chem. A 2002, 106, 7593−7598. (117) Amashukeli, X.; Gruhn, N. E.; Lichtenberger, D. L.; Winkler, J. R.; Gray, H. B. Inner-Sphere Electron-Transfer Reorganization Energies of Zinc Porphyrins. J. Am. Chem. Soc. 2004, 126, 15566− 15571. (118) Coropceanu, V.; Kwon, O.; Wex, B.; Kaafarani, B. R.; Gruhn, N. E.; Durivage, J. C.; Neckers, D. C.; Brédas, J.-L. Vibronic Coupling in Organic Semiconductors: The Case of Fused Polycyclic BenzeneThiophene Structures. Chem. - Eur. J. 2006, 12, 2073−2080. (119) Tipmanee, V.; Oberhofer, H.; Park, M.; Kim, K. S.; Blumberger, J. Prediction of Reorganization Free Energies for Biological Electron Transfer: A Comparative Study of Ru-modified Cytochromes and a 4-helix Bundle Protein. J. Am. Chem. Soc. 2010, 132, 17032−17040. 10350

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

Intersection of the 1A2 and 1B1 Excited States of Ozone. Chem. Phys. Lett. 1993, 216, 362−368. (144) Köppel, H.; Gronki, J.; Mahapatra, S. Construction Scheme for Regularized Diabatic States. J. Chem. Phys. 2001, 115, 2377−2388. (145) Kubas, A.; Gajdos, F.; Heck, A.; Oberhofer, H.; Elstner, M.; Blumberger, J. Electronic Couplings for Molecular Charge Transfer: Benchmarking CDFT, FODFT and FODFTB against High-Level Ab Initio Calculations. II. Phys. Chem. Chem. Phys. 2015, 17, 14342− 14354. (146) Ramos, P.; Mankarious, M.; Pavanello, M. Practical Aspects of Computational Chemistry IV; Springer: 2016; pp 103−134. (147) Gillet, N.; Berstis, L.; Wu, X.; Gajdos, F.; Heck, A.; de la Lande, A.; Blumberger, J.; Elstner, M. Electronic Coupling Calculations for Bridge-Mediated Charge Transfer Using Constrained Density Functional Theory (CDFT) and Effective Hamiltonian Approaches at the Density Functional Theory (DFT) and Fragment-Orbital Density Functional Tight Binding (FODFTB) Level. J. Chem. Theory Comput. 2016, 12, 4793−4805. (148) Mulliken, R. S. Molecular Compounds and their Spectra. II. J. Am. Chem. Soc. 1952, 74, 811−824. (149) Hush, N. Homogeneous and Heterogeneous Optical and Thermal Electron Transfer. Electrochim. Acta 1968, 13, 1005−1023. (150) Reimers, J. R.; Hush, N. S. Electronic Properties of TransitionMetal Complexes Determined from Electroabsorption (Stark) Spectroscopy. 2. Mononuclear Complexes of Ruthenium(II). J. Phys. Chem. 1991, 95, 9773−9781. (151) Cave, R. J.; Newton, M. D. Calculation of Electronic Coupling Matrix Elements for Ground and Excited State Electron Transfer Reactions: Comparison of the Generalized Mulliken-Hush and Block Diagonalization Methods. J. Chem. Phys. 1997, 106, 9213−9226. (152) Wu, Q.; Van Voorhis, T. Direct Optimization Method to Study Constrained Systems within Density-Functional Theory. Phys. Rev. A: At., Mol., Opt. Phys. 2005, 72, 024502. (153) Mukherji, A.; Karplus, M. Constrained Molecular Wavefunctions: HF Molecule. J. Chem. Phys. 1963, 38, 44−48. (154) Dederichs, P.; Blügel, S.; Zeller, R.; Akai, H. Ground States of Constrained Systems: Application to Cerium Impurities. Phys. Rev. Lett. 1984, 53, 2512−2515. (155) Akai, H.; Blügel, S.; Zeller, R.; Dederichs, P. Isomer Shifts and their Relation to Charge Transfer in Dilute Fe Alloys. Phys. Rev. Lett. 1986, 56, 2407−2410. (156) Hybertsen, M. S.; Schlüter, M.; Christensen, N. E. Calculation of Coulomb-Interaction Parameters for La 2 CuO 4 Using a Constrained-Density-Functional Approach. Phys. Rev. B: Condens. Matter Mater. Phys. 1989, 39, 9028−9041. (157) Zhang, Z.; Satpathy, S. Electron States, Magnetism, and the Verwey Transition in Magnetite. Phys. Rev. B: Condens. Matter Mater. Phys. 1991, 44, 13319. (158) Wesolowski, T. A.; Warshel, A. Frozen Density Functional Approach for Ab Initio Calculations of Solvated Molecules. J. Phys. Chem. 1993, 97, 8050−8053. (159) Hong, G.; Strajbl, M.; Wesolowski, T. A.; Warshel, A. Constraining the Electron Densities in DFT Method as an Effective Way for Ab Initio Studies of Metal-Catalyzed Reactions. J. Comput. Chem. 2000, 21, 1554−1561. (160) Behler, J.; Delley, B.; Lorenz, S.; Reuter, K.; Scheffler, M. Dissociation of O2 at Al (111): The Role of Spin Selection Rules. Phys. Rev. Lett. 2005, 94, 036104. (161) Behler, J.; Delley, B.; Reuter, K.; Scheffler, M. Nonadiabatic Potential-Energy Surfaces by Constrained Density-Functional Theory. Phys. Rev. B: Condens. Matter Mater. Phys. 2007, 75, 115409. (162) Wu, Q.; Van Voorhis, T. Extracting Electron Transfer Coupling Elements from Constrained Density Functional Theory. J. Chem. Phys. 2006, 125, 164105. (163) Wu, Q.; Van Voorhis, T. Constrained Density Functional Theory and its Application in Long-Range Electron Transfer. J. Chem. Theory Comput. 2006, 2, 765−774.

(120) Laplante, J.-P.; Siebrand, W. Non-Arrhenius Behaviour of Transitions across Energy Barriers Due to Crossing of Potential Energy Surfaces. Chem. Phys. Lett. 1978, 59, 433−436. (121) Jortner, J.; Ulstrup, J. Tunnelling in Low-Temperature AtomTransfer Processes. Chem. Phys. Lett. 1979, 63, 236−239. (122) Holstein, T. Studies of Polaron Motion: Part I. The MolecularCrystal Model. Ann. Phys. 1959, 8, 325−342. (123) Holstein, T. Studies of Polaron Motion: Part II. The “Small” Polaron. Ann. Phys. 1959, 8, 343−389. (124) Holstein, T. Quantal Occurrence-Probability Treatment of Small-Polaron Hopping. Philos. Mag. B 1978, 37, 49−62. (125) Barbara, P. F.; Meyer, T. J.; Ratner, M. A. Contemporary Issues in Electron Transfer Research. J. Phys. Chem. 1996, 100, 13148− 13168. (126) Geng, Y.; Wu, S.-X.; Li, H.-B.; Tang, X.-D.; Wu, Y.; Su, Z.-M.; Liao, Y. A Theoretical Discussion on the Relationships among Molecular Packings, Intermolecular Interactions, and Electron Transport Properties for Naphthalene Tetracarboxylic Diimide Derivatives. J. Mater. Chem. 2011, 21, 15558−15566. (127) Lichten, W. Molecular Wave Functions and Inelastic Atomic Collisions. Phys. Rev. 1967, 164, 131−142. (128) Smith, F. T. Diabatic and Adiabatic Representations for Atomic Collision Problems. Phys. Rev. 1969, 179, 111−123. (129) Cave, R. J.; Newton, M. D. Generalization of the MullikenHush Treatment for the Calculation of Electron Transfer Matrix Elements. Chem. Phys. Lett. 1996, 249, 15−19. (130) Mead, C. A.; Truhlar, D. G. Conditions for the Definition of a Strictly Diabatic Electronic Basis for Molecular Systems. J. Chem. Phys. 1982, 77, 6090−6098. (131) Domcke, W.; Stock, G. Theory of Ultrafast Nonadiabatic Excited-State Processes and their Spectroscopic Detection in Real Time. Adv. Chem. Phys. 1997, 100, 1−169. (132) Oberhofer, H.; Blumberger, J. Insight into the Mechanism of the Ru2+−Ru3+ Electron Self-Exchange Reaction from Quantitative Rate Calculations. Angew. Chem., Int. Ed. 2010, 49, 3631−3634. (133) Kubas, A.; Hoffmann, F.; Heck, A.; Oberhofer, H.; Elstner, M.; Blumberger, J. Electronic Couplings for Molecular Charge Transfer: Benchmarking CDFT, FODFT, and FODFTB against High-Level Ab Initio Calculations. J. Chem. Phys. 2014, 140, 104105. (134) Brédas, J.-L.; Calbert, J. P.; da Silva Filho, D. A.; Cornil, J. Organic Semiconductors: A Theoretical Characterization of the Basic Parameters Governing Charge Transport. Proc. Natl. Acad. Sci. U. S. A. 2002, 99, 5804−5809. (135) da Silva Filho, D. A.; Kim, E.-G.; Brédas, J.-L. Transport Properties in the Rubrene Crystal: Electronic Coupling and Vibrational Reorganization Energy. Adv. Mater. 2005, 17, 1072−1076. (136) Rangel, T.; Berland, K.; Sharifzadeh, S.; Brown-Altvater, F.; Lee, K.; Hyldgaard, P.; Kronik, L.; Neaton, J. B. Structural and ExcitedState Properties of Oligoacene Crystals from First Principles. Phys. Rev. B: Condens. Matter Mater. Phys. 2016, 93, 115206. (137) Worth, G.; Robb, M. Applying Direct Molecular Dynamics to Non-Adiabatic Systems. Adv. Chem. Phys. 2002, 124, 355−432. (138) Pacher, T.; Cederbaum, L. S.; Köppel, H. Approximately Diabatic States from Block Diagonalization of the Electronic Hamiltonian. J. Chem. Phys. 1988, 89, 7367−7381. (139) Baer, M. Adiabatic and Diabatic Representations for AtomMolecule Collisions: Treatment of the Collinear Arrangement. Chem. Phys. Lett. 1975, 35, 112−118. (140) Baer, M. Topological Effects in Molecular Systems: An Attempt Towards a Complete Theory. Chem. Phys. 2000, 259, 123− 147. (141) Macias, A.; Riera, A. Calculation of Diabatic States from Molecular Properties. J. Phys. B: At. Mol. Phys. 1978, 11, L489−L492. (142) Werner, H.-J.; Meyer, W. MCSCF Study of the Avoided Curve Crossing of the Two Lowest 1Σ+ States of LiF. J. Chem. Phys. 1981, 74, 5802−5807. (143) Domcke, W.; Woywod, C. Direct Construction of Diabatic States in the CASSCF Approach. Application to the Conical 10351

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

Moderate Mechanical Stretching Stresses. Phys. Rev. B: Condens. Matter Mater. Phys. 2012, 85, 075101. (185) Wolter, M.; Elstner, M.; Kubař, T. Charge Transport in Desolvated DNA. J. Chem. Phys. 2013, 139, 125102. (186) Heck, A.; Woiczikowski, P. B.; Kubař, T.; Giese, B.; Elstner, M.; Steinbrecher, T. B. Charge Transfer in Model Peptides: Obtaining Marcus Parameters from Molecular Simulation. J. Phys. Chem. B 2012, 116, 2284−2293. (187) Lüdemann, G.; Woiczikowski, P. B.; Kubař, T.; Elstner, M.; Steinbrecher, T. B. Charge Transfer in E. Coli DNA Photolyase: Understanding Polarization and Stabilization Effects via QM/MM Simulations. J. Phys. Chem. B 2013, 117, 10769−10778. (188) Heck, A.; Kranz, J. J.; Kubar, T.; Elstner, M. Multi-Scale Approach to Non-Adiabatic Charge Transport in High-Mobility Organic Semiconductors. J. Chem. Theory Comput. 2015, 11, 5068− 5082. (189) Heck, A.; Kranz, J. J.; Elstner, M. Simulation of TemperatureDependent Charge Transport in Organic Semiconductors with Various Degrees of Disorder. J. Chem. Theory Comput. 2016, 12, 3087−3096. (190) Woiczikowski, P. B.; Steinbrecher, T.; Kubař, T.; Elstner, M. Nonadiabatic QM/MM Simulations of Fast Charge Transfer in Escherichia Coli DNA Photolyase. J. Phys. Chem. B 2011, 115, 9846− 9863. (191) Ridley, J.; Zerner, M. An Intermediate Neglect of Differential Overlap Technique for Spectroscopy: Pyrrole and the Azines. Theor. Chim. Acta 1973, 32, 111−134. (192) Kirkpatrick, J. An Approximate Method for Calculating Transfer Integrals Based on the ZINDO Hamiltonian. Int. J. Quantum Chem. 2008, 108, 51−56. (193) Nelson, J.; Kwiatkowski, J. J.; Kirkpatrick, J.; Frost, J. M. Modeling Charge Transport in Organic Photovoltaic Materials. Acc. Chem. Res. 2009, 42, 1768−1778. (194) Akimov, A. V. Nonadiabatic Molecular Dynamics with TightBinding Fragment Molecular Orbitals. J. Chem. Theory Comput. 2016, 12, 5719−5736. (195) Pavanello, M.; Neugebauer, J. Modelling Charge Transfer Reactions with the Frozen Density Embedding Formalism. J. Chem. Phys. 2011, 135, 234103. (196) Wesolowski, T. A.; Weber, J. Kohn-Sham Equations with Constrained Electron Density: An Iterative Evaluation of the GroundState Electron Density of Interacting Molecules. Chem. Phys. Lett. 1996, 248, 71−76. (197) Jacob, C. R.; Neugebauer, J.; Visscher, L. A Flexible Implementation of Frozen-Density Embedding for Use in Multilevel Simulations. J. Comput. Chem. 2008, 29, 1011−1018. (198) Perdew, J. P.; Burke, K.; Ernzerhof, M. Generalized Gradient Approximation Made Simple. Phys. Rev. Lett. 1996, 77, 3865−3868. (199) Blum, V.; Gehrke, R.; Hanke, F.; Havu, P.; Havu, V.; Ren, X.; Reuter, K.; Scheffler, M. Ab Initio Molecular Simulations with Numeric Atom-Centered Orbitals. Comput. Phys. Commun. 2009, 180, 2175−2196. (200) Wesołowski, T. A. Application of the DFT-based Embedding Scheme Using an Explicit Functional of the Kinetic Energy to Determine the Spin Density of Mg+ Embedded in Ne and Ar Matrices. Chem. Phys. Lett. 1999, 311, 87−92. (201) Neugebauer, J.; Louwerse, M. J.; Baerends, E. J.; Wesolowski, T. A. The Merits of the Frozen-Density Embedding Scheme to Model Solvatochromic Shifts. J. Chem. Phys. 2005, 122, 094115. (202) Solovyeva, A.; Pavanello, M.; Neugebauer, J. Spin Densities from Subsystem Density-Functional Theory: Assessment and Application to a Photosynthetic Reaction Center Complex Model. J. Chem. Phys. 2012, 136, 194104. (203) Pavanello, M.; Van Voorhis, T.; Visscher, L.; Neugebauer, J. An Accurate and Linear-Scaling Method for Calculating Charge-Transfer Excitation Energies and Diabatic Couplings. J. Chem. Phys. 2013, 138, 054101.

(164) Wu, Q.; Van Voorhis, T. Direct Calculation of Electron Transfer Parameters through Constrained Density Functional Theory. J. Phys. Chem. A 2006, 110, 9212−9218. (165) Oberhofer, H.; Blumberger, J. Electronic Coupling Matrix Elements from Charge Constrained Density Functional Theory Calculations Using a Plane Wave Basis Set. J. Chem. Phys. 2010, 133, 244105. (166) Mulliken, R. S. Electronic Population Analysis on LCAO-MO Molecular Wave Functions. I. J. Chem. Phys. 1955, 23, 1833−1840. (167) Hirshfeld, F. Bonded-Atom Fragments for Describing Molecular Charge Densities. Theor. Chem. Acc. 1977, 44, 129−138. (168) Bader, R. F. Atoms in Molecules; Wiley Online Library: 1990. (169) Rezac, J.; Lévy, B.; Demachy, I.; de la Lande, A. Robust and Efficient Constrained DFT Molecular Dynamics Approach for Biochemical Modeling. J. Chem. Theory Comput. 2012, 8, 418−427. (170) Ř ezác,̌ J.; de la Lande, A. Robust, Basis-Set Independent Method for the Evaluation of Charge-Transfer Energy in Noncovalent Complexes. J. Chem. Theory Comput. 2015, 11, 528−537. (171) Rapacioli, M.; Spiegelman, F. Modelling Singly Ionized Coronene Clusters. Eur. Phys. J. D 2009, 52, 55−58. (172) Rapacioli, M.; Spiegelman, F.; Scemama, A.; Mirtschink, A. Modeling Charge Resonance in Cationic Molecular Clusters: Combining DFT-Tight Binding with Configuration Interaction. J. Chem. Theory Comput. 2011, 7, 44−55. (173) Rapacioli, M.; Simon, A.; Dontot, L.; Spiegelman, F. Extensions of DFTB to Investigate Molecular Complexes and Clusters. Phys. Status Solidi B 2012, 249, 245−258. (174) Porezag, D.; Frauenheim, T.; Köhler, T.; Seifert, G.; Kaschner, R. Construction of Tight-Binding-Like Potentials on the Basis of Density-Functional Theory: Application to Carbon. Phys. Rev. B: Condens. Matter Mater. Phys. 1995, 51, 12947−12957. (175) Seifert, G.; Porezag, D.; Frauenheim, T. Calculations of Molecules, Clusters, and Solids with a Simplified LCAO-DFT-LDA Scheme. Int. J. Quantum Chem. 1996, 58, 185−192. (176) Kubař, T.; Woiczikowski, P. B.; Cuniberti, G.; Elstner, M. Efficient Calculation of Charge-Transfer Matrix Elements for Hole Transfer in DNA. J. Phys. Chem. B 2008, 112, 7937−7947. (177) Senthilkumar, K.; Grozema, F.; Bickelhaupt, F.; Siebbeles, L. Charge Transport in Columnar Stacked Triphenylenes: Effects of Conformational Fluctuations on Charge Transfer Integrals and Site Energies. J. Chem. Phys. 2003, 119, 9809−9817. (178) Li, H.; Brédas, J.-L.; Lennartz, C. First-Principles Theoretical Investigation of the Electronic Couplings in Single Crystals of Phenanthroline-based Organic Semiconductors. J. Chem. Phys. 2007, 126, 164704. (179) Schober, C.; Reuter, K.; Oberhofer, H. Critical Analysis of Fragment-Orbital DFT Schemes for the Calculation of Electronic Coupling Values. J. Chem. Phys. 2016, 144, 054103. (180) Baumeier, B.; Kirkpatrick, J.; Andrienko, D. Density-Functional Based Determination of Intermolecular Charge Transfer Properties for Large-Scale Morphologies. Phys. Chem. Chem. Phys. 2010, 12, 11103− 11113. (181) Sutton, C.; Sears, J. S.; Coropceanu, V.; Bredas, J.-L. Understanding the Density Functional Dependence of DFTCalculated Electronic Couplings in Organic Semiconductors. J. Phys. Chem. Lett. 2013, 4, 919−924. (182) Lemaur, V.; da Silva Filho, D. A.; Coropceanu, V.; Lehmann, M.; Geerts, Y.; Piris, J.; Debije, M. G.; van de Craats, A. M.; Senthilkumar, K.; Siebbeles, L. D. A.; et al. Charge Transport Properties in Discotic Liquid Crystals: A Quantum-Chemical Insight into Structure-Property Relationships. J. Am. Chem. Soc. 2004, 126, 3271−3279. (183) Woiczikowski, P. B.; Kubař, T.; Gutiérrez, R.; Cuniberti, G.; Elstner, M. Structural Stability Versus Conformational Sampling in Biomolecular Systems: Why is the Charge Transfer Efficiency in G4DNA Better than in Double-Stranded DNA? J. Chem. Phys. 2010, 133, 035103. (184) Wolter, M.; Woiczikowski, P. B.; Elstner, M.; Kubař, T. Response of the Electric Conductivity of Double-Stranded DNA on 10352

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

(225) Voter, A. F. In Radiation Eﬀects in Solids; Sickafus, K. E., Kotamin, E. A., Uberuaga, B. P., Eds.; Springer: 2007; pp 1−23. (226) Vissenberg, M. C. J. M.; Matters, M. Theory of the Field-Effect Mobility in Amorphous Organic Transistors. Phys. Rev. B: Condens. Matter Mater. Phys. 1998, 57, 12964−12967. (227) Fichthorn, K. A.; Scheffler, M. Island Nucleation in Thin-Film Epitaxy: A First-Principles Investigation. Phys. Rev. Lett. 2000, 84, 5371−5374. (228) Yu, Z. G.; Smith, D. L.; Saxena, A.; Martin, R. L.; Bishop, A. R. Molecular Geometry Fluctuations and Field-Dependent Mobility in Conjugated Polymers. Phys. Rev. B: Condens. Matter Mater. Phys. 2001, 63, 085202. (229) Fähnle, M.; Drautz, R.; Lechermann, F.; Singer, R.; Diaz-Ortiz, A.; Dosch, H. Thermodynamic Properties from Ab-Initio Calculations: New Theoretical Developments, and Applications to Various Materials Systems. Phys. Status Solidi B 2005, 242, 1159−1173. (230) Zhang, Y.; Blum, V.; Reuter, K. Accuracy of First-Principles Lateral Interactions: Oxygen at Pd(100). Phys. Rev. B: Condens. Matter Mater. Phys. 2007, 75, 235406. (231) Lorenzi, J. M.; Matera, S.; Reuter, K. Synergistic Inhibition of Oxide Formation in Oxidation Catalysis: A First-Principles Kinetic Monte Carlo Study of NO + CO Oxidation at Pd(100). ACS Catal. 2016, 6, 5191−5197. (232) Idé, J.; Fazzi, D.; Casalegno, M.; Meille, S. V.; Raos, G. Electron Transport in Crystalline PCBM-like Fullerene Derivatives: a Comparative Computational Study. J. Mater. Chem. C 2014, 2, 7313− 7325. (233) Di Motta, S.; Di Donato, E.; Negri, F.; Orlandi, G.; Fazzi, D.; Castiglioni, C. Resistive Molecular Memories: Influence of Molecular Parameters on the Electrical Bistability. J. Am. Chem. Soc. 2009, 131, 6591−6598. (234) Huong, V. T. T.; Tai, T. B.; Nguyen, M. T. Theoretical Design of n-type Organic Semiconducting Materials Containing Thiazole and Oxazole Frameworks. J. Phys. Chem. A 2014, 118, 3335−3343. (235) McMahon, D. P.; Troisi, A. Evaluation of the External Reorganization Energy of Polyacenes. J. Phys. Chem. Lett. 2010, 1, 941−946. (236) Cornil, J.; Verlaak, S.; Martinelli, N.; Mityashin, A.; Olivier, Y.; Van Regemorter, T.; D’Avino, G.; Muccioli, L.; Zannoni, C.; Castet, F.; et al. Exploring the Energy Landscape of the Charge Transport Levels in Organic Semiconductors at the Molecular Scale. Acc. Chem. Res. 2013, 46, 434−443. (237) Athanasopoulos, S.; Kirkpatrick, J.; Martínez, D.; Frost, J. M.; Foden, C. M.; Walker, A. B.; Nelson, J. Predictive Study of Charge Transport in Disordered Semiconducting Polymers. Nano Lett. 2007, 7, 1785−1788. (238) Pershin, A.; Donets, S.; Baeurle, S. A. A New Multiscale Modeling Method for Simulating the Loss Processes in Polymer Solar Cell Nanodevices. J. Chem. Phys. 2012, 136, 194102. (239) Walker, A. B. Multiscale Modeling of Charge and Energy Transport in Organic Light-Emitting Diodes and Photovoltaics. Proc. IEEE 2009, 97, 1587−1596. (240) Jacoboni, C.; Lugli, P. The Monte Carlo Method for Semiconductor Device Simulation; Springer: 1989; pp 6−103. (241) LeBlanc, O. H., Jr. Band Structure and Transport of Holes and Electrons in Anthracene. J. Chem. Phys. 1961, 35, 1275−1280. (242) Wang, L.; Beljonne, D. Flexible Surface Hopping Approach to Model the Crossover from Hopping to Band-like Transport in Organic Crystals. J. Phys. Chem. Lett. 2013, 4, 1888−1894. (243) Blülle, B.; Troisi, A.; Häusermann, R.; Batlogg, B. Charge Transport Perpendicular to the High Mobility Plane in Organic Crystals: Bandlike Temperature Dependence Maintained Despite Hundredfold Anisotropy. Phys. Rev. B: Condens. Matter Mater. Phys. 2016, 93, 035205. (244) Parker, S. P. McGraw-Hill Encyclopedia of Physics; McGraw-Hill Book Co.: New York, NY, 1983. (245) Jacoboni, C.; Reggiani, L. The Monte Carlo Method for the Solution of Charge Transport in Semiconductors with Application to Covalent Materials. Rev. Mod. Phys. 1983, 55, 645−705.

(204) Ramos, P.; Papadakis, M.; Pavanello, M. Performance of Frozen Density Embedding for Modeling Hole Transfer Reactions. J. Phys. Chem. B 2015, 119, 7541−7557. (205) Solovyeva, A.; Pavanello, M.; Neugebauer, J. Describing LongRange Charge-Separation Processes with Subsystem Density-Functional Theory. J. Chem. Phys. 2014, 140, 164103. (206) Thom, A. J. W.; Head-Gordon, M. Hartree−Fock Solutions as a Quasidiabatic Basis for Nonorthogonal Configuration Interaction. J. Chem. Phys. 2009, 131, 124113. (207) Kondov, I.; Cízek, M.; Benesch, C.; Wang, H.; Thoss, M. Quantum Dynamics of Photoinduced Electron-Transfer Reactions in Dye-Semiconductor Systems: First-Principles Description and Application to Coumarin 343-TiO2. J. Phys. Chem. C 2007, 111, 11970− 11981. (208) Priyadarshy, S.; Skourtis, S. S.; Risser, S. M.; Beratan, D. N. Bridge-Mediated Electronic Interactions: Differences Between Hamiltonian and Green Function Partitioning in a Non-Orthogonal Basis. J. Chem. Phys. 1996, 104, 9473−9481. (209) Kurnikov, I. V.; Beratan, D. N. Abinitio Based Effective Hamiltonians for Long-Range Electron Transfer: Hartree−Fock Analysis. J. Chem. Phys. 1996, 105, 9561−9573. (210) Galperin, M.; Toledo, S.; Nitzan, A. Numerical Computation of Tunneling Fluxes. J. Chem. Phys. 2002, 117, 10817−10826. (211) Löwdin, P. O. On the Non-Orthogonality problem Connected with the Use of Atomic Wave Functions in the Theory of Molecules and Crystals. J. Chem. Phys. 1950, 18, 365−375. (212) Mayer, I. On Löwdin’s Method of Symmetric Orthogonalization. Int. J. Quantum Chem. 2002, 90, 63−65. (213) Aiken, J. G.; Erdos, J. A.; Goldstein, J. A. On Löwdin Orthogonalization. Int. J. Quantum Chem. 1980, 18, 1101−1108. (214) Prucker, V.; Rubio-Pons, O.; Bockstedte, M.; Wang, H.; Coto, P. B.; Thoss, M. Dynamical Simulation of Electron Transfer Processes in Alkanethiolate Self-Assembled Monolayers at the Au (111) Surface. J. Phys. Chem. C 2013, 117, 25334−25342. (215) Li, J.; Nilsing, M.; Kondov, I.; Wang, H.; Persson, P.; Lunell, S.; Thoss, M. Dynamical Simulation of Photoinduced Electron Transfer Reactions in Dye- Semiconductor Systems with Different Anchor Groups. J. Phys. Chem. C 2008, 112, 12326−12333. (216) Gajdos, F.; Valner, S.; Hoffmann, F.; Spencer, J.; Breuer, M.; Kubas, A.; Dupuis, M.; Blumberger, J. Ultrafast Estimation of Electronic Couplings for Electron Transfer between π-conjugated Organic Molecules. J. Chem. Theory Comput. 2014, 10, 4653−4660. (217) Geng, H.; Zheng, X.; Shuai, Z.; Zhu, L.; Yi, Y. Understanding the Charge Transport and Polarities in Organic Donor−Acceptor Mixed-Stack Crystals: Molecular Insights from the Super-Exchange Couplings. Adv. Mater. 2015, 27, 1443−1449. (218) Ramos, P.; Pavanello, M. Quantifying Environmental Effects on the Decay of Hole Transfer Couplings in Biosystems. J. Chem. Theory Comput. 2014, 10, 2546−2556. (219) Siddarth, P.; Marcus, R. Correlation between Theory and Experiment in Electron-Transfer Reactions in Proteins: Electronic Couplings in Modified Cytochrome c and Myoglobin Derivatives. J. Phys. Chem. 1993, 97, 13078−13082. (220) Gruschus, J. M.; Kuki, A. New Hamiltonian Model for LongRange Electronic Superexchange in Complex Molecular Structures. J. Phys. Chem. 1993, 97, 5581−5593. (221) Beeler, J. R. Displacement Spikes in Cubic Metals. I. α-Iron, Copper, and Tungsten. Phys. Rev. 1966, 150, 470−487. (222) Liu, D.-J.; Garcia, A.; Wang, J.; Ackerman, D. M.; Wang, C.-J.; Evans, J. W. Kinetic Monte Carlo Simulation of Statistical Mechanical Models and Coarse-Grained Mesoscale Descriptions of Catalytic Reaction−Diffusion Processes: 1D Nanoporous and 2D Surface Systems. Chem. Rev. 2015, 115, 5979−6050. (223) Reuter, K. Ab Initio Thermodynamics and First-Principles Microkinetics for Surface Catalysis. Catal. Lett. 2016, 146, 541−563. (224) Baumeier, B.; Stenzel, O.; Poelking, C.; Andrienko, D.; Schmidt, V. Stochastic Modeling of Molecular Charge Transport Networks. Phys. Rev. B: Condens. Matter Mater. Phys. 2012, 86, 184202. 10353

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

(246) Ziman, J. M. Principles of the Theory of Solids; Cambridge University Press: 1972. (247) Herring, C.; Vogt, E. Transport and Deformation-Potential Theory for Many-Valley Semiconductors with Anisotropic Scattering. Phys. Rev. 1956, 101, 944−961. (248) Askerov, B. M. Electron Transport Phenomena in Semiconductors; World Scientiﬁc: 1994; Vol. 394. (249) Xi, J.; Long, M.; Tang, L.; Wang, D.; Shuai, Z. First-Principles Prediction of Charge Mobility in Carbon and Organic Nanomaterials. Nanoscale 2012, 4, 4348−4369. (250) Szulczewski, G.; Sanvito, S.; Coey, M. A Spin of their Own. Nat. Mater. 2009, 8, 693−695. (251) Katz, J. L.; Rice, S. A.; Choi, S.; Jortner, J. On the Excess Electron and Hole Band Structures and Carrier Mobility in Naphthalene, Anthracene, and Several Polyphenyls. J. Chem. Phys. 1963, 39, 1683−1697. (252) Cheng, Y.; Silbey, R.; da Silva Filho, D. A.; Calbert, J. P.; Cornil, J.; Brédas, J.-L. Three-Dimensional Band Structure and Bandlike Mobility in Oligoacene Single Crystals: A Theoretical Investigation. J. Chem. Phys. 2003, 118, 3764−3774. (253) Troisi, A.; Orlandi, G. Band Structure of the Four Pentacene Polymorphs and Effect on the Hole Mobility at Low Temperature. J. Phys. Chem. B 2005, 109, 1849−1856. (254) Kobayashi, H.; Kobayashi, N.; Hosoi, S.; Koshitani, N.; Murakami, D.; Shirasawa, R.; Kudo, Y.; Hobara, D.; Tokita, Y.; Itabashi, M. Hopping and Band Mobilities of Pentacene, Rubrene, and 2, 7-dioctyl[1]benzothieno[3, 2-b][1]benzothiophene (C8-BTBT) from First Principle Calculations. J. Chem. Phys. 2013, 139, 014707. (255) Bardeen, J.; Shockley, W. Deformation Potentials and Mobilities in Non-Polar Crystals. Phys. Rev. 1950, 80, 72−80. (256) Harrison, W. A. Scattering of Electrons by Lattice Vibrations in Nonpolar Crystals. Phys. Rev. 1956, 104, 1281−1290. (257) Fratini, S.; Ciuchi, S. Bandlike Motion and Mobility Saturation in Organic Molecular Semiconductors. Phys. Rev. Lett. 2009, 103, 266601. (258) Fratini, S.; Mayou, D.; Ciuchi, S. The Transient Localization Scenario for Charge Transport in Crystalline Organic Materials. Adv. Funct. Mater. 2016, 26, 2292−2315. (259) Northrup, J. Two-Dimensional Deformation Potential Model of Mobility in Small Molecule Organic Semiconductors. Appl. Phys. Lett. 2011, 99, 062111. (260) Beleznay, F.; Bogár, F.; Ladik, J. Charge Carrier Mobility in Quasi-One-Dimensional Systems: Application to a Guanine Stack. J. Chem. Phys. 2003, 119, 5690−5695. (261) Price, P. Two-Dimensional Electron Transport in Semiconductor Layers. I. Phonon Scattering. Ann. Phys. 1981, 133, 217− 239. (262) Walukiewicz, W.; Ruda, H.; Lagowski, J.; Gatos, H. Electron Mobility in Modulation-Doped Heterostructures. Phys. Rev. B: Condens. Matter Mater. Phys. 1984, 30, 4571−4582. (263) Fishman, G. Phonon-Limited Mobility in a Quasi-OneDimensional Semiconductor. Phys. Rev. B: Condens. Matter Mater. Phys. 1987, 36, 7448−7456. (264) Takagi, S.; Hoyt, J. L.; Welser, J. J.; Gibbons, J. F. Comparative Study of Phonon-Limited Mobility of Two-Dimensional Electrons in Strained and Unstrained Si Metal-Oxide-Semiconductor Field-Effect Transistors. J. Appl. Phys. 1996, 80, 1567−1577. (265) Togo, A.; Chaput, L.; Tanaka, I.; Hug, G. First-Principles Phonon Calculations of Thermal Expansion in Ti 3 SiC 2, Ti 3 AlC 2, and Ti 3 GeC 2. Phys. Rev. B: Condens. Matter Mater. Phys. 2010, 81, 174301. (266) Giuggioli, L.; Andersen, J. D.; Kenkre, V. Mobility Theory of Intermediate-Bandwidth Carriers in Organic Crystals: Scattering by Acoustic and Optical Phonons. Phys. Rev. B: Condens. Matter Mater. Phys. 2003, 67, 045110. (267) Li, Y.; Yi, Y.; Coropceanu, V.; Brédas, J.-L. Optical Conductivity and Optical Effective Mass in a High-Mobility Organic Semiconductor: Implications for the Nature of Charge Transport. Phys. Rev. B: Condens. Matter Mater. Phys. 2014, 90, 245112.

(268) Yang, H.; Gajdos, F.; Blumberger, J. Intermolecular Charge Transfer Parameters, Electron-Phonon Couplings, and the Validity of Polaron Hopping Models in Organic Semiconducting Crystals: Rubrene, Pentacene, and C60. J. Phys. Chem. C 2017, 121, 7689−7696. (269) Troisi, A. The Speed Limit for Sequential Charge Hopping in Molecular Materials. Org. Electron. 2011, 12, 1988−1991. (270) Dong, H.; Fu, X.; Liu, J.; Wang, Z.; Hu, W. 25th Anniversary Article: Key Points for High-Mobility Organic Field-Effect Transistors. Adv. Mater. 2013, 25, 6158−6183. (271) Gershenson, M.; Podzorov, V.; Morpurgo, A. Colloquium: Electronic Transport in Single-Crystal Organic Transistors. Rev. Mod. Phys. 2006, 78, 973−989. (272) Mott, N. F.; Davis, E. A. Electronic Processes in Non-Crystalline Materials; Oxford University Press: Oxford, 2012. (273) Street, R.; Northrup, J.; Salleo, A. Transport in Polycrystalline Polymer Thin-Film Transistors. Phys. Rev. B: Condens. Matter Mater. Phys. 2005, 71, 165202. (274) Troisi, A.; Orlandi, G. Dynamics of the Intermolecular Transfer Integral in Crystalline Organic Semiconductors. J. Phys. Chem. A 2006, 110, 4065−4070. (275) Emin, D. Phonon-Assisted Transition Rates I. Optical-PhononAssisted Hopping in Solids. Adv. Phys. 1975, 24, 305−348. (276) de Raedt, H.; Lagendijk, A. Numerical Study of Holstein’s Molecular-Crystal Model: Adiabatic Limit and Influence of Phonon Dispersion. Phys. Rev. B: Condens. Matter Mater. Phys. 1984, 30, 1671− 1678. (277) Kenkre, V.; Andersen, J. D.; Dunlap, D.; Duke, C. Unified Theory of the Mobilities of Photoinjected Electrons in Naphthalene. Phys. Rev. Lett. 1989, 62, 1165−1168. (278) Wu, M.; Conwell, E. Transport in α-sexithiophene Films. Chem. Phys. Lett. 1997, 266, 363−367. (279) Hannewald, K.; Bobbert, P. Ab Initio Theory of ChargeCarrier Conduction in Ultrapure Organic Crystals. Appl. Phys. Lett. 2004, 85, 1535−1537. (280) Friedman, L. Electron-Phonon Interaction in Organic Molecular Crystals. Phys. Rev. 1965, 140, A1649−A1667. (281) Munn, R.; Silbey, R. Theory of Electronic Transport in Molecular Crystals. II. Zeroth Order States Incorporating Nonlocal Linear Electron−Phonon Coupling. J. Chem. Phys. 1985, 83, 1843− 1853. (282) Troisi, A. Prediction of the Absolute Charge Mobility of Molecular Semiconductors: the Case of Rubrene. Adv. Mater. 2007, 19, 2000−2004. (283) Cheng, Y.-C.; Silbey, R. J. A Unified Theory for Charge-Carrier Transport in Organic Crystals. J. Chem. Phys. 2008, 128, 114713. (284) Ortmann, F.; Bechstedt, F.; Hannewald, K. Theory of Charge Transport in Organic Crystals: Beyond Holstein’s Small-Polaron Model. Phys. Rev. B: Condens. Matter Mater. Phys. 2009, 79, 235206. (285) Ortmann, F.; Bechstedt, F.; Hannewald, K. Charge Transport in Organic Crystals: Theory and Modelling. Phys. Status Solidi B 2011, 248, 511−525. (286) Troisi, A. Charge Transport in High Mobility Molecular Semiconductors: Classical Models and New Theories. Chem. Soc. Rev. 2011, 40, 2347−2358. (287) Girlando, A.; Masino, M.; Visentini, G.; Della Valle, R. G.; Brillante, A.; Venuti, E. Lattice Dynamics and Electron-Phonon Coupling in the β-(BEDT-TTF)2I3 Organic Superconductor. Phys. Rev. B: Condens. Matter Mater. Phys. 2000, 62, 14476. (288) Girlando, A.; Grisanti, L.; Masino, M.; Bilotti, I.; Brillante, A.; Della Valle, R. G.; Venuti, E. Peierls and Holstein Carrier-Phonon Coupling in Crystalline Rubrene. Phys. Rev. B: Condens. Matter Mater. Phys. 2010, 82, 035208. (289) Li, X.; Tully, J. C.; Schlegel, H. B.; Frisch, M. J. Ab Initio Ehrenfest Dynamics. J. Chem. Phys. 2005, 123, 084106. (290) Tully, J. C. Molecular Dynamics with Electronic Transitions. J. Chem. Phys. 1990, 93, 1061−1071. (291) Tully, J. C. In Classical and Quantum Dynamics in Condensed Phase Simulations; Berne, B. J., Ciccotti, G., Coker, D. F., Eds.; World Scientiﬁc: 1998; pp 34−71. 10354

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

(292) Tully, J. C. Perspective: Nonadiabatic Dynamics Theory. J. Chem. Phys. 2012, 137, 22A301. (293) Plasser, F.; Lischka, H. Semiclassical Dynamics Simulations of Charge Transport in Stacked π-systems. J. Chem. Phys. 2011, 134, 034309. (294) Mitrić, R.; Bonačić-Kouteckỳ, V.; Pittner, J.; Lischka, H. Ab Initio Nonadiabatic Dynamics Study of Ultrafast Radiationless Decay over Conical Intersections Illustrated on the Na3F Cluster. J. Chem. Phys. 2006, 125, 024303. (295) Blancafort, L.; Hunt, P.; Robb, M. A. Intramolecular Electron Transfer in Bis(methylene)adamantyl Radical Cation: A Case study of Diabatic Trapping. J. Am. Chem. Soc. 2005, 127, 3391−3399. (296) Plasser, F.; Granucci, G.; Pittner, J.; Barbatti, M.; Persico, M.; Lischka, H. Surface Hopping Dynamics Using a Locally Diabatic Formalism: Charge Transfer in the Ethylene Dimer Cation and Excited State Dynamics in the 2-pyridone Dimer. J. Chem. Phys. 2012, 137, 22A514. (297) Craig, C. F.; Duncan, W. R.; Prezhdo, O. V. Trajectory Surface Hopping in the Time-Dependent Kohn-Sham Approach for ElectronNuclear Dynamics. Phys. Rev. Lett. 2005, 95, 163001. (298) Tapavicza, E.; Tavernelli, I.; Rothlisberger, U. Trajectory Surface Hopping within Linear Response Time-Dependent DensityFunctional Theory. Phys. Rev. Lett. 2007, 98, 023001. (299) Curchod, B.; Penfold, T.; Rothlisberger, U.; Tavernelli, I. Nonadiabatic Ab Initio Molecular Dynamics Using Linear-Response Time-Dependent Density Functional Theory. Cent. Eur. J. Phys. 2013, 11, 1059−1065. (300) Doltsinis, N. L.; Marx, D. Nonadiabatic Car-Parrinello Molecular Dynamics. Phys. Rev. Lett. 2002, 88, 166402. (301) Doltsinis, N. L.; Marx, D. First Principles Molecular Dynamics Involving Excited States and Nonadiabatic Transitions. J. Theor. Comput. Chem. 2002, 01, 319−349. (302) Fabiano, E.; Keal, T.; Thiel, W. Implementation of Surface Hopping Molecular Dynamics Using Semiempirical Methods. Chem. Phys. 2008, 349, 334−347. (303) Lan, Z.; Fabiano, E.; Thiel, W. Photoinduced Nonadiabatic Dynamics of Pyrimidine Nucleobases: On-the-Fly Surface-Hopping Study with Semiempirical Methods. J. Phys. Chem. B 2009, 113, 3548− 3555. (304) Nelson, T.; Fernandez-Alberti, S.; Chernyak, V.; Roitberg, A. E.; Tretiak, S. Nonadiabatic Excited-State Molecular Dynamics Modeling of Photoinduced Dynamics in Conjugated Molecules. J. Phys. Chem. B 2011, 115, 5402−5414. (305) Nelson, T.; Fernandez-Alberti, S.; Roitberg, A. E.; Tretiak, S. Nonadiabatic Excited-State Molecular Dynamics: Modeling Photophysics in Organic Conjugated Materials. Acc. Chem. Res. 2014, 47, 1155−1164. (306) Sterpone, F.; Rossky, P. J. Molecular Modeling and Simulation of Conjugated Polymer Oligomers: Ground and Excited State Chain Dynamics of PPV in the Gas Phase. J. Phys. Chem. B 2008, 112, 4983− 4993. (307) Elstner, M.; Porezag, D.; Jungnickel, G.; Elsner, J.; Haugk, M.; Frauenheim, T.; Suhai, S.; Seifert, G. Self-Consistent-Charge DensityFunctional Tight-Binding Method for Simulations of Complex Materials Properties. Phys. Rev. B: Condens. Matter Mater. Phys. 1998, 58, 7260−7268. (308) Kubař, T.; Elstner, M. Efficient Algorithms for the Simulation of Non-Adiabatic Electron Transfer in Complex Molecular Systems: Application to DNA. Phys. Chem. Chem. Phys. 2013, 15, 5794−5813. (309) Kubař, T.; Elstner, M. A Hybrid Approach to Simulation of Electron Transfer in Complex Molecular Systems. J. R. Soc., Interface 2013, 10, 20130415. (310) Mitric, R.; Werner, U.; Wohlgemuth, M.; Seifert, G.; BonačićKoutecký, V. Nonadiabatic Dynamics within Time-Dependent Density Functional Tight Binding Method. J. Phys. Chem. A 2009, 113, 12700− 12705. (311) Wang, L.; Beljonne, D. Charge Transport in Organic Semiconductors: Assessment of the Mean Field Theory in the Hopping Regime. J. Chem. Phys. 2013, 139, 064316.

(312) Press, W. H.; Teukolsky, S. A.; Vetterling, W. T.; Flannery, B. P. Numerical Recipes, 3rd ed.; Cambridge University Press: Cambridge, 2007. (313) Schleife, A.; Draeger, E. W.; Kanai, Y.; Correa, A. A. PlaneWave Pseudopotential Implementation of Explicit Integrators for Time-Dependent Kohn-Sham Equations in Large-Scale Simulations. J. Chem. Phys. 2012, 137, 22A546. (314) Castro, A.; Marques, M. A. Time-Dependent Density Functional Theory; Springer: 2006; pp 197−210. (315) Wang, L.; Beljonne, D.; Chen, L.; Shi, Q. Mixed QuantumClassical Simulations of Charge Transport in Organic Materials: Numerical Benchmark of the Su-Schrieffer-Heeger Model. J. Chem. Phys. 2011, 134, 244116. (316) Troisi, A.; Orlandi, G. Charge-Transport Regime of Crystalline Organic Semiconductors: Diffusion Limited by Thermal Off-Diagonal Electronic Disorder. Phys. Rev. Lett. 2006, 96, 086601. (317) Hultell, M.; Stafström, S. Polaron Dynamics in Highly Ordered Molecular Crystals. Chem. Phys. Lett. 2006, 428, 446−450. (318) Castro, A.; Gross, E. Optimal Control Theory for QuantumClassical Systems: Ehrenfest Molecular Dynamics Based on TimeDependent Density-Functional Theory. J. Phys. A: Math. Theor. 2014, 47, 025204. (319) Akimov, A. V.; Long, R.; Prezhdo, O. V. Coherence Penalty Functional: A Simple Method for Adding Decoherence in Ehrenfest Dynamics. J. Chem. Phys. 2014, 140, 194107. (320) Granucci, G.; Persico, M. Critical Appraisal of the Fewest Switches Algorithm for Surface Hopping. J. Chem. Phys. 2007, 126, 134114. (321) Wang, L.; Akimov, A. V.; Prezhdo, O. V. Recent Progress in Surface Hopping: 2011−2015. J. Phys. Chem. Lett. 2016, 7, 2100− 2112. (322) Bittner, E. R.; Rossky, P. J. Quantum Decoherence in Mixed Quantum-Classical Systems: Nonadiabatic Processes. J. Chem. Phys. 1995, 103, 8130−8143. (323) Fang, J.-Y.; Hammes-Schiffer, S. Improvement of the Internal Consistency in Trajectory Surface Hopping. J. Phys. Chem. A 1999, 103, 9399−9407. (324) Hack, M. D.; Wensmann, A. M.; Truhlar, D. G.; Ben-Nun, M.; Martınez, T. J. Comparison of Full Multiple Spawning, Trajectory Surface Hopping, and Converged Quantum Mechanics for Electronically Nonadiabatic Dynamics. J. Chem. Phys. 2001, 115, 1172−1186. (325) Subotnik, J. E.; Shenvi, N. A New Approach to Decoherence and Momentum Rescaling in the Surface Hopping Algorithm. J. Chem. Phys. 2011, 134, 024105. (326) Subotnik, J. E.; Shenvi, N. Decoherence and Surface Hopping: When Can Averaging over Initial Conditions Help Capture the Effects of Wave Packet Separation? J. Chem. Phys. 2011, 134, 244114. (327) Shushkov, P.; Li, R.; Tully, J. C. Ring Polymer Molecular Dynamics with Surface Hopping. J. Chem. Phys. 2012, 137, 22A549. (328) Habershon, S.; Manolopoulos, D. E.; Markland, T. E.; Miller, T. F., III Ring-Polymer Molecular Dynamics: Quantum Effects in Chemical Dynamics from Classical Trajectories in an Extended Phase Space. Annu. Rev. Phys. Chem. 2013, 64, 387−413. (329) Lu, J.; Zhou, Z. Path Integral Molecular Dynamics with Surface Hopping for Thermal Equilibrium Sampling of Nonadiabatic Systems. J. Chem. Phys. 2017, 146, 154110. (330) Schwartz, B. J.; Bittner, E. R.; Prezhdo, O. V.; Rossky, P. J. Quantum Decoherence and the Isotope Effect in Condensed Phase Nonadiabatic Molecular Dynamics Simulations. J. Chem. Phys. 1996, 104, 5942−5955. (331) Zhu, C.; Nangia, S.; Jasper, A. W.; Truhlar, D. G. Coherent Switching with Decay of Mixing: An Improved Treatment of Electronic Coherence for Non-Born−Oppenheimer Trajectories. J. Chem. Phys. 2004, 121, 7658−7670. (332) Landry, B. R.; Subotnik, J. E. Communication: Standard Surface Hopping Predicts Incorrect Scaling for Marcus’ Golden-Rule Rate: The Decoherence Problem Cannot be Ignored. J. Chem. Phys. 2011, 135, 191101. 10355

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

(333) Chen, H.-T.; Reichman, D. R. On the Accuracy of Surface Hopping Dynamics in Condensed Phase Non-Adiabatic Problems. J. Chem. Phys. 2016, 144, 094104. (334) Landry, B. R.; Subotnik, J. E. How to Recover Marcus Theory with Fewest Switches Surface Hopping: Add Just a Touch of Decoherence. J. Chem. Phys. 2012, 137, 22A513. (335) Falk, M. J.; Landry, B. R.; Subotnik, J. E. Can Surface Hopping sans Decoherence Recover Marcus Theory? Understanding the Role of Friction in a Surface Hopping View of Electron Transfer. J. Phys. Chem. B 2014, 118, 8108−8117. (336) Worth, G. A.; Cederbaum, L. S. Beyond Born-Oppenheimer: Molecular Dynamics through a Conical Intersection. Annu. Rev. Phys. Chem. 2004, 55, 127−158. (337) Fernandez-Alberti, S.; Roitberg, A. E.; Nelson, T.; Tretiak, S. Identification of Unavoided Crossings in Nonadiabatic Photoexcited Dynamics Involving Multiple Electronic States in Polyatomic Conjugated Molecules. J. Chem. Phys. 2012, 137, 014512. (338) Wang, L.; Prezhdo, O. V. A Simple Solution to the Trivial Crossing Problem in Surface Hopping. J. Phys. Chem. Lett. 2014, 5, 713−719. (339) Hurd, P.; Cusati, T.; Persico, M. Trajectory Integration with Potential Energy Discontinuities. J. Comput. Phys. 2010, 229, 2109− 2116. (340) Schmidt, J.; Parandekar, P. V.; Tully, J. C. Mixed QuantumClassical Equilibrium: Surface Hopping. J. Chem. Phys. 2008, 129, 044104. (341) Sherman, M.; Corcelli, S. Thermal Equilibrium Properties of Surface Hopping with an Implicit Langevin Bath. J. Chem. Phys. 2015, 142, 024110. (342) Shenvi, N.; Cheng, H.; Tully, J. C. Nonadiabatic Dynamics near Metal Surfaces: Decoupling Quantum Equations of Motion in the Wide-Band Limit. Phys. Rev. A: At., Mol., Opt. Phys. 2006, 74, 062902. (343) Provorse, M. R.; Isborn, C. M. Electron Dynamics with RealTime Time-Dependent Density Functional Theory. Int. J. Quantum Chem. 2016, 116, 739−749. (344) Runge, E.; Gross, E. K. U. Density-Functional Theory for Time-Dependent Systems. Phys. Rev. Lett. 1984, 52, 997−1000. (345) Hohenberg, P.; Kohn, W. Inhomogeneous Electron Gas. Phys. Rev. 1964, 136, B864−B871. (346) van Leeuwen, R. Mapping from Densities to Potentials in Time-Dependent Density-Functional Theory. Phys. Rev. Lett. 1999, 82, 3863. (347) Kohn, W.; Sham, L. J. Self-Consistent Equations Including Exchange and Correlation Effects. Phys. Rev. 1965, 140, A1133− A1138. (348) Maitra, N. T.; Burke, K.; Woodward, C. Memory in TimeDependent Density Functional Theory. Phys. Rev. Lett. 2002, 89, 023002. (349) Marques, M. A.; Maitra, N. T.; Nogueira, F. M.; Gross, E. K.; Rubio, A. Fundamentals of Time-Dependent Density Functional Theory; Springer Science & Business Media: 2012; Vol. 837. (350) Thiele, M.; Gross, E.; Kümmel, S. Adiabatic Approximation in Nonperturbative Time-Dependent Density-Functional Theory. Phys. Rev. Lett. 2008, 100, 153004. (351) Elliott, P.; Fuks, J. I.; Rubio, A.; Maitra, N. T. Universal Dynamical Steps in the Exact Time-Dependent Exchange-Correlation Potential. Phys. Rev. Lett. 2012, 109, 266404. (352) Fuks, J. I.; Elliott, P.; Rubio, A.; Maitra, N. T. Dynamics of Charge-Transfer Processes with Time-Dependent Density Functional Theory. J. Phys. Chem. Lett. 2013, 4, 735−739. (353) Fuks, J.; Maitra, N. Charge Transfer in Time-Dependent Density-Functional Theory: Insights from the Asymmetric Hubbard Dimer. Phys. Rev. A: At., Mol., Opt. Phys. 2014, 89, 062502. (354) Castro, A.; Marques, M. A.; Alonso, J. A.; Bertsch, G. F.; Rubio, A. Excited States Dynamics in Time-Dependent Density Functional Theory. Eur. Phys. J. D 2004, 28, 211−218. (355) Alonso, J. L.; Andrade, X.; Echenique, P.; Falceto, F.; PradaGracia, D.; Rubio, A. Efficient Formalism for Large-Scale Ab Initio

Molecular Dynamics Based on Time-Dependent Density Functional Theory. Phys. Rev. Lett. 2008, 101, 096403. (356) Kreibich, T.; Gross, E. Multicomponent Density-Functional Theory for Electrons and Nuclei. Phys. Rev. Lett. 2001, 86, 2984. (357) Butriy, O.; Ebadi, H.; de Boeij, P.; van Leeuwen, R.; Gross, E. Multicomponent Density-Functional Theory for Time-Dependent Systems. Phys. Rev. A: At., Mol., Opt. Phys. 2007, 76, 052514. (358) Makri, N.; Miller, W. H. Time-Dependent Self-Consistent Field (TDSCF) Approximation for a Reaction Coordinate Coupled to a Harmonic Bath: Single and Multiple Configuration Treatments. J. Chem. Phys. 1987, 87, 5781−5787. (359) Meyer, H.-D.; Manthe, U.; Cederbaum, L. S. The MultiConfigurational Time-Dependent Hartree Approach. Chem. Phys. Lett. 1990, 165, 73−78. (360) Manthe, U.; Meyer, H.-D.; Cederbaum, L. S. Wave-Packet Dynamics within the Multiconfiguration Hartree Framework: General Aspects and Application to NOCl. J. Chem. Phys. 1992, 97, 3199− 3213. (361) Beck, M. H.; Jäckle, A.; Worth, G.; Meyer, H.-D. The Multiconfiguration Time-Dependent Hartree (MCTDH) Method: A Highly Efficient Algorithm for Propagating Wavepackets. Phys. Rep. 2000, 324, 1−105. (362) Worth, G.; Meyer, H.-D.; Köppel, H.; Cederbaum, L.; Burghardt, I. Using the MCTDH Wavepacket Propagation Method to Describe Multimode Non-Adiabatic Dynamics. Int. Rev. Phys. Chem. 2008, 27, 569−606. (363) Wang, H.; Thoss, M. Multilayer Formulation of the Multiconfiguration Time-Dependent Hartree Theory. J. Chem. Phys. 2003, 119, 1289−1299. (364) Manthe, U. A Multilayer Multiconfigurational Time-Dependent Hartree Approach for Quantum Dynamics on General Potential Energy Surfaces. J. Chem. Phys. 2008, 128, 164116. (365) Vendrell, O.; Meyer, H.-D. Multilayer Multiconfiguration Time-Dependent Hartree Method: Implementation and Applications to a Henon−Heiles Hamiltonian and to Pyrazine. J. Chem. Phys. 2011, 134, 044135. (366) Tamura, H.; Martinazzo, R.; Ruckenbauer, M.; Burghardt, I. Quantum Dynamics of Ultrafast Charge Transfer at an Oligothiophene-Fullerene Heterojunction. J. Chem. Phys. 2012, 137, 22A540. (367) Binder, R.; Wahl, J.; Römer, S.; Burghardt, I. Coherent Exciton Transport Driven by Torsional Dynamics: A Quantum Dynamical Study of Phenylene-Vinylene Type Conjugated Systems. Faraday Discuss. 2013, 163, 205−222. (368) Tamura, H.; Burghardt, I. Potential Barrier and Excess Energy for Electron-Hole Separation from the Charge-Transfer Exciton at Donor−Acceptor Heterojunctions of Organic Solar Cells. J. Phys. Chem. C 2013, 117, 15020−15025. (369) Zheng, J.; Xie, Y.; Jiang, S.; Lan, Z. Ultrafast Nonadiabatic Dynamics of Singlet Fission: Quantum Dynamics with the Multilayer Multiconfigurational Time-Dependent Hartree (ML-MCTDH) Method. J. Phys. Chem. C 2016, 120, 1375−1389. (370) Tan, D.; Chen, Z. On a General Formula of Fourth Order Runge-Kutta Method. J. Math. Sci. Math. Educ. 2012, 7, 1−10. (371) Mori-Sánchez, P.; Cohen, A. J.; Yang, W. Localization and Delocalization Errors in Density Functional Theory and Implications for Band-Gap Prediction. Phys. Rev. Lett. 2008, 100, 146401. (372) Kubo, R. Statistical-Mechanical Theory of Irreversible Processes. I. General Theory and Simple Applications to Magnetic and Conduction Problems. J. Phys. Soc. Jpn. 1957, 12, 570−586. (373) Gunnarsson, O.; Han, J. The Mean Free Path for Electron Conduction in Metallic Fullerenes. Nature 2000, 405, 1027−1030. (374) Wang, Y.; MacKernan, D.; Cubero, D.; Coker, D. F.; Quirke, N. Single Electron States in Polyethylene. J. Chem. Phys. 2014, 140, 154902. (375) Greenwood, D. A. The Boltzmann Equation in the Theory of Electrical Conduction in Metals. Proc. Phys. Soc., London 1958, 71, 585−596. (376) Dura, J.; Triozon, F.; Barraud, S.; Munteanu, D.; Martinie, S.; Autran, J. L. Kubo-Greenwood Approach for the Calculation of 10356

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357

Chemical Reviews

Review

Mobility in Gate-All-Around Nanowire Metal-Oxide-Semiconductor Field-Effect Transistors including Screened Remote Coulomb ScatteringComparison with Experiment. J. Appl. Phys. 2012, 111, 103710. (377) Ren, J.; Vukmirović, N.; Wang, L.-W. Nonadiabatic Molecular Dynamics Simulation for Carrier Transport in a Pentathiophene Butyric Acid Monolayer. Phys. Rev. B: Condens. Matter Mater. Phys. 2013, 87, 205117. (378) Wang, L.; Akimov, A. V.; Chen, L.; Prezhdo, O. V. Quantized Hamiltonian Dynamics Captures the Low-Temperature Regime of Charge Transport in Molecular Crystals. J. Chem. Phys. 2013, 139, 174109. (379) Zhang, W.; Zhong, X.; Zhao, Y. Electron Mobilities of N-Type Organic Semiconductors from Time-Dependent Wavepacket Diffusion Method: Pentacenequinone Derivatives. J. Phys. Chem. A 2012, 116, 11075−11082. (380) Wilcox, D. E.; Lee, M. H.; Sykes, M. E.; Niedringhaus, A.; Geva, E.; Dunietz, B. D.; Shtein, M.; Ogilvie, J. P. Ultrafast ChargeTransfer Dynamics at the Boron Subphthalocyanine Chloride/C60 Heterojunction: Comparison between Experiment and Theory. J. Phys. Chem. Lett. 2015, 6, 569−575. (381) Johansson, A. A.; Stafström, S. Nonadiabatic Simulations of Polaron Dynamics. Phys. Rev. B: Condens. Matter Mater. Phys. 2004, 69, 235205. (382) Johansson, Å.; Stafström, S. Polaron Dynamics in a System of Coupled Conjugated Polymer Chains. Phys. Rev. Lett. 2001, 86, 3602. (383) An, Z.; Wu, C.; Sun, X. Dynamics of Photogenerated Polarons in Conjugated Polymers. Phys. Rev. Lett. 2004, 93, 216407. (384) Bauer, T.; Jäger, C. M.; Jordan, M. J. T.; Clark, T. A MultiAgent Quantum Monte Carlo Model for Charge Transport: Application to Organic Field-Effect Transistors. J. Chem. Phys. 2015, 143, 044114.

10357

DOI: 10.1021/acs.chemrev.7b00086 Chem. Rev. 2017, 117, 10319−10357